# Download Modelling of the Floating Zone Growth of Silicon Single Crystals with

Document related concepts

Phase transition wikipedia, lookup

State of matter wikipedia, lookup

Partial differential equation wikipedia, lookup

Thermal conduction wikipedia, lookup

Superconductivity wikipedia, lookup

Coandă effect wikipedia, lookup

Turbulence wikipedia, lookup

Equation of state wikipedia, lookup

Time in physics wikipedia, lookup

Derivation of the Navier–Stokes equations wikipedia, lookup

Navier–Stokes equations wikipedia, lookup

Transcript
```University of Latvia
Faculty of Physics and Mathematics
Department of Physics
Modelling of the Floating Zone Growth
of Silicon Single Crystals with Diameter
up to 8 Inch
Ph.D. Thesis
by
Gundars Ratnieks
Prof. Dr.-Phys. A. Muižnieks
2007
i
Anotācija
Šajā darbā tiek piedāvāta noslēgta aksiālsimetrisku matemātisku modeļu sistēma stacionārai peldošās zonas (FZ) kristāla augšanai, kas piemērota peldošo zonu aprēķinam
liela diametra (piem., 8 collu) kristāliem. Fāzu robežu aprēķinu sērija 8 collu peldošajai
zonai vispirms tiek veikta, neievērojot kausējuma plūsmu tajā, tad 8, 4 un 2 collu peldošajām zonām aprēķini tiek veikti, ņemot vērā arı̄ kausējuma plūsmu. Tiek noskaidrots,
ka aprēķini, kuros nav ņemta vērā kausējuma kustı̄ba, dod tikai fāzu robežu pirmo
tuvinājumu, kurpretim konvektı̄vās siltuma pārneses ievērošana noved pie ļoti labas
aprēķinu rezultātu atbilstı̄bas eksperimentāliem datiem. Tiek analizēta arı̄ kausējuma
plūsmas tiešā ietekme uz kausējuma brı̄vās virsmas formu. Darba otra daļa veltı̄ta
induktora novirzes no aksiālās simetrijas ietekmei uz kausējuma 3D kustı̄bu peldošajā
zonā un uz ı̄patnējās pretestı̄bas sadalı̄jumu izaudzētajā kristālā. Rotācijas joslu (angļu
val.: rotational striations) parādı̄šanās FZ kristālos tiek pētı̄ta skaitliski, un aprēķini
tiek salı̄dzināti ar eksperimenta rezultātiem.
ii
Abstract
A closed system of axisymmetric mathematical models for steady-state FZ crystal
growth is proposed as applicable for calculation of floating zones with large crystal
diameters, e.g., 8 inch. Parametric studies of the phase boundaries for an 8 inch
floating zone are performed first by neglecting the melt flow, then calculations for 8-,
4- and 2 inch floating zones are performed with account for the melt flow as well. It is
found that the calculations neglecting the melt motion yield only a first approximation
of the phase boundaries, whereas accounting for the convective heat transfer brings a
very good agreement with experiments. The direct influence of the melt flow on the
free melt surface shape is analysed as well. Another part of the work is devoted to the
effect of the three-dimensionality of the inductor on the 3D melt flow in the floating
zone and on the resistivity distribution in the grown crystal. The phenomenon of
rotational striations in FZ crystals is examined numerically and the calculation results
are compared to experiment.
iii
Acknowledgements
The present work has been carried out partly at the University of Latvia, partly while
working as research associate at the Institute for Electrothermal Processes, University
of Hanover, and finished during my work at Siltronic AG, Burghausen.
First I would like to thank Prof. A. Muižnieks, my thesis advisor, and Prof. B. Nacke,
director of the Institute for Electrothermal Processes, for making my work on the
interesting topic about modelling floating zone possible. I am also greatly indebted to
Prof. A. Mühlbauer, the former director of the Institute for Electrothermal Processes
(then Institute for Electroheat), who, unfortunately, left us too early.
I would like to thank Prof. A. Muižnieks also for his support, advice and the many
I owe much to my colleagues at the University of Latvia, especially A. Rudevičs, for
his valuable help in objected-oriented programming during the elaboration of the code
FZONE, and K. Dadzis, for his patience with some very time-consuming computations.
My thanks go also to Prof. L. Buligins for his kind support with respect to the CFD
package FLUENT.
Thesis on modelling of the industrial floating zone growth would not have been possible
without the permanent interest in FZ research by the present and former co-workers
at Siltronic AG. Especially I would like to thank Dr. W. v. Ammon, L. Altmannshofer,
Dr. J. Virbulis, Dr. M. Grundner, Dr. R. Knobel, K. Niederer and Dr. Th. Wetzel.
For supplying photo-scanning measurements, I am greatly indebted to Dr. A. Lüdge
and Dr. H. Riemann from the Institute for Crystal Growth (IKZ), Berlin.
Last but not least, I would like to express my gratitude to my mother Ligita and sister
Inese for their kind support and understanding during the times I worked on my thesis
in Rı̄ga.
iv
CONTENTS
v
Contents
1 Introduction
1
2 Historical and literature survey
7
2.1
Short history of the floating zone method . . . . . . . . . . . . . . . . .
7
2.2
Modelling of floating zone growth . . . . . . . . . . . . . . . . . . . . .
9
2.3
Objectives and publications of the present work . . . . . . . . . . . . .
13
3 Physical features of FZ-Si process
15
3.1
Properties of silicon . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
15
3.2
High-frequency EM field . . . . . . . . . . . . . . . . . . . . . . . . . .
17
3.3
Joulean power and EM force in HF approximation . . . . . . . . . . . .
19
3.4
Melt flow in the floating zone . . . . . . . . . . . . . . . . . . . . . . .
21
3.5
Free surface of the floating zone . . . . . . . . . . . . . . . . . . . . . .
24
3.6
Flow influence on the free surface shape
28
. . . . . . . . . . . . . . . . .
4 Axisymmetric model of phase boundaries
31
4.1
Phase interfaces . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
31
4.2
Axisymmetric model of high-frequency EM field . . . . . . . . . . . . .
33
4.3
Open melting front: the “fluid film model” . . . . . . . . . . . . . . . .
40
4.4
Shape of the free melt surface . . . . . . . . . . . . . . . . . . . . . . .
44
4.5
ITP and related numerical aspects . . . . . . . . . . . . . . . . . . . . .
46
4.6
Axisymmetric melt flow . . . . . . . . . . . . . . . . . . . . . . . . . .
58
vi
CONTENTS
4.7
. . . . . . . . . . . . . . . . . .
74
4.8
Coupling of all models in FZONE . . . . . . . . . . . . . . . . . . . . . .
83
5 Calculation of phase boundaries
88
5.1
Calculation example . . . . . . . . . . . . . . . . . . . . . . . . . . . .
88
5.2
Numerical study without melt flow . . . . . . . . . . . . . . . . . . . .
93
5.3
Influence of melt flow and its verification . . . . . . . . . . . . . . . . . 107
6 3D Melt flow and rotational striations
119
6.1
Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 119
6.2
Included paper 1: Effect of EM and Marangoni forces . . . . . . . . . . 120
6.3
Included paper 2: Steady-state 3D flow . . . . . . . . . . . . . . . . . . 137
6.4
Included paper 3: Unsteadiness and parametric study . . . . . . . . . . 154
7 Summary and conclusions
164
Bibliography
169
1
1
Introduction
Hyper-pure single-crystalline silicon wafers are the usual substrate to the semiconductor devices and integrated circuit (IC) chips for the state-of-the-art micro-electronics
industry. Single crystal silicon is used instead of poly-crystalline silicon since the former does not have defects associated with grain boundaries found in polysilicon and
limiting the lifetimes of minority carriers. The silicon substrates must also have a
high degree of chemical purity and a high degree of crystalline perfection. The silicon
wafers presenting thin discs of small thickness (e.g. 0.70 to 0.75 mm) and relatively
large diameter (e.g. 76 to 300 mm) are obtained by slicing single crystal ingots, which
are grown carefully from molten polysilicon. The silicon wafer market is nowadays
the largest materials market in the semiconductor materials industry and obeys the
extreme dynamics of the semiconductor branch. An illustration can be seen on the
basis of data published by Gartner, Inc. Due to a major slump of semiconductor chip
demand, the worldwide silicon wafer market revenue in year 2001 totaled \$ 5.4 billion
in U.S. dollars, a 31% decline from 2000 revenue of \$ 7.8 billion. The industry returned
to positive growth in 2002. Wafer demand on surface area basis surged 19% in 2002 to
ca. 4,700 millions of square inches (ca. 30 billions of square centimeters) and produced
a total revenue of \$ 5.7 billion, an increase of ca. 5% from 2001. The wafer market
continued to grow with uneven growth rates in the next years, topping the revenue
of the year 2000 first in 2004 and reaching \$ 10.2 billion market volume in 2006, a
24% growth in revenues and 21% rise in area-based demand over 2005, according to
Gartner. In view of this market dynamics, a hard competition takes place and an
extreme flexibility of the participants is essential. The first and most critical step in
the manufacturing of silicon wafers is the growth of single crystal silicon ingots. The
high expenses of the single-crystalline silicon wafer production and the competition
among several main players in the branch have been a strong push for an intensive
research and development in the field of crystal growth over the last decade.
The single crystal silicon ingots are grown either by Czochralski or floating zone process. Czochralski (CZ) crystal growth, the idea of which was first invented by Czochral-
2
CHAPTER 1. INTRODUCTION
ski already in 1917, involves the crystal pulling from the melt sustained in a crucible
and heated by the infrared radiation of a resistance heater. Since the silica crucibles
used for silicon growth add oxygen to the melt, CZ technique only permits growth
of silicon crystals having relatively low resistivity, which is alright for application in
substrates of IC chips. The floating zone (FZ) crystal growth technique, the basic idea
of which was patented by Theuerer  in 1952, is in contrast crucible-free and more
complicated than CZ technique. The principle of FZ growth is shown schematically
in Fig. 1.1. The polysilicon feed rod is pushed continuously from above and melted
by a high-frequency induction coil. The molten silicon makes a liquid bridge between
the feed rod and the single crystal, which is pulled downwards as it grows. The melt
mass on top of the growing crystal is stabilized by the surface tension of the liquid.
The crystal and feed rods are rotated to ensure a better thermal symmetry and melt
mixing. A sketch of a modern FZ puller after  is shown in Fig. 1.2.
Feed rod
Inductor
Melt
Single crystal
a
b
Figure 1.1: Schematic picture of the bottom-seeded floating zone process for small
crystal diameters (a) and for large crystal diameters (b). The first one is the classical
FZ process, the last one is the so-called needle-eye process. In the classical process,
Featuring low oxygen content in a crystal, FZ method is suitable for obtaining single crystals with high resistivity that is not available by CZ method. Furthermore,
by intentional introduction of electrically active elements (dopants) during the growth
process, the resistivity of FZ silicon can be varied in a very wide range from few mΩ·cm
to several thousand Ω·cm to cover the most different industry needs. The common
substitutional dopants are boron as p-type dopant and phosphorus as n-type dopant.
3
Figure 1.2: Schematic sketch of a modern FZ-Si puller for the growth of large crystals
(after ).
The introduction of the dopants is usually carried out by gas doping1 through nozzles
built in the coil which direct the gas jet onto the melt surface. The dopants are hence
transported with the fluid through the liquid zone toward the crystallization interface, and consequently the resistivity homogeneity in the crystal is much dependent
on the melt flow pattern. An important issue for the crystal growers is to obtain the
resistivity distribution as homogeneous as possible both in the radial and axial direction of silicon ingot to meet the increasing quality requirements of the semiconductor
device industry. As an alternative to the doping during the growth process, for a
better resistivity homogeneity, the grown silicon ingot can be doped later through the
neutron transmutation doping process in which silicon isotopes
phosphorous
1
31
30
Si are converted in
P leading to an n-type material. Nevertheless, since the neutron trans-
As a doping gas, B2 H6 is used for doping with boron and PH3 , for doping with phosphorus.
4
CHAPTER 1. INTRODUCTION
mutation doping technique is rather expensive and there is no suitable reaction for a
p-type dopant available, the early dopant incorporation during the growth process is
the usual approach.
FZ wafers are used primarily for applications in which very high resistivity or superior
purity (particularly the absence of oxygen) are necessary for good device performance.
Such applications include discrete power, MOS power, high efficiency solar cells and
RF/wireless communication chips. FZ wafers make approximately 5% of the total
silicon wafer market, the other 95% are CZ wafers . Provided that there is success
in producing FZ silicon significantly cheeper, the FZ share has a strong potential to
grow, e.g., due to the solar application segment .
Beside the crystal purity and resistivity homogeneity, the crystalline quality is of utmost importance for the device industry. So crystals with dislocations do not satisfy
the modern technological needs. Fortunately by the seed necking technique invented
by Dash [4, 5, 6], it is possible to grow fully dislocation-free crystals, which are now
standard in the silicon semiconductor industry. The Dash technique, however, only
ensures that the crystal is free of dislocations at the initial stage of the growth process. The appearance of dislocations during the whole process must be avoided by the
crystal grower self. It is believed (see e.g. ) that a certain kind of disturbance at the
growth interface is enough to release the dislocation production by the high thermal
stress in the crystal. The disturbance can be a strong local change of temperature and
crystallization rate or small external particle reaching the growth interface. In many
cases the degree of probability of occurrence of such perturbations can be substantially
influenced by altering the puller configuration or growth parameters.
The crystalline quality of the single crystals is determined also by the intrinsic point
defects, i.e., vacancies and Si interstitial atoms, which are incorporated during the
growth process. While single point defects are normally not critical to the semiconductor device performance, their aggregation to large clusters during the cool-down
phase of the crystal can lead to significant deterioration of the material. So the socalled A-swirls or L-pit defects are related to self-interstitial aggregates and result in
damage to devices owing to their large size of several µm. The voids or vacancy aggregates, named also crystal originated particles (COP), have a smaller size of ca. 150 nm
but make also effect on device functionality. It is well established that the pull rate
V and the local axial temperature gradient G at the growth interface of the growing
crystal have a dominant influence on the defect types that develop in the crystal and
5
their spatial as well as their density/size distribution. If V /G exceeds a critical value,
vacancy aggregates develop, and if V /G is less than the critical value, self-interstitial
related defects are built (it was noticed first by Voronkov in 1982 ). The change
of the local value of V /G(r) along the crystal radius determine the concentric defect
regions in the grown crystal. A region free of significant defect agglomerates is found
where V /G is close to the critical value. The radial extension of the defect-free ring is,
however, determined by how homogeneous the radial distribution of V /G is. An appropriate control of the pull rate and the thermal field in the crystal helps to increase
the area of the defect-free region and even to extend the region along the whole crystal
radius. The latter is a necessary condition to be met for the growth of the so-called
perfect or ultimate silicon, which is produced by the Czochralski method. With regard
to the FZ crystals, the aggregation of single point defects is fortunately suppressed by
the nitrogen, which is introduced in the atmosphere to avoid the arcing between the
electrodes of the inductor. Hence the FZ crystals grown in presence of nitrogen are
free of COP’s and L-pits but contain nitrogen atoms, which are usually of no relevance
for device production.
Another important issue is the size of the wafers. The semiconductor industry is
currently experiencing a changeover from 150 mm to 200 mm diameter for FZ crystals
and from 200 mm to 300 mm diameter for CZ crystals. Many semiconductor devices,
or chips, are made from the same wafer, and all chips from a particular wafer are
manufactured and processed simultaneously at each stage in the device manufacturing
process. Because of this, larger-sized wafers allow for a greater throughput from the
same semiconductor manufacturing process and allow semiconductor manufacturers
to spread their fixed costs of production over a larger volume of finished products.
Meanwhile the growing demand for larger and larger chips for the integration of higherdensity semiconductor circuits tends to reduce the number of chips that can be made
from one wafer. Hence the large-diameter crystal growth gets increasingly important.
Whereas the 8 inch (200 mm) FZ wafer has appeared not so long ago as a new market
product, the 6 inch (150 mm), 5 inch (125 mm) and 4 inch (100 mm) FZ wafers keep
significant industrial importance. FZ crystals of that large diameters are grown by
the so-called needle-eye technique [9, 10], which differs from the classical FZ technique
used for the growth of thin crystals up to ca. 15 mm in diameter. The problem with
the classical inductor (see Fig. 1.1a) is the inability to maintain the liquid bridge
between the polysilicon feed rod and the growing crystal if the diameter gets large.
The needle-eye inductor (see Fig. 1.1b) is therefore a pancake-shaped one-turn coil
6
CHAPTER 1. INTRODUCTION
with a central hole (the needle eye) smaller than the feed rod and crystal, in order to
allow the melting of the feed rod in its full thickness.
With regard to the diameter increase, the FZ technology meets several challenges due
to the high complexity of FZ process. One of them is that the induction coil must
be designed to melt off uniformly the polysilicon rod and, simultaneously, supply the
right distribution of heat to the melt in a way that ensures a round shaped and dislocation free growth of the crystal despite the thermal stresses augmented with its size.
Meanwhile the radial resistivity distribution must stay homogeneous enough, which
fortunately is a minor problem for 8 inch crystal growth in contrast to 4 inch case,
due to a better melt mixing in a larger melt volume. To mention the other difficulties
of the FZ technology at large crystal diameter, the necessary voltage between the two
electrodes of the inductor reaches a level where arcing can hardly be avoided. Furthermore, the polysilicon rod must meet certain specifications, e.g., a smooth surface and
the absence of cracks, which are increasingly difficult to achieve with a larger diameter.
Due to the importance of the large-diameter crystal growth and, on the other hand, the
challenges associated with it, the research and development and hence also the numerical modelling of the crystal growth processes gets increasingly relevant. The present
work focuses on the numerical modelling (in frame of the mechanics of continuous
media) of the needle-eye floating zone growth of silicon crystals of large diameter.
The work consists of the following parts. A short historical overview on the evolution of
the floating zone method with references to the relevant patents and other publications
as well as a survey of literature sources considering the modelling of the floating zone
process is given in Chapter 2, at the end of which also the objectives of the present work
can be found. The important physical features of a floating zone process with selected
derivations and equations used in the following parts are provided in Chapter 3. The
main part of the work is described in Chapters 4 and 5, which deal with axisymmetric
modelling of phase boundaries in FZ process. This is accomplished by analysis of
some three-dimensional effects in Chapter 6. Summary and conclusions are provided
in Chapter 7.
7
2
Historical and literature survey
2.1
Short history of the floating zone method
With the beginning of the transistor technology era in 1947/1948, there emerged a need
for semiconductor materials such as germanium or silicon with impurity concentration
as small as 1014 cm−3 or even less, which seemed unrealistic in those years. The first
solution was proposed in 1952 by US-American engineer William G. Pfann working at
Bell Laboratories and inventing the zone refining process for purifying germanium .
The multiple-pass purification process took advantage of the concentration change
by segregation for most impurities during the liquid–solid transition: the melt will
sustain a higher level of impurity concentration than the crystal itself. Pfann was
apparently unaware that a single pass purification technique had been proposed in a
paper published in 1928 by Russian physicist Peter Kapitza working for Rutherford
at Manchester University. The Pfann process involved localized melting by induction,
or other, heating the germanium ingot supported in a graphite boat inside a tube. By
moving the heater along the tube the molten zone passes down the ingot melting the
impure solid at its forward edge and leaving a wake of purer material solidified behind
it. In this way the impurities concentrate in the melt, and with each pass are moved
to one end of the ingot. After multiple passes the impure end of the ingot is cut off.
Unfortunately, while Pfann’s method worked well for refining germanium with a melting point of 937◦ C, it did not work for silicon whose melting point is 1414◦ C because
no suitable boat material could be found to withstand the high temperatures without
contaminating the melt. The problem was solved in 1953 by Bell Laboratories metallurgist Henry C. Theuerer with the development of the floating zone method . He
was able to create a molten zone in silicon by holding the ingot in a vertical position
and moving it relative to the heating element. In this vertical configuration the surface
tension of the molten silicon was sufficient to keep it from coming apart.
P. H. Keck and M. J. E. Golay (Bell Laboratories, ) grew the first silicon crystal
with this new method, still without rotating the crystal. R. Emeis  independently
8
CHAPTER 2. HISTORICAL AND LITERATURE SURVEY
invented and initiated the development of the floating-zone process at Siemens, Germany. He rotated the growing crystal, thus producing straight cylindrical crystals
with diameters up to 10 mm. The high-frequency induction heating instead of the
radiation heating of the floating zone was introduced by S. Müller  and P. H. Keck
with coworkers . By the end of 1954, the basic techniques for the floating-zone
growth of industrial high purity silicon had been established. Further development
(see the historical survey and description of technical aspects in ) was directed
mainly toward automation of the process control, improving the crystalline perfection
(reducing dislocations) as well as increasing the diameter of the grown crystals.
Figure 2.1: The worldwide first dislocation-free 200 mm FZ silicon crystal (courtesy
of Siltronic AG).
In 1956, Wolfgang Keller (Siemens) introduced a slim seed to reduce the dislocation
density. The first fully dislocation-free crystals, both float-zone and Czochralski, were
however grown by William C. Dash from General Electric, USA, during the late fifties.
Dash used a special seeding technique with an extremely thin tapered seed, tip etched
down to 0.25 mm [4, 5, 6]. In 1960, G. Ziegler (Siemens) simplified the seeding by
transforming the Dash’s method to the so-called bottle-neck technique. Ziegler used
an untapered thin seed and made a bottle-neck at the fusion point of seed crystal and
supply rod by means of rapid pulling . This method established in the industrial
scale growth of dislocation-free float-zoned (FZ) silicon crystals.
2.2. MODELLING OF FLOATING ZONE GROWTH
9
Until the end of the 1950s the crystal diameter size did not exceed 20 mm, whereas
during the 60s and beginning of 70s a dramatic increase to 50 mm and 75 mm was
achieved. One of the most important improvements that enabled the growth of large
diameter dislocation-free silicon crystals was the bottom-seeded needle-eye floatingzone technique (invented first by Keller , then also by US-American researchers
) with application of a flat one-turn pancake coil having the inner hole diameter
smaller than the diameter of both, the crystallizing single crystal and the feed rod. In
the last decades a further increase of crystal diameter has taken place: the 100 mm
crystal appears at the end of the 1970s, the 125 mm one in 1986, and the 150 mm one
at the end of the 1980s. The worldwide first dislocation-free 200 mm silicon crystal
was grown at Wacker Siltronic in September 2000 (Fig. 2.1).
Although the silicon crystals of large diameters are always grown by the needle-eye
FZ process and modelling of that is in the focus of the current work, the modelling of
the classical FZ process will be touched in the following literature survey as well, due
to the similarity of both processes and the common issues in modelling them. The
survey is, however, limited according to the content of the work to the macroscopic
(continuous media) theoretical investigations of FZ growth.
2.2
Modelling of floating zone growth
Separate theoretical aspects of the floating zone growth were considered already in
the 1950s. So Heywang  analysed the stability of the free melt surface during
FZ growth. Neglecting the electromagnetic forces, the so-called Heywang limit for
the zone height in case of equal diameters of the grown crystal and feed rod was
q
found approximately at 2.84 ργl g where ρl stands for the density of liquid silicon, γ
is the surface tension coefficient, and g, the gravity. Later, in the 1970s, more precise
q
numerical calculations by Coriell and Cordes  corrected this result to 2.67 ργl g ,
which corresponds to ca. 15 mm for silicon. Heywang had also found an estimation to
the maximum zone length if the crystal and feed rod diameters are strongly different.
q
√ q
His result, (2 + 2) ργl g ≈ 3.41 ργl g , which corresponds to ca. 19–20 mm1 , shows
agreement with the maximum zone limit that can be found also numerically in the
asymptotic case when both diameters are large keeping strong difference between them.
1
It depends on the chosen surface tension of silicon, whose experimentally measured values are
distributed in a wide range, see the references mentioned below Table 3.1.
10
CHAPTER 2. HISTORICAL AND LITERATURE SURVEY
With realistic crystal and melting interface diameters, as applicable for the calculation
of typical needle-eye processes, the Heywang limit is, however, a bit too high because
the diameter of the melting interface is not large enough for the asymptotic estimation
to work well.
In the late eighties, Riahi and Walker  studied the shape stability of a small floating
zone under the influence of electromagnetic pressure in case of the classical shape
inductor and Lie et al.  extended the study to a needle-eye inductor.
Till the mid-1990s, numerous two-dimensional (i.e. axisymmetric) computational studies including heat conduction with Stefan problem and fluid flow had been made to
investigate the classical optically heated floating zone process (in a mirror furnace) for
oxide crystals of small diameters [22, 23, 24, 25, 26, 27, 28, 29]. So in  Lan and Kou
(Taiwan) considered melt convection and calculated the convex interfaces induced by
the Marangoni flow. In  they considered also the effect of rotation and compared
with experimental observations. Further in , Lan considered the effects of magnetic
fields on dopant transport and investigated multiple steady states.
In the second half of the 1990s, Lan et al. [30, 31] extended their model to three
dimensions, first without melt convection. The 3D heat transfer in a double-ellipsoid
mirror furnace was considered. Later also the 3D melt flow and particularly its stability
was analysed by several authors [32, 33].
In the beginning years of the century, the models developed by Lan et al. for the classical optically heated FZ process included already the whole coupling of the 3D shape
of phase interfaces with the 3D time-dependent Marangoni-driven melt convection
[34, 35].
Also the group of Benz (Germany) had worked intensively on the modelling of the
classical FZ process. So in  Kaiser and Benz use the commercial program package
FIDAP to study numerically the melt flow, temperature- and dopant distribution with
a fixed geometry of the liquid zone and under the influence of different magnetic fields.
The heat sources due to the optical heater were approximated by a parabolic function.
It was shown that the Marangoni convection is in general three-dimensional but can
be reduced to axisymmetric under an axial magnetic field. A more general study of
the influence of different magnetic fields in the classical FZ process has been performed
in the Ph.D. thesis of Kaiser . Rotating magnetic fields have been considered later
by Dold et al. in  showing their symmetrizing influence on the 3D flow structure.
2.2. MODELLING OF FLOATING ZONE GROWTH
11
Beside the numerous studies on the magnetic fields as means of altering the fluid flow
in the floating zone, also e.g. the influence of axial vibrations has been investigated
numerically by Lyubimova et al. (Russia), see  and references therein.
As seen above, the numerical studies of the classical FZ process usually consider an
optical heater. The classical FZ process for a crystal of diameter 10 mm with a
radio-frequency inductor has been investigated by Munakata and Tanasawa (Japan)
at the end of the nineties. In  they use a two-dimensional model to calculate the
time-dependent melt flow numerically and compare it with experimental results. The
influence of an axial magnetic field on the flow is considered and a reduction of the
flow oscillations is detected.
For the modelling of the classical FZ growth of small-diameter crystals several simplifications are typically possible: the zone shape can be assumed cylindrical or quasicylindrical, which makes it easy to use structured finite volume grids, and the heat
sources or the heat flux on the free surface may be approximated by a predefined coordinate function. These simplifications are normally not applicable in case of the more
complex needle-eye process calculations because of the specific shape of the molten
zone, the forming of the open melting front above the inductor, and the strong dependence of the induced heat sources on the shape of the high-frequency inductor and
phase boundaries. The first numerical calculations for the needle-eye configuration
were though made in a simplified way by Mühlbauer et al. (Germany)  already in
the 1980s. They calculated the induced current distribution at the free melt surface
and the electromagnetically driven fluid flow in the floating zone with a presumed free
surface shape.
In the 1990s, Lie et al.  calculated the melt motion in the floating zone under
strong axial magnetic field. The influence of the inductor slit on the distribution of
the electromagnetic (EM) field has been analysed by Mühlbauer et al. [43, 44] by
means of 3D (i.e. three-dimensional) calculations of the EM field.
In the following publication by the international team of Mühlbauer in 1995  and
in the Ph.D. thesis of Virbulis (Latvia)  an axisymmetric model was presented for
calculation of the phase boundaries and global heat transfer with melt convection in
a needle-eye FZ process for growth of large crystals of diameter e.g. 4 inch (ca. 100
mm). Their model considered most of the physical features possible to consider in a
2D model, even including the large open part of the melting front, which is characteristic to the needle-eye process. Meantime Riemann et al.  performed calculations
12
CHAPTER 2. HISTORICAL AND LITERATURE SURVEY
of the interface shape and heat transfer by a more limited model, without melt convection and open melting front calculation, and analysed the thermal stress inside the
crystal. Later Mühlbauer, Muižnieks and Virbulis [48, 49] completed their model with
axisymmetric calculation of the time-dependent dopant transport in the melt, derived
the resistivity variation in the grown crystal from the time-dependent dopant distribution, and compared the theoretical results with resistivity measurements performed
by Riemann and Lüdge. A good agreement of the calculation model with laboratory
experiment was achieved with regard to the interface shape and the radial resistivity
profile. An overview of the full model is given in . Raming et al. used the above
model to study the influence of different magnetic fields on the resistivity distribution
of FZ-grown crystals  (see also the Ph.D. thesis of Raming ).
Also Japanese researchers have developed axisymmetric calculation models of the
needle-eye FZ process and compared the results to crystal resistivity measurements.
Togawa et al.  calculate the global heat transfer and the liquid zone shape, a timedependent melt flow and the dopant transport, and they obtain the radial resistivity
distribution in the crystal. The work of Togawa et al. is complemented with better
radiation heat transfer models by Guo et al. in . The effect of the vertical magnetic
field on the FZ growth process has been investigated by Kimura et al. [54, 55]. Their
calculations, however, have been performed for a very simplified shape of the molten
zone.
The approximation of the radiation heat transfer is an important issue of the modelling
of the phase boundaries in FZ growth of large crystals. Regarding the references
mentioned above, only Guo et al.  have considered the view factors associated
with surface of the sample including crystal, melt and feed rod, with the inductor and
with the casing. They also study the importance of the consideration of the specular
property of the crystal and melt surfaces instead of treating all of them as diffuse.
Guo et al. conclude that the specular property is important. It can however be seen
in Fig. 8 of  that the corrections made by accounting the specular character of the
free melt surface and crystal are rather small from the practical point of view.
Togawa et al. and Guo et al., as well as Riemann et al. before, do not calculate the shape
of the open melting front and the position of the inner triple point (the melt/feed/gas
trijunction where the wetting of the feed rod by the bulk melt begins) but take it from
experimental observations. Virbulis and Mühlbauer et al. [45, 46] do calculate the open
front, but they meet two problems with it : 1) the calculated position of the open
2.3. OBJECTIVES AND PUBLICATIONS OF THE PRESENT WORK
13
front near the feed rim tends to lie lower than that at the middle radius due to the
insufficiency of the semi-empirical model used (see the empirical constant ξ in );
and 2) the calculation of the position of the inner triple point (ITP) is a bit handwork
because of lack of a reliable automated calculation procedure. Another point is that
the model of the electromagnetic field calculation does not include the influence of the
main inductor slit. They also use the simplest model for the radiation heat transfer,
i.e., the T 4 -radiation to ambience neglecting view factors, which lowers the precision of
results, particularly in case of large crystal growth where the temperature differences
at the radiating surfaces are higher. Hence the models described in [45, 46] loose their
applicability with larger crystal diameters (like 8 inch).
Excepting the works by Mühlbauer et al. [43, 44], where the influence of the inductor
slit on the distribution of the EM field has been analysed by means of 3D calculations
of the EM field, the rest of publications before year 1999 that were considering the
needle-eye FZ process treated the system in frame of a 2D model as axisymmetric.
2.3
Objectives and publications of the present work
Motivated by the industrial needs on the one hand (see Chapter 1) and the abovementioned limitations of the floating zone modelling on the other hand, the objectives
of the present work have been set as follows:
• Development of a fully closed system of mathematical models for axisymmetric
calculations of steady-state phase boundaries for large floating zones up to 8 inch
diameter and implementing the models into a computation code.
• Investigation of the phase boundaries with the developed computation code and
verification of the results by comparison to experimental data.
• Going beyond the axisymmetric model by studying the influence of the inductor’s
three-dimensionality in order to see the 3D structure of the melt flow and the
resulting rotational striations in the grown crystal.
Significant part of this work has already been published. Here a short outline follows.
To overcome the disadvantages with respect to 8 inch crystal growth modelling inherent
in the phase boundary calculation model by Virbulis and Mühlbauer et al. [45, 46] and
14
CHAPTER 2. HISTORICAL AND LITERATURE SURVEY
to proceed with modelling transient processes like cone growth, we developed our own
calculation model as published in [57, 58]. The content of these publications can
be found in a more complete form in Chapters 4 and 5, which contain also recent
unpublished work concerning parametric studies of the phase boundaries for 8 inch
crystal growth and modelling of the melt flow effect on the crystallization interface
shape, as well as the experimental verification of the predicted phase boundaries.
Usually it is enough to consider a steady-state floating zone by assuming that the process parameters like pulling rate and crystal diameter stay approximately unchanged.
For modelling inherently transient stages of the growth process like cone growth, additional enhancement of the above model has been done in collaboration with Rudevičs
et al., see publications [59, 60, 61]. These model developments, however, stay outside
the scope of the present work, which is fully devoted to the steady-state floating zone.
In  we presented for the first time a coupled 3D model for the melt flow-, temperatureand dopant concentration fields in the floating zone under influence of a 3D EM field
created by a pancake-shaped one-turn inductor with a slit and current suppliers. The
calculation results demonstrated the generation of the rotational striations in the crystal, assuming the EM field as the single source of asymmetry. The study was extended
in our further publications [63, 64, 65, 66], three of which are included in Chapter 6,
as well as in the project report for the VW-foundation . The results of the work
are reviewed also in the articles [68, 69].
15
3
Physical features of FZ-Si process
Here we consider the main characteristic features of large floating zone silicon growth
processes: the physical properties of silicon, the distribution of the magnetic field, the
forces acting in the melt, the melt flow and the free surface of the melt. The aim
is to put down the background assumptions and equations that are common for the
two-dimensional and three-dimensional models in Chapters 4 and 6. The more specific
parts of the models are not considered here but postponed instead to the respective
sections where the models are developed.
At the end of this chapter, a more detailed analysis is devoted to the influence of the
fluid motion on the free surface of the melt, since it seems that this aspect has not
been considered in previous works about FZ modelling.
3.1
Properties of silicon
In the temperature region about the melting point of silicon, not all physical properties
of silicon are known precisely enough. Hence some of the properties assumed for the
floating zone modelling and summarized in Table 3.1 are just a choice between different
values in literature. Not shown in the table is the temperature dependence of the
thermal conductivity and emissivity of solid silicon, which is assumed, after [45, 46],
as follows:
λs (T ) = λs (T0 ) · 4.495 − 7.222 · (T /T0 ) + 3.728 · (T /T0 )2 ,

εs (T0 ) · 1.39,
if T /T0 < 0.593,
εs (T ) =
ε (T ) · [1.96 − 0.96 · (T /T )] , if T /T ≥ 0.593,
s 0
0
0
where the designations correspond to those in Table 3.1.
Some of the silicon properties used in the 3D flow calculations in Chapter 6, which
have been performed earlier, have values differing from the ones listed in Table 3.1.
They can be found together with the calculations in Chapter 6.
16
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
Silicon property
Symbol
Value
Melting point
T0
1687 K
Density of liquid
ρl
2580 kg/m3
Density of solid
ρs
2329 kg/m3
Heat capacity
cp
1000 J/(kg·K)
Latent heat of fusion
Q
1.8 · 106 J/kg
Electric conductivity of liquid
σl
1.2 · 106 S/m
Electric conductivity of solid
σs
5.0 · 104 S/m
Thermal conductivity of liquid
λl
67 W/(m·K)
λs (T0 )
22 W/(m·K)
εl
0.27
εs (T0 )
0.46
γ
0.88 N/m
∂γ/∂T
−2.5 · 10−4 N/(m·K)
φ0
11 deg
Thermal expansion coefficient of liquid
β
1.0 · 10−4 K−1
Dynamic viscosity
η
8.6 · 10−4 kg/(m·s)
Thermal conductivity of solid at T0
Emissivity of liquid
Emissivity of solid at T0
Surface tension
Growth angle
Table 3.1: Physical properties of silicon, after [45, 46, 70, 71, 72, 73].
3.2. HIGH-FREQUENCY EM FIELD
3.2
17
High-frequency EM field
Let us consider the alternating harmonic electromagnetic (EM) field created by the
inductor in a typical FZ growth system. The frequency of the field is f ≈ 3 MHz. Since
the typical size of the puller is much smaller than the wavelength of the field (c/f ≈
100 m), the EM field is quasi-stationary and we neglect the displacement currents.
There are no ferromagnetic materials in the FZ growth system under consideration,
i.e., µ = 1.
Due to the high frequency, the EM field penetrates only in a thin skin layer of the
silicon sample and inductor itself, the latter being made of copper or silver. The
penetration depth of the field is calculated by (see e.g. )
δ=√
1
,
πµ0 f σ
(3.1)
where σ is the electrical conductivity of silicon or inductor material. Values of δ for
the materials usually relevant in case of FZ growth are listed in Table 3.2.
material
σ, S/m
Si (solid)
4
5 · 10 
Si (liquid) 1.2 · 106 
5 · 107 — 6 · 107
Cu, Ag
δ, mm
1.3
0.27
0.041— 0.038
Table 3.2: The penetration depth of EM field of frequency 3 MHz in different materials.
Since the penetration depth δ is small in comparison to the characteristic length scales
of the floating zone, the equivalent integrated quantities such as the surface density
of electric current, Joulean heat flux density on silicon surfaces and surface density of
EM force are used instead of the volume current density, volume power density and
volume force density, respectively.
In order to write the relations between these quantities, we introduce local orthogonal
coordinates (ξ1 , ξ2 , ξ3 ) with ξ1 and ξ2 along the surface of the conductor and ξ3 directed
into the material and normal to the surface. Due to the distinct skin-effect, we can
assume that the magnetic field B and the current volume density j in the skin layer
are parallel to the surface, i.e.
B = e1 B1 + e2 B2 ,
j = e 1 j1 + e 2 j2 ,
B3 = 0,
(3.2)
j3 = 0,
(3.3)
18
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
where e1 and e2 are unity vectors in the directions ξ1 and ξ2 , respectively.
The change of the electromagnetic field in the normal direction ξ3 is much steeper as
in the directions ξ1 and ξ2 . Under these circumstances, the solution of the Maxwell’s
equations (see ) and the material relation between the electric field intensity and
volume current density (the Ohm’s law1 ),
j = σE,
(3.4)
j = ja · exp(−ξ3 /δ) · cos(ωt − ξ3 /δ + π/4),
(3.5)
yield
where ja designates the amplitude of j at the surface, and ω = 2πf . The reference
point of time t is chosen in order to reduce the expressions following below.
The surface current density is defined by
Z
i=
∞
j dξ3
(3.6)
0
and with account of (3.5) we have
i = ia · cos(ωt),
(3.7)
where ia , the amplitude of i, is related to ja by
δ
ia = ja · √ .
2
(3.8)
The corresponding effective value of the time-dependent surface current, ief , is defined
as follows (line above variable stands for averaging in time):
i2ef
=
i2
or
ia
√
ief =
.
2
(3.9)
From the current density distribution (3.5) and the Maxwell’s equation for the quasistationary EM field, neglecting the displacement currents,
µ0 j = rotB,
1
(3.10)
At that high frequencies, the second part in the Ohm’s law j = σ(E + u × B), i.e., the cross-
product of fluid velocity and magnetic field, is much smaller than the electric field E that is induced
by the change of B. Indeed, one can show that u · B E will be true if u/L f , where L is the
characteristic length (radius). In our case, f ≈ 3 · 106 Hz, u ≈ 0.1 m/s, L ≈ 0.1 m, and the above
inequality is satisfied.
3.3. JOULEAN POWER AND EM FORCE IN HF APPROXIMATION
19
with account of (3.2), (3.3) and (3.8), we get the distribution of the magnetic field in
the skin layer:
B = Ba · exp(−ξ3 /δ) · cos(ωt − ξ3 /δ),
(3.11)
Ba = µ0 · e3 × ia ,
(3.12)
Bef = µ0 ief · exp(−ξ3 /δ),
(3.13)
where Ba is the amplitude of B at the surface and the effective value Bef is defined
like that of i, cf. (3.9).
Comparing (3.7) and (3.11) we see that there is no phase shift between the surface
current i and the magnetic field near the surface of the conductor, B|ξ3 =0 . Since the
EM field is quasi-stationary (i.e., no wave process has to be taken into account), the
B–field has a constant phase in the whole atmosphere between the inductor and the
silicon body. The above conclusion about the phases of B|ξ3 =0 and i holds for silicon
surface as well as for the surface of the inductor. As a consequence, we have no phase
shift other than 0◦ or 180◦ between the surface currents on inductor and silicon parts2 .
That brings a simplification for the calculation procedures both in 3D and 2D models:
the surface currents may be treated as real vectors and the mathematical formalism
in complex numbers, which is often used in harmonic EM field analysis, becomes
redundant (as stated in ).
The above thesis about no phase shift between the surface currents and magnetic field
is based on the used high-frequency approximation: it works if the skin layer depth is
sufficiently small and the magnetic field has no normal component to the conducting
surface, see (3.2). The applicability of this approximation for the FZ system with field
frequency about 3 MHz has been tested and found appropriate in .
3.3
Joulean power and EM force in HF approximation
In the high-frequency approximation, the induction heating effect can be described by
the Joulean heat flux density at the conducting surface, q EM , called also the surface
power density, which can be expressed via surface current i by using expressions (3.5),
2
If the system is close to axisymmetric, the surface currents on inductor are oriented opposite to
the surface currents on the other parts. That is why one speaks about a phase shift of 180◦ , although
there is no principal difference to the phase shift of 0◦ .
20
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
(3.8) and (3.9):
∞
j2
ief 2
dξ3 =
.
(3.14)
σ
δ·σ
0
This formula is only valid if the thickness of the conducting body is large compared to
q
EM
Z
=
the EM field penetration depth δ, otherwise the high-frequency approximation would
not be applicable.
The melt flow in the floating zone is strongly influenced by the EM force. From the
expression for the force volume density f ,
f = j × B,
(3.15)
and from the Maxwell’s equation (3.10) it follows that
f =−
1
1
2µ0
µ0
(3.16)
In the high-frequency approximation, from the equations (3.2), (3.3) and (3.10) we
also have ∂B2 /∂ξ1 = ∂B1 /∂ξ2 , and consequently
1
1
∂B 2
∂B 2
(B∇)B =
e1
+ e2
2
∂ξ1
∂ξ2
2
With respect to the fluid flow in the melt and the shape of the free melt surface, the
time-averaged value of the force (3.16) is relevant:
2
2
Bef
Bef
.
2µ0
2µ0
(3.17)
It can be seen that the first part of the expression (3.17) is a potential force and we
denote it by fp = − grad pEM . The second part is a tangential force having no normal
component, we denote this part by fτ . Both the expression denoted by pEM and fτ
decay to zero with ξ3 → ∞. It can be shown that the splitting up of the total force in
two parts having the above properties,
f = fp + fτ = − grad pEM + fτ ,
(3.18)
is unique3 , and that the potential part fp has no direct influence on the solution of the
3
Let us assume that f = − grad(p1 + p2 ) + fτ and that there is another way of splitting up,
namely f = − grad p1 + (fτ − grad p2 ), such that the normal component of (fτ − grad p2 ) is zero. The
latter means that ∂p2 /∂ξ3 = 0, i.e., p2 depends only on the tangential coordinates. According to the
condition that the EM pressure in both expressions of f decays to zero deep in the conducting body,
we have (p1 + p2 )|ξ3 →∞ = 0 and p1 |ξ3 →∞ = 0. Consequently p2 |ξ3 →∞ = 0 must be fulfilled for all
tangential coordinates. Recalling the previous constraint on p2 , we have p2 ≡ 0. Hence both ways of
splitting up of f are identical.
3.4. MELT FLOW IN THE FLOATING ZONE
21
Navier-Stokes equations4 and hence is only responsible for the equilibrium shape of
the free surface of the liquid, whereas the tangential part fτ influences solely the fluid
motion. The influence on the shape of the free surface by the fluid motion itself must
not be considered at this point and is postponed to Section 3.5.
The above splitting up of f defines a unique coordinate function pEM that decays to
zero at ξ3 → ∞. We call it the electromagnetic pressure and have the expression
pEM =
Bef2
.
2µ0
We will not consider the values of the electromagnetic pressure inside the skin layer,
hence we keep the designation pEM for the electromagnetic pressure at the free surface
of the liquid. With account of (3.13) we have on the surface ξ3 = 0:
p
EM
µ0 ief 2
=
.
2
(3.19)
For the tangential part fτ we have with account of (3.13):
fτ =
µ0
grad1,2 (ief 2 ) · exp(−2ξ3 /δ).
2
(3.20)
The tangential force volume density fτ is integrated over the skin layer to get the force
surface density, called also the tangential shear stress:
Z ∞
1
EM
fτ dξ3 = µ0 δ · grad1,2 (ief 2 ).
F =
4
0
3.4
(3.21)
Melt flow in the floating zone
In the high-frequency approximation, there are no volume forces except the gravity
acting in the bulk of melt. We consider the silicon melt flow as an incompressible
Newtonian fluid flow described by the Navier-Stokes equation (see e.g. ):
∂u
ρ̃l
+ (u∇)u = −∇p + η∆u + ρ̃l g,
∂t
(3.22)
where u and p are the velocity- and pressure fields, respectively, g is the gravity, η,
the dynamic viscosity, which is assumed constant, and ρ̃l is the melt density (the
4
Writing the modified pressure p0 = p + pEM instead of the fluid pressure p in the Navier-Stokes
equations of an incompressible fluid flow allows to account for the potential force fp = −∇pEM without
changing the velocity field of the fluid.
22
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
subscript l stands for liquid). The assumption of incompressibility means that the
density change due to the changes in pressure may be neglected. The temperature
dependence of the density, however, has to be taken into account at least for the
gravity term, in order to allow for the buoyancy effect. In the other terms of the
equation, the density variation may be neglected (the Boussinesq approximation, see
e.g. ). The temperature dependence of density is expressed using the coefficient of
volume expansion, β = −(1/ρ̃l )(∂ ρ̃l /∂T )p , as follows:
ρ̃l = ρl × [1 − β(T − T0 )],
where T is the temperature and ρl is the density of liquid at the melting point T0 . It
is, of course, assumed that β|T − T0 | 1 overall in the liquid volume.
Consequently, the original equation (3.22) transforms to:
∂u
ρl
+ (u∇)u = −∇p + ρl g + η∆u − ρl β(T − T0 )g.
∂t
Since ρl g is a potential force, it is balanced exactly by a pressure equal to
pHS = ρl gz + const = −ρl gz + const,
(3.23)
i.e., the hydrostatic pressure of fluid in rest and equilibrium (u = 0, T = T0 ). In
the above expression g = |gz | and the constant depends on the reference point of the
coordinate z being measured vertically upwards.
The rest of the absolute pressure p can be named the hydrodynamic pressure,
pHD = p − pHS ,
(3.24)
and is the only part of pressure left in the above Navier-Stokes equation after elimination of the hydrostatic part: −∇p + ρl g = −∇(p − pHS ) = −∇pHD .
The system of equations for the fluid flow in the floating zone consists of the continuity equation, the Navier-Stokes equation transformed as shown before, and the
temperature equation neglecting viscous dissipation :
∇u = 0,
1
∂u
η
+ (u∇)u = − ∇pHD + ∆u − β(T − T0 )g,
∂t
ρl
ρl
λl
∂T
+ (u∇)T =
∆T,
∂t
ρl cp
where λl is the thermal conductivity and cp , the specific heat of the liquid.
(3.25)
(3.26)
(3.27)
3.4. MELT FLOW IN THE FLOATING ZONE
23
Marangoni force
EM force
Buoyancy force
Figure 3.1: Schematic sketch of the action of forces in the floating zone.
As boundary condition for the temperature on the melting and crystallization interfaces, the melting point temperature is used. On the free melt surface, both the
radiation heat transfer and the heat flux corresponding to the electromagnetic power
surface density (3.14) have to be accounted. For considering boundary conditions for
the fluid flow in the molten zone, a cylindrical coordinate system (r, ϕ, z) with the symmetry axis coinciding with the crystal and feed rod rotation axis and the cylindrical
components of the velocity vector u, i.e., ur , uϕ and uz , are practical.
The boundary conditions for the velocity field consider the rotation of the feed rod
and melting process at the melting interface:
ur = 0,
uz = −VS ,
uϕ = 2πr ΩF ,
(3.28)
where VS is the supply velocity of molten silicon from feed rod and ΩF , the rotation
rate of feed rod. It is a simplification to assume that VS is constant over the melting
interface. On the growth interface, the crystallization process and the rotation of the
crystal are considered:
ur = 0,
uz = −VCr ,
uϕ = 2πr ΩCr ,
(3.29)
where VCr is the pull rate of the single crystal and ΩCr , its rotation rate.
Due to the small penetration depth of the EM field in the melt, the free surface of the
melt is considered as a boundary with tangential shear stress, or the so-called surface
force F. For the total value of F, both the electromagnetic force (3.21) and Marangoni
force (see Fig. 3.1) are accounted:
F = FEM +
∂γ
∂T
(3.30)
24
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
where γ is the surface tension of the melt.
The precise flow boundary conditions at the free surface and the equation of the free
surface shape are described later in Section 3.5. Here, let us first consider the dimensionless numbers characterizing the flow in the floating zone. For this purpose
we introduce the characteristic length scale L as a half of crystal radius RCr and the
characteristic azimuthal velocity Uϕ = 2πLΩCr , and take the characteristic meridional
velocity Urz = 0.01 m/s and the characteristic melt temperature difference Θ = 30 K
from numerical calculations of 4 to 8 inch floating zones. We also assume the characteristic values of crystal rotation rate ΩCr being 5 rpm for 4 inch crystals and 2 rpm
for 8 inch crystals.
The ratio of inertial to viscous forces and the stability of the flow is characterized by
the Reynolds number. Since the flow structure could have certain anisotropy due to
the crystal rotation, it is meaningful to consider two Reynolds numbers: the meridional
Reynolds number Rerz = LUrz /ν and the azimuthal Reynolds number Reϕ = LUϕ /ν,
where we use the kinetic viscosity ν = η/ρl . Other important dimensionless numbers
are: the Prandtl number Pr = ν/χ, i.e., the ratio of momentum diffusivity (viscosity)
and thermal diffusivity χ = λl /(ρl cp ); the Grashof number Gr = gβΘL3 /ν 2 , which approximates the ratio of the buoyancy to viscous force acting on the liquid; the Rayleigh
number Ra = Gr · Pr, which characterizes whether conduction or free convection dominates the heat transfer; and the Péclet number Pe = Re · Pr relating the rate of
advection of a flow to its rate of thermal diffusion.
The estimated values of the dimensionless numbers are shown in Table 3.3. The
values of Reynolds number show that the transition to turbulence, which could be
expected occurring in Reynolds number region 2000—3000, is not yet achieved even
with the large 8 inch zone. The Rayleigh number, however, is high, which indicates to
a significant presence of buoyancy.
3.5
Free surface of the floating zone
To obtain the boundary conditions at the free surface we use the equation for the jump
in stress across the interface between gas (g) and liquid (l), see e.g. , with adding
the contributions (3.19) and (3.30) caused by the high-frequency electromagnetic field
3.5. FREE SURFACE OF THE FLOATING ZONE
Characteristic quantity Units
25
FZ 4”
FZ 8”
RCr
m
0.050
0.100
L = RCr /2
m
0.025
0.050
Urz
m/s
0.010
0.010
Θ
K
30
30
ΩCr
1/s
0.083
0.033
Uϕ = 2πLΩCr
m/s
0.013
0.010
ν = η/ρl
m2 /s
3.3 · 10−7
3.3 · 10−7
χ = λl /(ρl cp )
m2 /s
2.6 · 10−5
2.6 · 10−5
Pr = ν/χ
1
0.013
0.013
Rerz = LUrz /ν
1
750
1500
1
980
1500
1
6
4.1 · 10
3.3 · 107
Ra = gβΘL3 /(νχ)
1
5.3 · 104
4.2 · 105
Pe = LUrz /χ
1
9.6
19
Reϕ = LUϕ /ν
3
Gr = gβΘL /ν
2
Table 3.3: The characteristic parameters and estimation of the dimensionless numbers
(rounded to two significant digits) for the melt flow in FZ processes.
26
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
n
ITP
Gas
j
t
Melt
ETP
Figure 3.2: Sketch of the local orthogonal coordinates (τ, ϕ, n) at the free surface of
the floating zone. ITP is the inner triple point and ETP, the exterior triple point.
and Marangoni forces:
X

σıg n −
X
σıl n = γKnı + pEM nı − Fı ,
(3.31)

where the normal vector n points from liquid into gas and K is the curvature of the
interface, being reckoned here as positive when the corresponding center of curvature
lies in the liquid region. Since we do not intend to calculate the flow of gas, the stress
everywhere in the gas may be approximated (see ) by σıg = −pg δı , where pg is a
constant gas pressure. The stress in the incompressible Newtonian liquid, however,
is considered explicitly: σıl = −(pHS + pHD )δı + 2ηeı , where pHS and pHD are the
hydrostatic pressure (3.23) and hydrodynamic pressure (3.24), respectively, and eı is
the rate-of-strain tensor. Consequently, substituting the stresses into (3.31) yields the
following boundary condition for the rate of strain of liquid at the free surface:
2η
X
eı n = p0 − ρl gz − γK − pEM + pHD nı + Fı ,
(3.32)

where p0 is containing constant contributions from pHS and pg and might be named
the gauge pressure.
Let us assume now that the liquid zone has an axisymmetric shape. We obtain the
local orthogonal coordinate system (τ, ϕ, n) in each point of the free surface (τ standing
for the tangential direction and n, for the normal direction locally at the surface, see
Fig. 3.2) by rotation of the local cylindrical coordinates (r, ϕ, z) about the azimuthal
direction ϕ, which plays now the role of the other tangential direction beside τ .
With the local coordinate system introduced, the sum on the left side of equation
(3.32) is interpreted as eın , where ı stands for τ , ϕ or n. The respective expressions of
3.5. FREE SURFACE OF THE FLOATING ZONE
27
the rate-of-strain tensor’s components are:
1 ∂un ∂uτ
+
eτ n =
2 ∂τ
∂n
1 1 ∂un
∂(uϕ /r)
eϕn =
+r
2 r ∂ϕ
∂n
∂un
enn =
∂n
The expressions of eτ n and eϕn can be simplified by taking into account that for a
static free surface
un = 0,
(3.33)
which implies that also the gradient of un along the free surface vanishes. Consequently,
(3.32) yields the following free surface conditions:
Fτ
∂uτ
=
∂n
η
∂uϕ
uϕ ∂r Fϕ
=
+
∂n
r ∂n
η
p0 − ρl gz − γK − pEM + pHD − 2η
(3.34)
(3.35)
∂un
=0
∂n
(3.36)
The conditions (3.33), (3.34) and (3.35) are the flow boundary conditions at the free
surface of the floating zone. The additional equation (3.36) determines the static shape
of the free surface. The last two terms on the left side of (3.36) describe the influence
of fluid flow on the surface shape.
Let us consider the distribution of the hydrodynamic pressure pHD along the free
surface under assumption of an axisymmetric fluid flow. The τ -projection of the
Navier-Stokes equation (3.26) with taking into account the continuity (3.25) yields:
u2ϕ ∂r
∂uτ
∂uτ
∂uτ
1 ∂pHD
η ∂(rω)
+ uτ
+ un
−
=−
+
− gτ β(T − T0 ),
∂t
∂τ
∂n
r ∂τ
ρl ∂τ
ρl r ∂n
where
∂uτ
∂un
−
.
∂n
∂τ
Taking into account un = 0 at the free surface and assuming that the time-dependence
ω ≡ (∇ × u)ϕ =
of the flow is slow enough, the Navier-Stokes equation simplifies and we have the
expression for the gradient of the hydrodynamic pressure along the free surface,
ρl u2ϕ ∂r ρl ∂u2τ
∂pHD
η ∂(rω)
∂r
=
−
+
+ ρl gβ(T − T0 ) ,
∂τ
r ∂τ
2 ∂τ
r ∂n
∂n
28
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
the integration of which yields:
p
HD
Z
τ
(τ ) =
τ0
ρl u2ϕ ∂r
ρl u2τ
dτ −
+
r ∂τ
2
Z
τ
τ0
η ∂(rω)
∂r
+ ρl gβ(T − T0 )
r ∂n
∂n
dτ,
(3.37)
where τ0 is a reference point where uτ = 0, so that pHD (τ0 ) = 0. Let us choose as
reference point the outmost end-point of the free surface: τ0 = τETP .
3.6
Flow influence on the free surface shape
Since it seems that this question has not found place in works on modelling of floating
zone before, let us consider the flow influence on the free surface shape in more detail
and roughly estimate the comparative order of magnitude of the different flow-related
terms in the free surface equation (3.36) with (3.37).
We need for analysis more characteristic quantities than already introduced in Section 3.4. From numerical calculations of 4 to 8 inch floating zones we take the characteristic length scale in the vertical direction, Lz , as a half of the bulk liquid height
HL , and the characteristic electric current surface density at the free surface, Is :
Lz = HL /2 = 0.0085 m,
Is = 8000 A/m.
To avoid underestimation of the ω-term in (3.37), let us assume that the characteristic
flow boundary layer thickness Ln at the free surface is significantly smaller than the
√
length scale L and has the expression: Ln = L/ Rerz .
We use below the following dimensionless numbers beside the ones from Table 3.3:
• Galilei number, Ga = gLz L2 /ν 2 ,
• Laplace number, La = γL2 /(ρl ν 2 Lz ),
• and an electromagnetic number, Em = µ0 Is2 L2 /(ρl ν 2 ).
The equations (3.36) and (3.37) are made dimensionless by dividing them by ρl gLz ,
which is the characteristic value of the hydrostatic pressure pHS . The following list
shows the terms of equations and their respective dimensionless representation (a hat
3.6. FLOW INFLUENCE ON THE FREE SURFACE SHAPE
Equation term
29
FZ 4”
FZ 8”
ρgz-term (3.38)
1
1
γK-term (3.39)
0.5
0.5
pEM -term (3.40)
0.2
0.2
u2ϕ -term (3.41)
2 · 10−3
1 · 10−3
u2τ -term (3.42)
6 · 10−4
6 · 10−4
ω-term (3.43)
1 · 10−3
1 · 10−3
T -term (3.44)
Λ · 9 · 10−3
Λ · 2 · 10−2
6 · 10−6
3 · 10−6
∂un /∂n-term (3.45)
b l gLz ) of the terms in the free
Table 3.4: Estimated dimensionless magnitudes Υ/(Υρ
surface equations (3.36) and (3.37).
over a term denotes that it is dimensionless):
pHS = const − ρl gz
→
pLa = −γK
→
µ0 ief 2
−pEM = −
2
Z τ
2
ρl uϕ ∂r
dτ
Υ1 =
r ∂τ
τETP
ρl u 2
Υ2 = − τ
2
Z τ
η ∂(rω)
Υ3 =
dτ
τETP r ∂n
Z τ
∂r
Υ4 =
ρl gβ(T − T0 ) dτ
∂n
τETP
∂un
∂uτ
uτ ∂r
= 2η
+
Υ0 = −2η
∂n
∂τ
r ∂τ
→
→
→
→
→
→
pHS
ρl gLz
pLa
ρl gLz
−pEM
ρl gLz
Υ1
ρl gLz
Υ2
ρl gLz
Υ3
ρl gLz
Υ4
ρl gLz
Υ0
ρl gLz
=
1
· pbHS
(3.38)
=
−La/Ga
· pbLa
(3.39)
=
− 21 Em/Ga
· pbEM
(3.40)
=
−Re2ϕ /Ga
b1
·Υ
(3.41)
b2
= − 21 Re2rz /Ga · Υ
(3.42)
±Re2rz /Ga
b3
·Υ
(3.43)
b4
= −Λ · Gr/Ga · Υ
(3.44)
b0
= ±4Rerz /Ga · Υ
(3.45)
=
The factor Λ in (3.44) is the characteristic value of ∂r/∂n at the free surface and
emphasizes that the term Υ4 can become negligible independently on how large the
Grashof number is, if the free surface is horizontal.
Finally, the resulting dimensionless magnitudes, i.e., the dimensionless coefficients of
b l gLz ), are calculated for all the different terms in Table 3.4. It can be seen
kind Υ/(Υρ
that, for the considered 4 inch and 8 inch floating zones, the gravitational, capillary
and electromagnetic terms in the free surface equation are some orders of magnitude
30
CHAPTER 3. PHYSICAL FEATURES OF FZ-SI PROCESS
larger than any of the flow-related correction terms. Hence it is justified, in these
cases, to neglect the flow effect on the shape of the free surface or just to take the
largest of the correction terms.
Comparing the flow correction terms, it should be taken into account that the factor
Λ in the temperature term is small because of a rather horizontal free surface if the
diameter of the crystal is large enough. One of the largest of the flow correction terms
is hence the u2ϕ -term (3.41), which represents the effect of the centrifugal forces. An
advantage of this flow-related term is that it is possible to account for it even without
calculating the melt flow explicitly. If approximating the fluid rotation in the floating
zone by a solid-body rotation with the rotation rate of the crystal, then uϕ ≈ 2πr ΩCr
and integration yields:
Z
τ
τETP
ρl u2ϕ ∂r
dτ ≈ 2π 2 ρl Ω2Cr r2 + const,
r ∂τ
(3.46)
2
and can be eliminated from the final surface
where the constant equals −2π 2 ρl Ω2Cr RCr
equation by a corresponding redefinition of the gauge pressure p0 .
31
4
Axisymmetric model of phase
boundaries
In this chapter, the models and methods of calculation of FZ phase boundaries as
implemented in own calculation code FZONE are described.
The FZ growth system is assumed to be axisymmetric except the inductor, which
may have radial slits according to the industrial practice (Fig. 4.1). The influence of
the inductor slits is taken into account in an approximate way and an axisymmetric
electromagnetic field is used instead of the real three-dimensional one for the heat
generation and phase boundary calculation.
The placement and shape of the phase interfaces between solid and melt is solved by
a transient approach (see Section 4.1), meanwhile the free melt surface is treated by a
simplified steady-state method without requesting conservation of the melt volume (see
Section 4.4). Beside that, the mathematical models contain some other steady-state
features. Thus it is altogether a partly transient approach and is usable for obtaining
the final stationary growth situation but not the explicit evolution in time.
4.1
Phase interfaces
Starting from an initial phase interface shape, the move rates of each point of the
melting and crystallization interfaces are calculated by requesting fulfilment of the
local heat balance equation at the respective interface:
∂T ∂T λs
= λl
+ ρs QVn ,
∂n s
∂n l
(4.1)
where the temperature field T in solid and liquid is known after solving the global heat
transfer (see Section 4.8.1), Q denotes the latent heat of fusion, ρ, the density, λ, the
thermal conductivity, the subscripts s and l stand for solid and liquid, respectively,
and Vn is the unknown front’s normal rate of solidification in the reference system of
the solid phase or, equally, the normal projection of the front’s move rate with the
32
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Inductor
Feed
slits
Main slit
Melt
Reflector
Current
suppliers
Crystal
Figure 4.1: FZ growth system and the inductor with radial slits.
positive directions as shown by the vectors n in Fig. 4.2 (hence, for example, Vn < 0
when melting instead of solidification occurs). The solidification rate Vn is related to
the local front’s normal velocity vn in the laboratory reference system (i.e. the reference
system of the inductor and the furnace around) by the relation:
Vn = Vs nz + vn ,
(4.2)
where Vs denotes the move rate of the solid silicon in the laboratory reference system,
which equals to the move rate of feed, VF , or crystal, VCr , when considering the melting
or crystallization interface, respectively. The value of vn characterizes how transient
the process is (e.g. in a steady-state case vn = 0) and can be calculated from the
balance equation (4.1):
λl ∂T λs ∂T −
− Vs nz .
vn =
ρs Q ∂n s ρs Q ∂n l
(4.3)
The formula (4.3) applies to the melting and crystallization interfaces. For the open
melting front, the velocity expression has to account also the Joulean heat flux q EM
λs ∂T q rad − q EM
vn =
+
− VF nz .
ρs Q ∂n F
ρs Q
(4.4)
The calculation of the Joulean heat flux q EM at the open front requires assumptions
about the open front structure. The fluid film model and the expression for q EM are
derived in Section 4.3. The calculation of the radiation heat flux q rad is considered in
Section 4.7.
4.2. AXISYMMETRIC MODEL OF HIGH-FREQUENCY EM FIELD
33
Figure 4.2: Sketch of the model for FZ growth.
For solving the phase boundaries numerically, they are divided into linear elements
and the velocities vn are calculated in the nodes according to the formulas (4.3) and
(4.4). All quantities needed for this procedure, including the temperature gradients,
electric currents and radiation heat fluxes, are interpolated to the nodes and the normal direction n is represented locally by the bisector at the respective node (e.g. see
Fig. 4.6). Chosen a time step ∆t, each node is moved by vn ∆t in the direction n.
4.2
Axisymmetric model of high-frequency EM field
In order to obtain the Joulean heat fluxes on all conducting surfaces and the electromagnetic pressure on the free melt surface, the electromagnetic field in the FZ system
has to be calculated.
Due to the inductor shape used in FZ process, a 3D EM calculation would actually be
necessary in order to take the azimuthal average of the Joulean heat source distribution,
for the axisymmetric phase boundary calculation. Since the EM field recalculation
34
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
is repeated several times in each calculation step, it costs too much computational
resources and must be replaced by effective 2D EM field calculations. It is possible to
include the approximate influence of the inductor slits in the axisymmetric EM field
model. The method and its physical background for induction furnaces with regularly
slitted crucible has been described in . In the present work, the methodology from
 is adapted to the case of FZ system with a slitted inductor. Additionally, an
approximate account of the main slit of the inductor is included.
The boundary lines in the cross-section of the FZ system that are relevant in the electromagnetic part of calculation are shown in Fig. 4.3: the silicon surface (SilSurf ), the
surface of the inductor part that is not slitted if not counting the main slit (IndSurf ),
the surface of the slitted part of the inductor (IndSlit), and the end-line of the slits
in the middle of inductor (IndMidd ). The inner plane of the slit is the shaded region
in Fig. 4.3. We can attach a local Cartesian coordinate system (x, y) to this (and any
other) slit plane. Assuming the axial symmetry is not disturbed much by the slits,
the electric current in the high-frequency approximation is going along the surfaces
SilSurf, IndSurf and IndSlit only in the azimuthal direction. We will designate, in
this section, this azimuthal surface current by J. A part of current is flowing also in
the plane of slit and has there some x- and y-component. The slit current will be
designated here by ‫ג{ = ג‬x , ‫ג‬y }.
4.2.1
Equations for the non-slitted parts
The EM field is solved in terms of the magnetic vector-potential A, defined by rot A =
B. The field is to be found in the space surrounding the conducting bodies by setting
boundary conditions at the surfaces of the conductors. The vector-potential in the nonconducting space is governed by the Poisson equation: ∆A = 0 . Only the azimuthal
component of A differs from zero in axisymmetric model, A ≡ Aϕ . Therefore
A(r, z)
1 ∂
∂A
A ∂2A
∆A(r, z) −
=
0
or
r
−
+
= 0.
r2
r ∂r
∂r
r2
∂z 2
(4.5)
It follows directly from the definition of the magnetic vector-potential that the field
lines of B are as well the isolines of (r · A), in the axisymmetric case. Using the
assumption about the magnetic field lines going parallel along the conducting surfaces,
it follows for the non-slitted surfaces:
∂(rA)
=0
∂τ
at SilSurf (and IndSurf without slit),
(4.6)
4.2. AXISYMMETRIC MODEL OF HIGH-FREQUENCY EM FIELD
35
z
SilSurf
Feed rod
rmidd
rmax
IndSurf
n t
y
x
IndMidd
Inductor
IndSlit
Melt
SilSurf
IndSurf
IndSlit
IndMidd
Crystal
different
kinds of
calculation
boundaries
plane of one of
the small slits
r
Figure 4.3: The different boundary lines relevant in the calculation.
where τ is the local tangential direction along the boundary lines. For IndSurf the
condition (4.6) is valid only when not accounting the main slit of the inductor. The
modification including the main slit’s influence see below.
Since the silicon surface includes points at the symmetry axis and A must have a finite
value everywhere, the boundary condition for vector-potential follows from (4.6):
A=0
at SilSurf .
(4.7)
In frame of a model not accounting the main slit’s influence, the equation (4.6) yields
the boundary condition also for the non-slitted part of inductor:
A=
4.2.2
C0
r
at IndSurf (without the main slit!)
(4.8)
Inductor model with m slits
It follows (see ) from the Maxwell equations that one can introduce a scalar potential for the slit current ‫ ג‬in the slit plane, z(x, y), such that
‫∇ = ג‬z
or
‫ג‬x =
∂z
,
∂x
‫ג‬y =
∂z
.
∂y
(4.9)
36
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
At the line IndSlit, the azimuthal current and the normal component of the current in
the slit plane are equal: ‫ג‬n = J (assuming the normal direction as shown in Fig. 4.3).
On the other hand, ‫ג‬n =
∂z
,
∂n
therefore we obtain:
J=
∂z
∂n
at IndSlit.
(4.10)
Taking into account the properties of the magnetic field B and the definition of the
vector-potential A, the relation between the magnetic fields outside and inside the slit
is yielding the following condition at the IndSlit-line :
∂(rA) mbµ0 ∂z
+
=0
∂τ
2π ∂τ
at IndSlit,
(4.11)
where m – the count of slits, b – the width of each slit, τ – the tangential coordinate
along the line IndSlit like shown in Fig. 4.3.
From the assumption that the normal component of the high-frequency magnetic field
at the conducting surfaces is zero, it follows:
∂z
=0
∂τ
at IndMidd .
(4.12)
Since the current satisfies the condition div‫ = ג‬0, we obtain with help of (4.9) the
equation for the scalar potential in the slit plane:
∆z(x, y) = 0
or
∂2z ∂2z
+
= 0.
∂x2
∂y 2
(4.13)
This equation should be solved in the slit plane (the shaded area in Fig. 4.3). For a
boundary condition we use (4.12), moreover we may choose zero level for the constant
z at IndMidd :
z=0
at IndMidd .
(4.14)
We have no other boundary conditions for z, but we have the equation (4.11) coupling
at IndSlit together the fields of scalar potential z and vector-potential A. This can
be rewritten in a more convenient form:
A+
µ0
C0
mbz =
2πr
r
at IndSlit,
(4.15)
where the constant C0 equals that in (4.8) to ensure fitting together of the conditions
(4.15), (4.8) and (4.14) in the two common endpoints of the boundary lines IndSlit,
IndSurf and IndMidd.
4.2. AXISYMMETRIC MODEL OF HIGH-FREQUENCY EM FIELD
4.2.3
37
Approximation for the main slit
There are several different possibilities of introducing the main slit in the mathematical
model above. However, some of them ask for a considerable increasing in the number of equations for the final numerical problem formulation, which is a disadvantage.
Since any of the axisymmetric models can, in principle, produce only a very approximate image of the main slit’s effect, we have chosen the most rough of the possible
The idea is to replace the constant C0 in the boundary condition (4.8) by a function
C̃(r) that is changing along IndSurf in order to take in account the vertical flux of
magnetic field going through the outer part (i.e., the part at the right hand side from
IndMidd ) of the main slit. The inner part of the main slit was already accounted
together with the small slits, therefore it is out of interest at this point. So the new
boundary condition takes the form
A=
C̃(r)
r
at IndSurf (with the main slit!)
(4.16)
The shape of the function C̃(r) must be obtained from physical considerations. The
vertical component of the magnetic field near the slit plane, By , is coupled with the
horizontal current density in the slit, ‫ג‬x , by the relation By = −µ0 ‫ג‬x . Let us introduce
an effective dimensionless parameter Islit defined as the ratio between the effective
integral current flowing horizontally in the slit plane and the total current I0 going
through the inductor. It is clear that always Islit < 1. Then the approximate expression
for the horizontal current density is: ‫ג‬x = Islit I0 /Hav , where Hav is the average height
of the outer part of the main slit. Consequently, if the length of the outer part of the
main slit is L1 and the width is b1 , then the magnetic flux going through is:
Φ = B · b1 · L1 = µ0 Islit I0 · b1 L1 /Hav .
(4.17)
On the other hand, the same magnetic flux can be expressed also with the vectorpotential values at the inner and outer radial positions of the outer part of the main
slit:
Φ = 2π [rmax A(rmax ) − rmid A(rmid )] ,
(4.18)
where rmax is the outer radius of the inductor and rmid is the maximum radius of the
line IndMidd as shown in Fig. 4.3. The previously introduced parameter L1 equals to
38
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
rmax − rmid . Using (4.16), the last expression for the magnetic flux can be transformed
in terms of C̃. Together with (4.17) it yields:
C̃(rmax ) − C̃(rmid ) =
µ0 Islit I0
· b1 L1 /Hav .
2π
(4.19)
Assuming a linear change of the function C̃(r) between rmid and rmax and recalling
that C̃(rmid ) must be equal to C0 in order to fit the boundary conditions at IndSlit
and IndMidd, we obtain:
C̃(r) =
µ0 Islit b1
I0 · max {0; r − rmid } + C0 .
2πHav
(4.20)
The meaning of the “max”-function is to retain consistent boundary conditions also
for a case with a slightly sloped IndMidd -line, as in the example in Fig. 4.3.
4.2.4
The numerical method
The problem formulated above with the modified boundary condition (4.16) and (4.20)
is solved numerically by the Boundary Element Method (BEM). The boundary lines
shown in Fig. 4.3 are discretised into boundary elements. The elements are indexed
with index k and we can write symbolically k ∈ SilSurf, IndSurf, IndSlit, IndMidd ,
meaning that the boundary element belongs to one of these surfaces. The vectorpotential A(ı) in some spatial point denoted by ı (or in the center of the boundary
element with index ı) is expressed as a sum of the partial vector-potentials (Ak (ı) ·
Jk ) created in the point ı by the element k (i.e., by the axisymmetric surface ring
represented in 2D by the line segment k):
X
A(ı) =

Ak (ı) · Jk .
(4.21)

 SilSurf 




k∈IndSurf




IndSlit
Each term (Ak (ı) · Jk ) is a fundamental solution of the Poisson’s equation (4.5) and
contains the current density Jk in the element k. The coefficients Ak (ı) can be expressed
with the elliptic integrals K(p) and E(p):
h
i
µ0 dk
p
Ak (ı) = √ ∗
· K(p) · 1 −
− E(p) ,
π r ·p
2
(4.22)
4.2. AXISYMMETRIC MODEL OF HIGH-FREQUENCY EM FIELD
with
p=
39
4r∗
,
r∗ 2 + z ∗ 2 + 2r∗ + 1
r
z − zk
,
z∗ =
,
rk
rk
where dk is the cross-section length of the boundary element k, while rk and zk are
r∗ =
the coordinates of its middle point.
The scalar potential z is expressed as a sum of the partial scalar potentials (Pk (ı) · Kk )
created by the so called “charges” Kk in the boundary elements k of the slit boundary:
X
z(ı) =
Pk (ı) · Kk .
(4.23)
IndSlit
IndMidd
)
k∈(
The coefficients Pk (ı) in the fundamental solutions (Pk (ı) · Kk ) of the equation (4.13)
are:
Pk (ı) = dk · ln
p
(r − rk )2 + (z − zk )2 .
(4.24)
It follows from the relation (4.10) that the azimuthal current density at the boundary
of the small slit is:
J(ı)
ı∈IndSlit
∂z(ı) =
=
∂n ı∈IndSlit
X
Nk (ı) · Kk ,
(4.25)
IndSlit
IndMidd
k∈(
)
where
Nk (ı) =
∂Pk (ı)
.
∂n
(4.26)
To solve the problem numerically, the equations arising from the boundary conditions
(4.14), (4.15), (4.7) and (4.16) by substituting the expressions (4.21), (4.23) and (4.25)
are written for each of the boundary elements (ı running over all the boundaries). The
variables to be solved are the currents Jk (k ∈ SilSurf, IndSurf ) and the “charges”
Kk (k ∈ IndSlit, IndMidd ). One additional variable, the total inductor current I
renormalized so that C0 = 1, arises because of the accounting of the main slit and
implies solving of an additional equation (the first one of the equations below). The
equations are as follows:
ı=0:
"
−I +
X
k∈IndSurf
dk · Jk +
IndSlit
IndMidd
k∈(
#
X
X
)
`∈IndSlit
d` Nk (`) · Kk = 0
(4.27)
40
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
ı ∈ SilSurf :
"
X
X
IndSlit
k∈(IndMidd
)
`∈IndSlit
Ak (ı) · Jk +
SilSurf
k∈(IndSurf
)
#
X
A` (ı)Nk (`) · Kk = 0
(4.28)
ı ∈ IndSurf :
rmid
µ0 b1 Islit
· max 0; 1 −
·I
−
2πHav
r(ı)
"
#
X
X
X
1
Ak (ı) · Jk +
A` (ı)Nk (`) · Kk =
+
(4.29)
r(ı)
IndSlit
SilSurf
k∈(IndMidd
k∈(IndSurf
) `∈IndSlit
)
ı ∈ IndSlit :
"
X
Ak (ı) · Jk +
SilSurf
k∈(IndSurf
)
X
#
1
µ0 mb
Pk (ı) · Kk =
(4.30)
A` (ı)Nk (`) +
2πr(ı)
r(ı)
`∈IndSlit
X
IndSlit
k∈(IndMidd
)
ı ∈ IndMidd :
X
Pk (ı) · Kk = 0
(4.31)
IndSlit
IndMidd
k∈(
)
The system of linear algebraic equations is solved by a direct method (Gauss elimination).
4.3
4.3.1
Open melting front: the “fluid film model”
Fluid film thickness h
The proposed model for the open melting front is an improvement of that used in
Ref. . Although in reality the structure is more complicated, we assume that the
molten silicon at the open melting front forms a thin fluid film, of which the thickness
changes smoothly in the meridional direction but not in the azimuthal direction. Due
to gravity, the fluid flow is directed downwards along the front in the meridional
direction and obeys the Navier-Stokes equation, which may be written in the specific
case as follows:
d2 v
+ ρl g sin θ = 0,
dn2
where η is the dynamic viscosity, g, the gravity and v = v(n), the flow velocity, which
η
together with the chosen reference of the normal coordinate n and the angle θ(r) is
4.3. OPEN MELTING FRONT: THE “FLUID FILM MODEL”
41
depicted in Fig. 4.2. Requiring zero velocity at the melt–solid boundary and zero shear
stress at the free surface of the fluid film, we get the parabolic velocity profile in the
film:
v(n) =
ρl g sin θ 2
h − n2 ,
2η
(4.32)
where h denotes the fluid film thickness. The fluid discharge at fixed location r is
proportional to the integral of the velocity over n and is related to the melting rate
upward from that location. For a stationary process:
Z
0
v(n)dn = ρs · π RF 2 − r2 VF ,
ρl · 2πr
(4.33)
−h
where VF is the constant feed move rate and RF , the radius of the feed rod. From (4.32)
and (4.33), we obtain, in frame of the simplified model, the film thickness distribution
along the open melting front:
"
3ηρs VF RF 2 − r2
h=
2ρl 2 g sin θ(r) · r
4.3.2
#1/3
.
(4.34)
Joulean heat flux at the open melting front
The integral surface density of the induced power in the skin layer of the bulk melt or
solid can be calculated by the formula (3.14), as shown in Section 3.3. This formula is
not applicable in case of the open melting front because of the inhomogeneous material
properties along the depth of the skin layer. The total Joulean heat flux density at
EM
the open front, q EM , including both, the power qM
in the molten film of depth h and
the power qFEM deeper in the solid feed, is expressed as follows:
EM
EM
+ qFEM = ξ · qh→∞
,
q EM ≡ qM
(4.35)
EM
where qh→∞
is the surface density of a fictitious power calculated for case when the fluid
film thickness is much larger than the skin layer depth, and the factor ξ is introduced
like in  to account how much higher is the power due to the finite depth of the film.
To derive ξ analytically, we consider the penetration of the EM field into the conducting
medium near the open front. By neglecting the displacement currents in the Maxwell
equation and using the material relation j = σE for the volume current density, we
have
rotB = µ0 σ(n)E,
42
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
where the change in the normal direction of the conductivity σ is emphasized due to
the jump at the melt–feed boundary at n = −h (see the orientation of the n-axis in
Fig. 4.2). With help of the other Maxwell equations, we obtain the equation for the
azimuthal component E of the electric field,
∂ 2 E(n, t)
E(n, t)
,
=
µ
σ(n)
0
∂n2
∂t
where we account for the spatial change only in the normal direction. The solution
is sought in the form E(n, t) = E a (n) cos(ωt + ∆), where ω = 2πf , and the field
amplitude E a must decrease exponentially with the penetration depth. The solution
satisfying the continuity at n = −h is:
n
cos ωt +
E(n, t)|−h<n<0 = E (0) · e
δ
l
n
h
a
−h/δ 0
n/δs
E(n, t)|n<−h = E (0)e
·e
cos ωt + − 0
δs δ
a
n/δl
with the designation δ 0 = (1/δl − 1/δs )−1 and
1
πµ0 f σl,s
δl,s = p
for the skin layer depth in the liquid and solid, respectively.
The relation between the field and the volume current density,
j(n, t) = σ(n)E(n, t),
and the relation between j and the effective surface current ief , i.e.,
i2ef
2
0
Z
j(n, t)dn
=
,
−∞
allow to express the amplitude of j at the free surface of the film, j a (0) = σl E a (0), in
terms of ief . The latter is known since calculated by the boundary element method
(Section 4.2). The volume current density distribution j(n, t) is hereby determined
and yields the Joulean heat flux:
q
EM
Z
0
=
−∞
j 2 (n, t)
dn.
σ(n)
This way, the expression (4.35) is evaluated and the coefficient ξ is found:
ξ(h) =
1 − (1 − κ) e−2`
,
1 − 2(1 − κ) e−` cos ` + (1 − κ)2 e−2`
(4.36)
4.3. OPEN MELTING FRONT: THE “FLUID FILM MODEL”
5
5
4
4
x(h)
3
2
1
1
0
0
0
0.2
0.4
x (h)
F
3
2
0.6
0.8
1
1.2
43
x (h)
M
0
0.2
h (mm)
0.4
0.6
0.8
1
1.2
h (mm)
Figure 4.4: Dependence of the dimensionless heat fluxes ξ, ξM and ξF on the film
thickness h in frame of the “fluid film model” for the open front.
where
` ≡ `(h) = h/δl ,
p
κ = σs /σl ≡ δl /δs .
EM
The expression for qh→∞
in (4.35) is identical to that for the Joulean heat flux at the
free surface of the bulk melt, cf. (3.14):
EM
qh→∞
i2
= ef ≡
σl δl
r
πµ0 f 2
i .
σl ef
(4.37)
Deriving the formula of ξ, respectively, q EM , we obtain by the way also the separate
EM
expressions of qM
and qFEM , which are needed when considering the vicinity of the inner
triple point (see Section 4.5.1). The coefficient ξ may be regarded as the dimensionless
counterpart of the heat flux q EM . Similarly, we can introduce the coefficients ξM and
EM
ξF (satisfying ξM + ξF = ξ) as the dimensionless counterparts of the heat fluxes qM
and qFEM :
EM
EM
qM
= ξM · qh→∞
and
EM
qFEM = ξF · qh→∞
.
(4.38)
The expressions for ξM and ξF are as follow:
ξM (h) =
1 − e−2`
,
1 − 2(1 − κ) e−` cos ` + (1 − κ)2 e−2`
(4.39)
ξF (h) =
κe−2`
.
1 − 2(1 − κ) e−` cos ` + (1 − κ)2 e−2`
(4.40)
44
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
The shapes of the functions ξ(h), ξM (h) and ξF (h) corresponding to the conductivities
of liquid and solid silicon and to the EM frequency of 2.8 MHz are shown in Fig. 4.4.
We see, e.g., that the value ξ = 1.4 used in  corresponds to a constant thickness of
the fluid layer h = 0.2 mm. The advantage of the new model is a variable h according
to (4.34) and, consequently, a variable ξ along the open front according to (4.36).
4.4
Shape of the free melt surface
The free surface equation has been derived in Section 3.5 and the flow-related terms
have been analysed in Section 3.6. Here, a simplified version of equation (3.36), i.e.,
with neglecting the most of the flow-related terms and keeping just the contribution
due to the centrifugal forces, which is integrated by assuming a solid-body rotation as
shown in (3.46), is used to derive a practical calculation procedure for the free melt
surface. From the above-mentioned equations, it follows that the effective pressure
imbalance
D = p0 − ρl gz − γ
cos φ
1
+ 0
r
R
− pEM + 2π 2 ρl Ω2Cr r2
(4.41)
must equal zero in the equilibrium state at every point (r; z) of the free melt surface.
The designations in (4.41): φ denotes the local surface angle with vertical (see Fig. 4.2),
γ is the surface tension of the melt, R0 , the meridional curvature radius (positive for
a convex surface), ΩCr , the rotation rate of the crystal rod, p0 , the gauge pressure
in the melt, and pEM , the EM pressure (3.19), i.e., the integral effective value in the
high-frequency approximation as derived in Section 3.3.
For a given gauge pressure p0 , the equality to zero of the imbalance (4.41) allows to
determine the shape of the free surface with fixed inner and exterior triple points. The
value of p0 is unknown and its determination needs an additional condition. In frame
of the steady-state model, the exterior rim of the crystal grows vertical and the free
surface makes a definite angle with the vertical, φETP = φ0 , at the exterior triple point
(ETP). For silicon, the meniscus angle required to keep a constant crystal diameter,
φ0 ≈ 11◦ , is known from the literature.
The free surface is divided into linear elements in order to require zero imbalances
(4.41) in every node. The curvature radius R0 is approximated in the nodes by the
radius of a circle drawn through the node of interest and its two neighbouring nodes.
At the inner triple point, the next node of the open melting front is taken as one
of the neighbouring nodes. A special approach is used at the exterior triple point.
4.4. SHAPE OF THE FREE MELT SURFACE
45
0
at the
Figure 4.5: The discretized free melt surface and the curvature radius RETP
exterior triple point.
A circle is drawn through ETP and a next node of the free surface and its radius is
chosen so that the tangent at ETP makes angle φ0 with the vertical. From geometrical
considerations, as shown in Fig. 4.5,
1
0
RETP
=
2 · sin(φ0 − α)
,
L
(4.42)
where L is the length of the first element and α, the actual angle that the first element
makes with the vertical.
The equality to zero of the imbalance at the exterior triple point, DETP = 0, yields
the gauge pressure:
p0 = ρl gzETP + γ
cos φ0
1
+ 0
rETP
RETP
2
2 2
+ pEM
ETP − 2π ρl ΩCr r ,
(4.43)
0
where the curvature radius at the triple point, RETP
, is obtained by (4.42). Thus,
for a fixed distribution of electric current, the gauge pressure p0 depends upon the
position of the first node next to ETP, i.e. p0 = p0 (L, α). Due to this reason, the
minimization of imbalance begins at this node and the other nodes of the free surface
are considered sequentially from ETP to ITP. The shifting of nodes is performed along
the bisector between the neighbouring surface elements. By displacing the first node
46
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
in the direction of action of the pressure imbalance, the minimum of |D| is searched
by putting the actual value (4.43) of p0 into formula (4.41). At the following nodes,
the imbalance is reduced similarly but the gauge pressure is kept constant as known
from the last calculation of the first node. The advantage of the described approach
is that no special iteration cycle for p0 is needed to accomplish the angle condition at
ETP.
With a fixed EM field, the sweeps through all nodes are repeated many times and the
imbalance value at ITP is used to judge about the convergence of the free surface. To
couple the free surface and the EM field, some outer iterations are performed. During
these iterations, ITP stays fixed but the value of the pressure imbalance at the inner
triple point, DITP , is obtained. It is further used to calculate the location of ITP as
described below.
4.5
4.5.1
The inner triple point and related numerical aspects
Inner triple point
The inner triple point is the point in the model where the melting interface, the free
surface and the open front are going together. The calculation procedure of ITP is
based on the assumption that the transition “melting interface—open front” is smooth.
This assumption fits well to the fluid film model of the open front since the transition
between the fluid film and the bulk melt must be smooth. The front’s normal direction
at ITP is calculated like in every other node of the melting interface or open front
(see Fig. 4.6) and the distribution of the front velocity vn is kept continuous at ITP,
as described below. Consequently, what concerns the front movement, we treat the
melting interface and the open front as one united front. This ensures the first degree
of freedom of ITP (denoted by “1” in Fig. 4.6), i.e., the motion due to moving of the
melting front.
Another degree of freedom of ITP (denoted by “2” in Fig. 4.6) is the motion due to
changing of the free surface shape, which raise the pressure imbalance at the inner
triple point, DITP , as considered in Section 4.4. The location of ITP at the united
melting front is chosen in order to minimize the absolute value of the imbalance. Each
new trial position of the inner triple point and detection of DITP requires a recalculation
of the free surface shape coupled with the EM field, therefore special algorithms are
4.5. ITP AND RELATED NUMERICAL ASPECTS
47
Figure 4.6: The numerical approach to the inner triple point.
used to reduce the count of recalculations needed.
The third possibility of motion of ITP in this model is the one denoted by “3” in
Fig. 4.6. When the free surface touches the melting interface below the ITP location,
the inner triple point moves downwards in order to eliminate the degenerate bulk melt
layer, the thickness of which is vanishing.
The above-mentioned continuity of the front velocity vn at ITP is essential and is
obtained by correcting the expression (4.3) for velocity of the melting interface to take
into account that a part of the interface is very close to the free melt surface. If the
penetration depth of the EM field is comparable to the depth of the fluid layer covering
the feed, a part of the total induced power q EM , namely, qFEM , is induced in the feed
volume and hence should be included in the velocity formula for the melting interface
close below ITP:
ṽn =
λs ∂T qFEM
λl ∂T −
−
− VF nz ,
ρs Q ∂n F ρs Q
ρs Q ∂n l
(4.44)
where T designates the temperature field calculated under assumption of a small EM
skin depth allowing the integral heat flux boundary conditions (4.62) as applied for
the temperature calculation in the melt (see Section 4.6). Consequently T does not
describe the temperature gradient inside the skin region. The terms in (4.44) that are
48
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
grouped in parenthesis correspond to the correct heat flux in feed in the vicinity of
the interface. Beside that, since qFEM is accounted inside the feed, it is meaningful to
EM
EM
use only the heat flux qM
, instead of the total q EM = qM
+ qFEM , as the boundary
condition at the free surface of the melt closely below ITP1 :
λl
∂T
EM
= qM
∂n
(4.45)
It can be seen that the open front velocity (4.4) and the corrected melting interface
velocity (4.44) are equivalent at the inner triple point if the field T satisfies the boundary condition (4.45) precisely. This condition is, however, not so precisely fulfilled due
to the numerical model used and it is thus better to calculate the velocity at ITP by
the open front formula (4.4). The accuracy of the melting interface formula (4.44)
improves in the next nodes below ITP with increasing distance between the front and
the free surface of the bulk melt.
In this context, we introduce a small transition zone, where the formula (4.4) smoothly
turns into formula (4.44). The transition zone is that part of the melting interface
from where the geometrical distance to the modelled free surface, hg , is less than the
fluid film thickness in the triple point, hITP . The transition zone allows to avoid the
contradiction between the modelling of the open front as a single line and ITP as a
single point, which means hgITP ≡ 0, and considering at the same time a finite fluid
film thickness h according to (4.34), i.e., hITP > 0. The following mixed velocity value
is used at the melting interface in the transition zone hg < hITP :
vnmix =
hg
hITP − hg film
· ṽn +
· vn ,
hITP
hITP
(4.46)
where ṽn is the corrected melting interface velocity (4.44) and vnfilm is the velocity
calculated according to (4.4) like for the open front under a fluid film of thickness
hg + hITP .
Under certain circumstances, it may happen that the front actually has a corner at the
location of the inner triple point and the respective front velocity undergoes a discontinuity. To maintain the degrees of freedom of ITP in our calculation, the algorithm
avoids a sharp corner between neighbouring discretization elements of the front by
using a local smoothing in the region of ITP (see Section 4.5.4). The smoothing, however, does not deteriorate the solution in larger scale with multiple elements as it can
1
Analogical considerations are applicable also to the calculation of the EM pressure on the free
surface near ITP.
4.5. ITP AND RELATED NUMERICAL ASPECTS
49
Figure 4.7: Examples of triangulation.
be seen in Fig. 4.6: the uppermost open front element shown and the leftmost melting
interface element shown make a corner of 90◦ . Thus it is enough to use reasonably fine
discretization to calculate states with a corner at ITP.
4.5.2
Triangular grid generation with refinement at ITP
The temperature field in the molten zone, feed rod and single crystal as well as the
hydrodynamics in the molten zone are calculated in FZONE by the Finite Element
Method (FEM) as described in further sections. Each of the three calculation domains
is discretized in linear finite elements (triangles). Since the domain boundaries are
changing during the calculation process, the triangular grid is adjusted at each step in
order to fit the respective boundaries.
The grid generator used in FZONE is the C code “Triangle” (version 1.2) by Jonathan
Richard Schewchuk [79, 80, 81]. It computes Delaunay triangulations and constrained
Delaunay triangulations by the exact arithmetic. Quality meshes, i.e. meshes having
no small angles are generated using Ruppert’s Delaunay refinement algorithm. Among
other features of the generator the ones used in FZONE are the possibility to set the
user-specified constraints on angles and triangle areas and the possibility to put the
50
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Figure 4.8: Examples of the ITP refinement with forced additional nodes.
obligatory nodes in the inner volume as well as on the boundary.
In the implementation in FZONE, the grid generation in each of the calculation domains
(melt, feed rod and crystal) is performed separately, one after each other. An example
of the mesh is shown in Fig. 4.7. The grid density in the domains is controlled by the
density of the elements at the domain boundaries. Hence beside the phase interfaces
and the boundaries that are needed for the electromagnetic field calculation by the
Boundary Element Method as described in Section 4.2, there are also boundaries
defined at the central axis of all three domains. To avoid too big element areas in the
middle of domains far from the boundaries, area constraint is imposed on the elements
generated. For a domain with maximum boundary element length being equal dmax ,
√
the area constraint is set to Amax = 3/4 · d2max (the area of a triangle whose each side
equals dmax ). Furthermore an angle constraint of 33◦ for the minimum inner angle of
the triangles is imposed for obtaining a high-quality mesh. This level of mesh quality
remains sometimes unachieved due to geometrical reasons like domain boundary with
a small inner angle or too big aspect ratio of two neighbouring boundary elements.
The first reason, the boundary with a small inner angle, usually takes place in the melt
domain closely below the inner triple point. To obtain an optimum grid for the region
below ITP, FZONE puts additional nodes in the melt volume that forces mesh generator
to make a better refinement at this place. Examples of the ITP refinement for two
different cases, smooth connection between the open front and melting interface and
a corner-like connection, are shown in Fig. 4.8.
4.5. ITP AND RELATED NUMERICAL ASPECTS
4.5.3
51
Numerical stabilization in case of quasi-vertical melting front
The melting front has often a vertical or nearly vertical part about or below the ITP.
The approach to the phase boundary calculation as described in Section 4.1 leads to
a numerical problem: the quasi-vertical part of the melting front becomes numerically
instable and shows nonphysical wavy shapes that change and even grow with time.
The reason of these convergence difficulties is explained in the following way.
Let us first consider vn , the local normal velocity of the melting front in the laboratory
reference system, i.e. the velocity that characterizes the unsteadiness of the process,
as described in Section 4.1. The vertical component nz of the normal vector n, the
direction of which at the melting front is depicted in Fig. 4.2, is significantly influencing
the value of vn . Indeed, the equation (4.2) can be rewritten in the form
vn = Vn − VF nz
with Vn , the normal front velocity in the reference system of the feed rod, i.e. the
melting rate from the atomic point of view, and VF , the feed move rate, which is a
positive constant. At the quasi-vertical part of the front we have Vn VF because
little melting occurs in the radial direction if we consider a nearly steady-state shape
of the front. Meantime the value of nz is close to zero at the quasi-vertical part
and consequently nz is changing relatively much from node to node and from one
calculation step to another due to the numerical character of the solution process.
For the purpose of illustration of the numerical problem, we can assume that the
fluctuation of nz brings along the fluctuation of the front velocity vn in agreement
with the relation
vn ≈ −VF nz .
(4.47)
Further we consider the discretization of the melting front. The variables in FZONE
are generally stored at the discretization nodes and, if necessary, the values of the
variables inside the boundary elements or triangular finite elements are found by linear
interpolation from the node values. This way also the local normal front velocity vn
and the local normal direction n are considered in the nodes of the front. For defining
the front normal direction in a boundary node, a bisector is drawn between the two
normal directions of the neighbouring boundary elements found each side from the
node. Figure 4.9 illustrates a vertical part of melting front with one node (the node
designated by “2”) shifted to the right, which can occasionally happen due to the
solution process with permanent shifting of the front. The melting front itself is
52
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Feed
Melt
n (nz>0)
1
vn
2
3
n (nz=0)
vn
n (nz<0)
z
Melting front
r
Figure 4.9: Illustration to the mechanism of appearing of numerical instabilities at
a quasi-vertical melting front if using the bisectors as normal directions for velocity
calculation in the nodes.
drawn by a thick solid line. The thin solid lines and arrows show the bisectors and
the corresponding normal vectors in the nodes 1, 2 and 3. The thick arrows are
the velocities vn calculated by the formula (4.47) from the normal vectors. After
performing the time step with those velocities, the new shape of the front will be
something like the dashed line. At the node 2, the bisector direction will be changed
and the corresponding new velocity is shown by the dashed arrow. Meanwhile, the
bisectors and the velocities in nodes 1 and 3 preserve their directions. Therefore the
following time steps will lead to nodes 1 and 2 shifting considerably to the left and
node 3 going to the right and making a sharp corner similar to that the node 2 made
at the beginning. Continuing the calculation this way, uncontrolled appearance and
motion of a sharp step somewhere at the front can be obtained due to the described
numerical effect.
Hence a small numerical fluctuation, like at the node 2 in the above example but
smaller, is enough to introduce growing deviations from an even front shape. The
issue is that using the bisectors as normal directions work well when those directions
are not changing too steep from one node to another, which can take place not only
4.5. ITP AND RELATED NUMERICAL ASPECTS
Feed
Melt
1
n (nz=0)
n (nz>0)
vn
2
3
z
53
vn
n (nz<0)
Melting front
r
Figure 4.10: Illustration to the calming of numerical fluctuations by a special choice
of nz in the expression of vn .
due to a fluctuation but also when the discretization is too coarse.
Let us consider the solution of this problem. In principle, the choice of the normal
direction at a node can be modified in the limits of the discretization error, i.e., the
normal direction can be any direction between the directions of the real normal vectors
of the two neighbouring boundary elements. Therefore, to calm down the influence of
fluctuations and in the same time not overrun the discretization error, one can choose
as the node-normal the one of the element-normals that brings a stabilizing effect on
the shape fluctuations.
Following this idea in FZONE, the value of the normal velocity vn at a node of the
melting front is calculated by using nz from the one of the two neighbouring elements
that makes a smaller angle by absolute value, in the limits 0◦ —180◦ , with a vertical
line drawn upwards from the node. Only the value of vn is modified, while the direction
of the velocity vector and therewith the node movement are preserved in the bisector
direction as previously. This approach solves the instability problem.
The illustration of how a successful smoothing works in case of the example discussed
above is shown in Fig. 4.10. The difference from the previous behaviour (Fig. 4.9)
54
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Figure 4.11: Large turning angle α from one boundary element to the next.
is that the moving velocities vn are converging to zero now, and the shape is getting
more smooth with each time step. It should be emphasized that the “smoothness” is
relative with respect to the discretization element sizes, therefore also strongly curved
melting front shapes can, of course, be solved well if they are discretized fine enough.
The method described above works under the threshold of the discretization error and
therefore does not cause any additional artificial surface tension at the melting front.
4.5.4
Smoothness control of the discretized melting interface
In order to enable a good performance of the inner triple point moving algorithm
described in Section 4.5.1, the melting interface must be smooth enough. Often there
arise a problem with the discretized melting interface bending at some nodes, i.e., the
turning angle α from one boundary element to the next becomes large (see Fig. 4.11),
which leads to big discretization errors when the front is moving. Especially this
problem tends to appear in the vicinity of ITP and deteriorates its flexibility needed
by the algorithm. A possible way to solve this problem would be simply refining
the discretization, however there are times when this does not help if the solution
intrinsically contains a corner. Consequently another approach is necessary. The
specific method implemented in FZONE for avoiding sharp melting interface angles by
using what we call “selective artificial surface tension” is described below. It is also
explained why this works only locally and does not damage the solution as a nonselective artificial surface tension could do.
The main principle of the method of “selective artificial surface tension” is to select
4.5. ITP AND RELATED NUMERICAL ASPECTS
55
and influence only those turning angles that are “bad”, i.e., greater than a predefined
critical value αcrit . The front moving velocity v at the bad nodes must be corrected so
that the correction δv supports the motion towards the center of the front’s curvature,
which means diminishing the badness of the angle. The value of the velocity correction
may be obtained by
(
δv =
0
if α < αcrit
γ · (α − αcrit ) if α > αcrit ,
(4.48)
where α is assumed positive and γ is the artificial surface tension coefficient, which is
unknown and must be determined by the algorithm. The original velocity v may be
directed either in the direction of the center of the curvature (the “good” direction)
or in the opposite direction (the “bad” direction) in which the movement is increasing
the angle α. A large value of γ ensures overcoming the original velocity in case it is
directed in the bad direction. On the other hand, a too large γ leads to steep changes
in the velocity magnitude from one time step to the next and makes the calculation
of the front moving process hard and slow.
The considerations above have led to the following method for the choice of γ. First
we introduce a new limiting value of angle, αmax , which is greater than αcrit and which
serves as the maximum allowed value of the turning angle. Let us assume now that
among the “bad” nodes there are some “very bad” nodes, i.e., nodes with angles larger
or equal to αmax . We can find for each of them the minimum γ necessary to ensure
that the corrected velocity is not directed in the bad direction. Indeed, for the original
velocity in the bad direction, which is assumed the positive direction, the corrected
velocity will be reduced to zero or even made negative (see Fig. 4.12), i.e.
vcorr ≡ v − δv ≡ v − γ · (α − αcrit ) ≤ 0,
if the artificial surface tension coefficient for the given node satisfies the inequality
γ≥
v
.
α − αcrit
We have to use the same artificial surface tension coefficient for all nodes with bad
angles α > αcrit . Hence the maximum over the very bad nodes of the minimum
necessary γ is taken. If the γ value in the previous step has been larger than the new
value, then the old value is retained for the actual step to avoid permanent fluctuations
of γ during the calculation. So we determine γ by
vı
γ = max
; γold ,
ı ∈ {nodes ı : αı ≥ αmax }.
ı
αı − αcrit
(4.49)
56
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Figure 4.12: The original “bad” velocity v in a node with the turning angle α ≥ αmax ,
the correction δv, and the resulting corrected velocity vcorr ≤ 0.
The calculation is started with γ = 0 and it is adjusted at each step using the formula
(4.49). Only the nodes with αı > αcrit are touched by the corrections δvı (see (4.48))
and only in case some angle tends to increase larger than αmax the coefficient γ is
increased. As a result, γ increases in the first steps till a certain level, which is the
minimum necessary to keep the angles below αmax . The influence of the specific value
of αmax chosen is illustrated in Fig. 4.13. The selectivity of this “surface tension” is the
reason why the effect is local and influences only some nodes, presumed the parameter
αcrit has been set large enough. We can suppose that the changes in these nodes are
not exceeding the actual limits of the discretization error due to the finite length of
the discretization elements. By refining the discretization, it is possible to obtain more
precise solution and the region of the influence of the selective artificial surface tension
becomes more localized.
Figure 4.14 illustrates the local character of the influence of smoothing with αcrit = 30◦
and αmax = 45◦ , which are the standard values approved for calculations. The difference in scales in Figs. 4.14(a)–4.14(b) can be seen from the distribution of nodes.
4.5. ITP AND RELATED NUMERICAL ASPECTS
(a) αcrit = 30◦ , αmax = 45◦ , n = 2
57
(b) αcrit = 15◦ , αmax = 30◦ , n = 3
Figure 4.13: Applying the smoothing algorithm with different parameters αmax and
αcrit , which results in different number of corrected nodes, n.
(a) Close view: the rounded corner
(b) More global view of the same picture:
the influence of smoothing vanishes
Figure 4.14: Local character of the smoothing at ITP (αcrit = 30◦ , αmax = 45◦ ).
58
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
4.6
4.6.1
Axisymmetric melt flow
The ψ − ω equations in cylindrical coordinates
To calculate the temperature field in the molten zone, an axisymmetric model of the
melt flow and heat transfer is applied. For the incompressible fluid flow, the massconservation equation (3.25) and the Navier-Stokes equations with the Boussinesq
approximation (3.26) are transformed from the pressure–velocity variables (pHD , ur ,
uϕ , uz ) to the variables ψ, ω and uϕ , which brings the advantage that the mass
conservation is satisfied automatically and the number of equations to solve is reduced
[76, 82]. The stream function ψ and the vorticity ω are defined by
ur = −
1 ∂ψ
,
r ∂z
uz =
1 ∂ψ
,
r ∂r
ω ≡ (∇ × u)ϕ =
∂ur ∂uz
−
,
∂z
∂r
(4.50)
and the whole set of hydrodynamic equations including the heat transfer equation
(3.27) is written in the cylindrical coordinates (r, ϕ, z) as follows2 :
∂ 1 ∂ψ
∂ 1 ∂ψ
+
+ω =0
∂r r ∂r
∂z r ∂z
∂T
∂T
1 ∂
∂T
∂T
∂
∂T
+ ur
+ uz
=
χr
+
χ
∂t
∂r
∂z
r ∂r
∂r
∂z
∂z
∂uϕ
∂ ν ∂(ruϕ )
∂
∂uϕ
ur
∂uϕ
∂uϕ
+ ur
+ uz
=
+
ν
− uϕ
∂t
∂r
∂z
∂r r ∂r
∂z
∂z
r
∂ω
∂ω
∂ ν ∂(rω)
2uϕ ∂uϕ
∂T
∂
∂ω
ur
∂ω
+ ur
+ uz
=
− gβ
+
ν
+ ω+
∂t
∂r
∂z
∂r r ∂r
∂z
∂z
r
r ∂z
∂r
(4.51)
(4.52)
(4.53)
(4.54)
where χ is the thermal diffusivity of the liquid, χ = λl /(ρl cp ), ν is the kinematic
viscosity, ν = η/ρl , and g = |gz |. Since the electromagnetic force is treated in the
high-frequency approximation as a surface force as well as the Joulean power is approximated by a heat flux through the boundary (see Section 3.3), there are no volume
forces beside gravity and no volume heat sources included in these equations.
2
Obviously there has been a mistake in expressing the vorticity equation in cylindrical coordinates
in previous works like [45, 46, 7] where the equation (4.54) has been written without the vortexstretching-related term ur ω/r, which arises due to the curvature of the coordinate system when
taking the ϕ-component of the vorticity equation
∂~
ω
+ (u∇)~
ω = ν∆~
ω + (~
ω ∇)u + gβ × ∇T.
∂t
Here ω
~ ≡ ∇ × u while the designation ω as defined by (4.50) always stands for the ϕ-component of
ω
~ = (ωr , ω, ωz ), with subscript ϕ just being dropped for convenience.
4.6. AXISYMMETRIC MELT FLOW
4.6.2
59
Boundary conditions
The general flow boundary conditions were considered in Section 3.4 and, particularly
for the free surface, in Section 3.5. Here the boundary conditions are rewritten for the
ψ − ω formulation.
Let us choose a vertical cross-section plane going through the symmetry axis of the
molten zone and a line in this plane, e.g., a line on the boundary of the melt. From
the coordinates (r, z), we can switch everywhere along this line to local coordinates
(τ , n), with τ being the tangential- and n, the normal direction locally at each point
of the chosen line. This coordinate transformation allows the following recasting of
the definitions (4.50):
uτ = −
1 ∂ψ
,
r ∂n
un =
1 ∂ψ
,
r ∂τ
ω=
∂uτ
∂un
−
.
∂n
∂τ
(4.55)
If neglecting the relatively slow (few millimeters per minute) flow across the solid–melt
interfaces occurring due to the crystallization and melting, we can assume un = 0 at
all boundaries of the melt3 . According to (4.55), we have then a constant value of ψ
at all melt boundaries and can choose this value equal to zero. At boundaries with
the no-slip condition we get additionally according to (4.55) a zero normal derivative
of the stream function.
Boundary with un = 0
⇒
ψ = 0,
Boundary with uτ = 0
⇒
∂ψ
=0
∂n
ω=
∂uτ
Fτ
=
∂n
η
(4.56)
(4.57)
Fτ in (4.56) is the tangential stress at the boundary. At the free melt surface, this
vorticity boundary condition corresponds to (3.34) and Fτ is created by the action
of the electromagnetic and Marangoni forces as given by the expressions (3.30) and
(3.21):
Fτ =
µ0 δ ∂(ief 2 ) ∂γ ∂T
+
.
4 ∂τ
∂T ∂τ
(4.58)
At the symmetry axis, which is also one of the melt boundaries in the axisymmetric
problem formulation, we can put simply Fτ = 0. At the rigid boundaries, however,
3
This corresponds to putting uz = 0 in (3.28) and (3.29). Such simplification is favourable for the
ψ − ω formulation, additional measures have, however, to be met if the precise resolution of the flow
at interfaces is necessary, e.g., in case of the calculation of dopant concentration, which typically has
a very steep boundary layer due to the segregation.
60
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
the tangential stress is not explicitly known and a more specific formulation of the
boundary condition for the vorticity ω has to be considered:
Boundary with un = 0, uτ = 0
⇒
1 ∂2ψ
ω=−
.
r ∂n2
To make this boundary condition of ω suitable for the calculation procedure, we approximate the second order derivative of ψ by lower order derivatives by using the
beginning of the Taylor series of the function ψ(n) near the boundary n = 0:
∂ψ n2 ∂ 2 ψ ψ(n) ≈ ψ(0) + n
+
.
∂n n=0
2 ∂n2 n=0
Due to the boundary conditions for ψ from (4.56) and (4.57), the first two terms on the
right-hand side of the approximate equation equal zero. Hence we have the following
no-slip boundary condition for ω, which is known as the Thom condition:
Boundary with un = 0, uτ = 0
⇒
ω=−
ψ(n)
2
lim 2 .
r n→0 n
(4.59)
To summarize, the boundary conditions for the thermal–hydrodynamic problem in the
melt are as follows.
1. Symmetry axis (un = 0, Fτ = 0):
∂T
= 0,
∂r
uϕ = 0,
ψ = 0,
ω = 0.
(4.60)
2. Crystallization and melting interfaces (un = 0, uτ = 0):
T = T0 ,
uϕ = 2πr ΩCr,F ,
ψ = 0,
ω=−
2 ψ(n∗ )
r n2∗
(4.61)
with T0 denoting the melting point temperature, ΩCr,F , the rotation rate of the
crystal (Cr) or feed rod (F), r, the radial coordinate of the considered boundary
point, and ψ(n∗ ), the value of the stream function at as small as possible distance
n∗ from the boundary (in practice this distance is determined by the locations
of the nearest nodes).
3. Free melt surface (un = 0, Fτ = (4.58)):
λl
∂T
= q EM − q rad ,
∂n
∂uϕ
uϕ ∂r
=
,
∂n
r ∂n
ψ = 0,
ω=
Fτ
,
η
(4.62)
4.6. AXISYMMETRIC MELT FLOW
61
where q rad is calculated as described in Section 4.7 and q EM is calculated by (3.14)
or (4.37) based on a previously calculated distribution of surface currents (the
calculation of the surface currents see in Section 4.2). For the free melt surface
EM
in the vicinity of ITP, the qM
must be used instead of q EM , as pointed out in
Section 4.5.1. The boundary condition for the azimuthal velocity uϕ comes from
(3.35) by setting Fϕ = 0 due to the axial symmetry of the model. For the sake
of the numerical method described below, the following equivalent form of the
free surface boundary condition for the azimuthal velocity is used:
∂(ruϕ )
∂r
= 2uϕ .
∂n
∂n
4.6.3
(4.63)
The numerical method: SUPG-stabilized FEM
For the numerical solving of the flow and heat transport problem, the Finite Element
Method (FEM) is used. Let us shortly consider the principles of the method for
application to a flow problem like that one formulated above.
The equations (4.51), (4.52), (4.53) and (4.54) have the general form
(2)
Lt u
|{z}
time change
+ Lconv u = Ldiff u + s(1)
u + s(0)
| {z }
| {z } |∗ {z ∗ }
convection
diffusion
source terms
where Lx are the differential operators corresponding to different parts of the equation,
u = u(x) is the unknown field over the calculation domain x ∈ Ξ, the source term
(0)
(1)
(s∗ u) is the part proportional to u, and s∗
is the u-independent part of sources.
Because the solution of the above equation is, in general, time dependent, we calculate
the instantaneous field u at time t by taking in account the “old” field distribution
uold at time t − ∆t. The field uold has been calculated or predefined previously. For
the sake of numerical robustness at large time steps ∆t, the implicit scheme is used:
the field uold appears only in the time-derivative term while the actual field u is placed
in the rest part of equation. The time derivative is approximated by
Lt u ≈
(1)
where st
(0)
= −1/∆t and st
u − uold
(1)
(0)
= −st u − st
∆t
= uold /∆t. This way the form of the general equation
can be simplified by including the time derivative in the source terms:
(2)
Lconv u = Ldiff u + s(1) u + s(0)
(4.64)
62
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
(1)
(1)
with s(1) = s∗ + st
(0)
(0)
and s(0) = s∗ + st .
We have discretized the calculation domain Ξ and look for the approximate solution
in the form of a linear combination of predefined basis functions Nı (called also shape
functions or trial functions):
u(x) =
X
Nı (x)uı ,
(4.65)
ı∈{nodes}
where uı are the unknown coefficients. The number of the basis functions and the
number of the coefficients are here both equal to the number of nodes. In FEM, only
the weak form of equation (4.64) is solved:
Z
(2)
(1)
(0)
Wı Lconv u − Ldiff u − s u − s
dΞ = 0,
ı ∈ {nodes},
(4.66)
Ξ
where Wı = Wı (x) are the weight functions (or test functions). The number of weight
functions is also equal to the number of nodes. The idea in FEM is to substitute (4.65)
into (4.66) to get the system of equations for the unknown coefficients uı . A typical
(2)
problem is however the diffusion term Ldiff , which has second order derivatives and
creates singularities if the first derivative of the basis functions Nı (and hence that of
the approximate solution (4.65)) is discontinuous. This takes place if the chosen basis
functions are piecewise linear, which is typical. The approach used in FEM is reducing
the order of derivatives from 2 to 1 with help of partial integration or the divergence
theorem. In general form:
I
Z
Z
(2)
Wı Ldiff u dΞ =
Ldiff (Wı , u) dΞ +
Ξ
Ξ
Wı Du d∂Ξ
(4.67)
∂Ξ
where Ldiff (·, ·) is a bilinear differential operator with first order derivatives only. The
last term on the right hand side integrates over the boundary ∂Ξ of the domain Ξ and
the operator D is a differential operator of first order as well (it is typically proportional
to the normal gradient at the boundary).
The boundary integral in (4.67) is evaluated by means of boundary conditions of the
second or third kind, which can be written in the general form as
rζ Du + q(1) u = q(0)
at part of ∂Ξ with 2nd or 3rd kind BCs,
(4.68)
where q(0) and q(1) are prescribed fields at the boundary and ζ equals 0 or 1 (dependent
on the specific form of the boundary condition). In case of the second kind boundary
conditions, q(1) equals zero.
4.6. AXISYMMETRIC MELT FLOW
63
Consequently, the equation system (4.66) transforms to:
Z
Ξ
q(1)
L(Wı , u) dΞ +
Wı ζ u d∂Ξ =
r
∂Ξ
I
Z
(0)
Wı s
I
dΞ +
Ξ
Wı
∂Ξ
q(0)
d∂Ξ,
rζ
ı ∈ {nodes},
where the bilinear operator
L(v, u) ≡ vLconv u − Ldiff (v, u) − vs(1) u
has been introduced for briefness. Substitution (4.65) yields a system of linear algebraic
equations with respect to the unknown coefficients uı :
X
∈{nodes}
Z
u
Ξ
q(1)
L(Wı , N ) dΞ +
Wı ζ N d∂Ξ =
r
∂Ξ
Z
I
q(0)
(0)
Wı s dΞ +
Wı ζ d∂Ξ,
r
Ξ
∂Ξ
I
ı ∈ {nodes}. (4.69)
The solution of the problem reduces hence to: 1) choosing appropriate basis and weight
functions and calculating the integrals, 2) solving the particular linear (or linearized)
system of equations (4.69) for one of the flow variables, and 3) iterating over the whole
(nonlinear) system of equations for all flow variables.
Choosing the weight functions equal to the basis functions, Wı = Nı , leads to the
standard Bubnov-Galerkin weak formulation. With convection-dominated problems,
i.e., when the nonlinearity is strong enough, the standard Bubnov-Galerkin FEM fails
if no stabilization is added to avoid non-physical oscillation of the solution. Artificial
addition of stabilization while using the Bubnov-Galerkin weight functions, however,
makes the problem statement inconsistent. Therefore it is preferable to introduce
the stabilization by changing the weight functions themselves, which is known as the
Petrov-Galerkin weak formulation. The Petrov-Galerkin weight functions Wı 6= Nı
can be viewed as perturbed Bubnov-Galerkin weight functions and the several possible Petrov-Galerkin approaches differ by the kind of perturbation used. One of
the most popular applications is the streamline upwind/Petrov-Galerkin stabilization (SUPG), which is constructed by adding streamline-upwind perturbations to the
Bubnov-Galerkin weight functions (see e.g. , ):
Wı = Nı + τ Lconv Nı ,
(4.70)
where τ is a stabilization parameter that weights the perturbation. Since according to
the weak problem formulation the perturbation is multiplied with the residual of the
64
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
differential equation, the consistency is fulfilled in that the exact solution also satisfies
the stabilized form exactly.
The stabilization parameter τ (denoted in what follows by τı , since it is, in general,
different for each weight function) determines the actual amount of stabilization and is
calculated with help of the coth-formula (also called the optimal stabilization formula),
which is derived from a simplified (1D) convection–diffusion model, see Section 4.6.7.
4.6.4
Basis functions and system matrix
When calculating the integrals in (4.69), it has to be taken into account that we work
with cylindrical coordinates in a 3D domain Ξ. Often, however, the term “calculation
domain” is also used to indicate the cross-section of the domain Ξ with one half-plane
(r, z) with r ≥ 0. Let us denote here this cross-section by S and its boundary by
Γ. The domain S is discretized i.e. subdivided in triangular elements Se such that
P
e Se = S, as described in Section 4.5.2. Each element has three nodes and each node
belongs to several elements. The nodes are connected by edges. Hence the boundary
Γ is subdivided in edges that connect the boundary nodes. The elements e that are
P
placed near the boundary Γ have got edges4 Γe on the boundary, such that e Γe = Γ.
For elements having no edges on the boundary, the Γe is an empty set (or zero).
According to the approach of linear FEM, we choose piecewise linear and localized
basis functions Nı , i.e., basis functions that are linear inside every element and have a
value 1 just at one node, with zero at all other nodes:

1 if  = ı
Nı (node ) =
0 if  6= ı.
(4.71)
This choice of basis functions implies that the coefficients uı in (4.65) receive the
meaning of nodal values of u.
Inside element e with nodes ı,  and k, the basis function Nı equals:
Nı (r, z) =
c ı + b ı r + aı z
,
2A
(4.72)
where A is the area of element e and the element-specific coefficients aı , bı and cı are
4
We assume here for simplicity of notation that there are no elements with more than one edge
lying on the boundary.
4.6. AXISYMMETRIC MELT FLOW
65
defined based on coordinates (rı , zı ) of the three nodes of the same element by



aı = r k − r 






b = z − zk


 ı
cı = r zk − rk z





ı 6= k 6= 





 1 (bı a − b aı ) = A > 0.
2
A consequence of the choice of basis functions Nı as local functions is that the weight
functions Wı (4.70) are local as well. Hence if splitting the integrals of (4.69) into
separate element integrals, the ı-th equation will only include non-zero integrals over
elements e that contain the node ı. Let us designate the set of such elements by e 3 ı.
Equation (4.69) can be rewritten:
Z
Z
X X
(1)
1−ζ
Wı q N r dΓ =
u
L(Wı , N ) rdrdz +
Γe
Se
e3 ı ∈{nodes}
X Z
(0)
Wı s
Z
Wı q
rdrdz +
r
1−ζ
dΓ ,
ı ∈ {nodes}.
Γe
Se
e3 ı
(0)
Another consequence of the locality of N is that L(·, N ) is local too. Hence the
integral over Se on the left hand side equals zero if the -th node does not belong to
the same element. The boundary integral on the left hand side behaves, of course,
similarly due to N in the integral. Concerning the weight functions (4.70), we follow
 and define the stabilization contributions only inside element interiors, setting
them to zero on the boundaries. Hence we replace Wı by Nı in the boundary integrals
and find the final reduced form of the equation (4.69):
Z
X X Z
(1)
1−ζ
u
L(Wı , N ) rdrdz +
Nı q N r dΓ =
e3 ı ∈ e
Se
Γe
X Z
e3 ı
(0)
Wı s
Z
rdrdz +
Se
Nı q
(0)
r
1−ζ
dΓ ,
ı ∈ {nodes}, (4.73)
Γe
or in matrix form:
XX
e3 ı ∈ e
Mı(e) u =
X
Bı(e) ,
ı ∈ {nodes}.
(4.74)
e3 ı
The matrices M (e) and B (e) are called the local (or element) matrices because the
indices are running over the three nodes of the element e only. Building the global
66
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
matrix of the system of linear algebraic equations includes thus calculating 9 matrix
(e)
(e)
elements Mı and 3 matrix elements Bı
4.6.5
for each element e.
Integration of diffusion terms and boundary conditions
In order to perform the integration, let us write down explicitly the diffusion terms
obtained by the transformation (4.67). For the temperature we have:
Z S
1 ∂
r ∂r
∂T
χr
∂r
∂
+
∂z
∂T
χ
∂z
Z
Wı rdrdz =
∂T ∂Nı ∂T ∂Nı
− χr
+
∂r ∂r
∂z ∂z
S
I
drdz +
χr
Γ
where the weight function Wı (cf. (4.70)) has been taken equal to:
∂Nı
∂Nı
Wı = Nı + τı urı
+ uzı
.
∂r
∂z
∂T
Nı dΓ, (4.75)
∂n
(4.76)
Here urı and uzı are the values of velocity components at the node ı. Such weight
function implies that the stabilization contribution is constant in each element and:
∂Wı
∂r
=
∂Nı
.
∂r
For the vorticity and azimuthal velocity the diffusion term is slightly different because
of the nature of these variables as ϕ-components of vectorial fields:
Z S
∂
∂r
ν ∂(ruϕ )
∂
∂uϕ
+
ν
Wı rdrdz =
r ∂r
∂z
∂z
Z
I
ν ∂(ruϕ ) ∂(rNı ) ∂(ruϕ ) ∂(rNı )
∂(ruϕ )
−
+
drdz + ν
Nı dΓ, (4.77)
∂r
∂r
∂z
∂z
∂n
Γ
S r
where, in order to eliminate the stabilization contribution from the diffusion term as
successfully as for the T -equation above, the following slightly modified weight function
has been chosen for the ω- and uϕ -equations (rı stands for the node value of r):
rı
W ı = Nı + τ ı
r
which implies that
∂(rWı )
∂r
=
∂(rNı )
∂r
∂Nı
∂Nı
urı
+ uzı
∂r
∂z
,
(4.78)
in each element.
The first integral on the right hand side of (4.77) can be transformed further to:
Z
Z ∂uϕ ∂Nı ∂uϕ ∂Nı
∂uϕ
∂Nı uϕ
− νr
+
drdz − ν
Nı + u ϕ
+ Nı drdz. (4.79)
∂r ∂r
∂z ∂z
∂r
∂r
r
S
S
4.6. AXISYMMETRIC MELT FLOW
67
In the stream function equation, there is no convection term and hence no streamlineupwind correction to the weight function: Wı = Nı . Consequently the diffusion term
becomes:
Z ∂ 1 ∂ψ
∂ 1 ∂ψ
+
Nı rdrdz =
r ∂r
∂z r ∂z
S ∂r
I
Z ∂ψ
1 ∂ψ ∂(rNı ) ∂ψ ∂Nı
+
drdz +
Nı dΓ, (4.80)
−
∂r
∂z ∂z
Γ ∂n
S r ∂r
where the first integral on the right hand side can be transformed further to:
Z Z
∂ψ ∂Nı ∂ψ ∂Nı
1 ∂ψ
−
+
drdz −
Nı drdz.
∂z ∂z
S ∂r ∂r
S r ∂r
(4.81)
Taking into account the form (4.72) of the basis functions Nı , the following approximations for the diffusion integrals in elements are obtained:
Z
aı a + b ı b 
T : −
Ldiff (Wı , N ) rdrdz = χr
4A
S
Z e
aı a + b ı b  b ı + b 
A
Ldiff (Wı , N ) rdrdz = ν r
+
+
(1 + δı )
ω, uϕ : −
4A
6
12r
Se
Z
aı a + b ı b 
b
ψ : −
Ldiff (Wı , N ) rdrdz =
+ ,
4A
6r
Se
where a bar above a variable stands for the average nodal value of the variable in
the chosen element (it coincides with the average value over the element area only for
variables that are linear coordinate functions):
in element Se :
X≡
1X
Xı .
3 ı∈ e
The boundary integrals like in equations (4.75) and (4.77) are calculated with help of
the second or third kind boundary conditions. As seen at the end of Section 4.6.2, we
have 2nd kind boundary conditions for the temperature and both 2nd and 3rd kind
boundary conditions for the azimuthal velocity. With using the denotation of (4.68),
the respective edge integrals are then written as follows:
∂T
T : DT = χ , ζ = 0, q(1) = 0
∂n
Z
L (0)
(0)
Nı q(0) rdΓ =
rı q + rq(0)
+
rq
ı
6
Γe
ν ∂(ruϕ )
uϕ : Duϕ =
, ζ=1
r ∂n
Z
L (0)
(0)
(0)
Nı q dΓ =
q + 2q
6 ı
ZΓe
L (1)
(1)
(1)
(1)
Nı q N dΓ =
q + q + 2δı q
,
12 ı
Γe
68
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
where L is the length of the edge Γe and a bar above a variable stands this time for
the average nodal value of the variable on this edge (hence averaging over two nodes
only):
on edge Γe :
X≡
1X
Xı .
2 ı∈ Γ
e
Both temperature and azimuthal velocity have also first kind boundary conditions. For
the vorticity and stream function, according to the introduced problem formulation,
the first kind boundary conditions even are the only ones existent. The treatment of
these boundary conditions is different from that above: the equations of (4.73) that
correspond to the boundary nodes ı with first kind boundary conditions are simply
rewritten with using explicitly the boundary value uBC
ı :
uı = uBC
ı ,
ı ∈ {nodes with 1st kind BC}
(4.82)
(the matrix elements for all u6=ı are set to zero).
4.6.6
Integration of convection and source terms
Since there is no convection term in the stream function equation, the weight function
for this variable is taken equal to the basis function. For the other variables, however,
we use the stabilized version of the weight function as shown above in (4.76) and (4.78):
r ζ ∂N
∂Nı
ı
ı
W ı = Nı + τ ı
+ uzı
,
urı
r
∂r
∂z
where ζ = 0 for temperature and ζ = 1 for the vorticity and azimuthal velocity. After
integration, taking into account (4.72), the convection terms have hence the form:
Z
Se
Wı Lconv N rdrdz =
Z
Z ∂Nı
∂Nı
ζ
Nı Lconv N rdrdz + τı rı
urı
+ uzı
Lconv N r1−ζ drdz =
∂r
∂z
Se
Se
r ζ (u b + u a )(u b + u a )
3 + rı /r
∂ψ
∂ψ
ı
rı ı
zı ı
rı 
zı 
a
− b
+ τı
r
.
24
∂r
∂z
r
4A
The elements near the symmetry axis need special treatment. In the elements whose
at least one node lies on the axis, the first part of the above expression is replaced by
Z
3 + rı /r ∂ψ 9 + 3r2 /r2 + 6rı /r + 2(rı /r)2 ∂ψ
Nı Lconv N rdrdz =
a
−
b .
24
∂r
120
∂z
Se
r→0
4.6. AXISYMMETRIC MELT FLOW
69
The derivatives of ψ in the above expressions are assumed constant inside every element
and are obtained from the three node values of ψ of that element, according to (4.65)
and (4.72), in the following way:
∂ψ
1 X
=
bı ψı ,
∂r
2A ı∈ e
∂ψ
1 X
=
aı ψı .
∂z
2A ı∈ e
(4.83)
The node values of the radial and axial velocity components are obtained after each
calculation of the stream function field by averaging the stream function derivatives
in the neighbouring elements:
, X
X 1 ∂ψ Ae
urı = −
Ae ,
r
∂z
e
e
e3ı
e3ı
, X
X 1 ∂ψ Ae
uzı =
Ae .
r
∂r
e
e
e3ı
e3ı
(1)
(1)
Let us now consider the source terms s(1) = s∗ + st . For the azimuthal velocity,
(1)
s∗ = −ur /r. The respective contribution to the system matrix is as follows:
Z
A ∂ψ
rı urı (urı bı + uzı aı )
−
Wı s(1)
(1 + δı ) + τı
.
∗ N rdrdz = −
12 r ∂z
6r
Se
For elements near the symmetry axis, the first term on the right hand side of the above
expression is replaced by
−
(3r + rı + r )A ∂ψ
(1 + δı ).
∂z
60 r2
(1)
For the vorticity, there is a similar source term, s∗
= ur /r, and consequently the
expressions of the integrals are analogous to the ones above but with the opposite
sign.
(1)
The inertial part of source term, st , is present for all variables excepting ψ. For the
azimuthal velocity and vorticity we have:
Z
(3r + rı + r )A
rı (urı bı + uzı aı )
(1)
−
Wı st N rdrdz =
(1 + δı ) + τı
.
60 ∆t
6 ∆t
Se
For temperature, the same expression is used but the stabilization part is replaced by
τı
(3r + r )(urı bı + uzı aı )
.
24 ∆t
And finally, we write down the contributions to the left side of the linear equation
(0)
(0)
system arising due to the source terms s(0) = s∗ + st .
70
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
(0)
For the stream function ψ we have s(0) = s∗ = ω and the respective integral equals:
Z
A
Wı s(0)
[3(3r + rı )ω + (3r + 2rı )ωı + 3rω] .
∗ rdrdz =
60
Se
(0)
For the vorticity ω, the s∗ -part of the source term is more complicated and equal to
(0)
s∗ =
Z
Se
2uϕ ∂uϕ
r ∂z
Wı s(0)
∗
− gβ ∂T
. The respective integral is expressed as follows:
∂r
∂uϕ gβ
∂T
A
(3uϕ + uϕı )
−
(3r + rı )
+
rdrdz =
6
∂z
2
∂r
τı rı (urı bı + uzı aı )
uϕ ∂uϕ gβ ∂T
−
r ∂z
2 ∂r
.
The derivatives of azimuthal velocity and temperature are assumed constant in elements and are calculated in an analogous way as the derivatives of ψ, see (4.83). For
elements near the symmetry axis, the first term on the right hand side of the above
expression is replaced by
"
A (3r + rı )uϕ ∂uϕ gβ
−
6
r
∂z
10
3r2 + 2rı2
3(3r + 2rı ) +
r
!
#
∂T
.
∂r
(0)
For the temperature and azimuthal velocity, there are no sources s∗ .
(0)
The inertial part of the source term, written in the general form as st
= uold /∆t,
yields the following integral for the temperature T :
Z
i
A h
(0)
3(3r + rı )T old + (3r + 2rı )Tıold + 3rT old +
Wı st rdrdz =
60∆t
Se
urı bı + uzı aı τı
3rT old + rT old .
8 ∆t
For the azimuthal velocity uϕ and vorticity ω, the expressions of the integral are similar
old
but T old is replaced by uold
, respectively, and the stabilization term is modified:
ϕ or ω
τı
urı bı + uzı aı
rı uold
ϕ
2 ∆t
(or with ω old instead of uold
ϕ , for the vorticity).
4.6.7
Stabilization parameter τ
The stabilization parameter τ , which is responsible for the appropriate weighting of
the amount of stabilization, is calculated in each element based on a formula derived
4.6. AXISYMMETRIC MELT FLOW
71
from a simplified equation in one dimension. Let us consider the one-dimensional
convection–diffusion equation for the scalar field y(x),
u
∂2y
∂y
= D 2,
∂x
∂x
which has the exact solution
y ex (x) = C1 exp
ux
+ C2 ,
D
where the constants C1 and C2 depend on the boundary conditions. Then it can
be shown (see e.g. ) that using the linear FEM and a uniform distribution of
nodes along x brings the nodally exact solution of the above equation if the following
stabilization parameter is applied:
∆x
1
τ=
coth(Pe) −
,
2|u|
Pe
where ∆x is the distance between nodes and Pe is the Peclet number defined by
Pe =
|u| ∆x
.
2D
Such definition of τ is often called the “optimal” in the literature. A more complicated
formula can be written for an irregular node distribution as well, the usage of the above
simple coth-law can, however, be well justified also in this case, since most important
part of the stabilization effect (the stabilization of the downstream node) will be in
both cases equal . Noteworthy, the stabilization parameter depends always only
on the relative positions of the next two nodes and is independent on the boundary
conditions, hence the definition of τ is local.
The above formula is used as approximation for the general case of more than one
dimension and arbitrary node or element distributions. For our specific case, the
stabilization parameter is introduced in the triangle elements:
he
1
τe =
coth(Pee ) −
,
2|ue |
Pee
where the element length in streamline direction, he , is used instead of ∆x, and the
Peclet number of element e is defined by
Pee =
|ue | he
.
2D
Here D stands for the respective diffusion coefficient, i.e., ν or χ, and the elemental
velocity ue comprises only the radial and azimuthal components:
p
1 ∂ψ
1 ∂ψ
|ue | = u2re + u2ze , ure = −
, uze =
,
re ∂z
re ∂r
72
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
where the derivatives of ψ are obtained according to (4.83).
The element length in streamline direction, he , can be calculated by using the functions
Nı (see (4.72)) of the three nodes of the element e:
!−1
X 1 ∂Nı
∂N
ı ure
he = 2
+ uze
.
|u
|
∂r
∂z
e
ı∈e
In order to ensure that one constant stabilization parameter is used throughout the
ı-th equation, we define the nodal value of stabilization parameter, τı , as the maximum
of the values of τe in the elements containing the considered node:
τı = max τe .
e3 ı
4.6.8
Numerical solution and coupling of all flow variables
The equation systems are build for each of the flow variables (ψ, T , uϕ and ω) as
shown above. Since each node interacts only with the neighbouring nodes and itself,
the matrices of the linear systems are sparse and the diagonal elements are nonzero. No
preconditioning is needed and the sparsity is used to speed up the process of iterative
solution and reduce the storage memory by introducing arrays of neighbouring node
indices for each node. These arrays define hence the positions of the nonzero matrix
elements at each row of the system matrix and allow skipping the large amount of
non-necessary arithmetic operations with zero elements.
The full solution of the axisymmetric fluid flow at a given time step includes a cyclic
recalculation of the four systems of equations: first we calculate the stream function,
which yields the radial and axial velocity components, then the azimuthal velocity
and temperature. At this point also the boundary conditions for the vorticity are
modified. At the last step, the vorticity itself is solved. The cycle is repeated until the
convergence is reached. Normally, with a small enough time step (typically 0.002 s),
only one such cycle per time step is needed, due to the good initial conditions (the
change of solution from one time step to another is small), and the calculation proceeds
for the next time step.
4.6. AXISYMMETRIC MELT FLOW
4.6.9
73
Test of the flow solver
The developed axisymmetric HD solver of FZONE was tested by comparing to another
axisymmetric HD solver FZHD (which uses also the ψ − ω formulation) developed in
the nineties by Prof. Muižnieks. The code FZHD solves hydrodynamics in the melt
with prescribed shape of boundaries and uses a somewhat different approximation
and numerical implementation as FZONE. Instead of the streamline upwind/PetrovGalerkin scheme, a simpler upwind approximation scheme with empirically chosen
weighting factor for the stabilization of the convective terms is used in FZHD. The test
calculations with FZONE and FZHD have shown :
• If calculating on similar triangular grids, the calculation results between FZONE
and FZHD differ. If refining the grid for FZHD, the results get equal. This is
explained by a higher numerical viscosity in FZHD, hence the choice of the stabilization parameter in FZONE is better.
• FZONE is more stable than FZHD if the grid is bad (i.e., the triangles are somewhere too stretched): the solution with FZHD diverges whereas FZONE just may
get a worse convergence. That FZONE does not diverge is explained by a better approximation of the integrals. This advantage of FZONE is important for
successful calculation of fluid flow with permanently deforming grid due to the
change of the shape of the floating zone.
Since the code FZHD has been compared earlier to the well-known commercial CFD
package FLUENT and the agreement was well, i.e., FZHD showed even better behaviour
than FLUENT5 , the above comparison between FZONE and FZHD was enough to conclude
that FZONE is in agreement with FLUENT as well.
5
FLUENT needed finer grid than FZHD to get the same solution, hence FLUENT had a higher numerical
viscosity, which could be related to the fact that FLUENT solves in the natural velocity–pressure
variables.
74
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
4.7
The surface-to-surface radiation model with view factors is modelled in FZONE mainly
following the recipes by Dupret et al. in  (the publication considers the Czochralski
growth) and including additionally a formalism in terms of “space node” for the case of
a non-closed radiative surface system, i.e., when the enclosing surfaces are left outside
the model, as preferred for floating zone modelling. Also the numerical implementation
of the radiation model is different from that described in .
4.7.1
Equations for an open radiative system
Introductory assumptions and relations
The following assumptions are used:
• Radiation is only diffuse. This approximation is supposed to work satisfactory
well because real solid surfaces are generally non-smooth.
• Surfaces are opaque. Emission, absorption and reflection of radiating waves only
occur at the surfaces of the bodies and not within the bodies themselves.
• Bodies are optically gray. The optical material properties are assumed temperature and wavelength independent in the whole spectrum.
According to the Planck’s law, the spectral emissive power ebλ (T ) of a black body (or
a perfect absorber) at the given temperature T and wavelength λ equals
ebλ (T ) =
λ5
2πC1
C
(e 2 /λT −
1)
,
where C1 = 0.595448 · 108 W µm4 m−2 and C2 = 14388 µm K. Integrating over the
whole spectrum yields the total power qb (T ) emitted by the black body per unit area,
Z ∞
qb (T ) =
ebλ (T ) dλ = σSB T 4 ,
0
where σSB = 5.67 · 10−8 W m−2 K−4 is the Stefan-Boltzmann constant. The total
power qe emitted by a non-black body per unit area is given by the expression
qe (x) = (x) qb (T (x)) = (x) σSB T 4 (x),
(4.84)
4.7. RADIATION MODELLING WITH VIEW FACTORS
75
where (x) 6 1 is the surface emissivity at a generic point x on the radiating surface.
Any surface element is emitting itself and meanwhile bombarded by waves coming
from the other surface elements. The incident heat flux qi (x) can either penetrate
the body or be reflected. The penetrating waves are totally absorbed by the opaque
surfaces. The absorbed heat flux equals
qa (x) = α(x) qi (x),
where α is the surface absorptivity. According to the Kirchhoff’s law for thermodynamic equilibrium in isothermal enclosure, the absorptivity and emissivity are equal.
Hence, the absorbed and reflected heat fluxes, qa and qr , are given by
qa (x) = (x) qi (x),
(4.85)
qr (x) = (1 − (x)) qi (x).
(4.86)
The total outgoing heat flux qo is the sum of the emitted and reflected fluxes:
qo (x) = qe (x) + qr (x)
= (x) σSB T 4 (x) + (1 − (x)) qi (x).
(4.87)
What one actually needs for the global heat exchange calculation is the net radiationcaused heat flux from the radiating surfaces, i.e., the difference between the outgoing
and incident fluxes:
q rad (x) = qo (x) − qi (x).
(4.88)
Using equations (4.87) and (4.88), the incident and outgoing fluxes at x are expressed
in terms of the net flux q rad (x):


qi (x) = σSB T 4 (x) −

q (x) = σ T 4 (x) −
o
SB
1
(x)
1−(x)
(x)
(4.89)
q
(x).
View factors
The total incident heat flux qi (x) is the sum of the contributions of the outgoing fluxes
qo (x∗ ) from all other points x∗ on the enclosure. If the system of surfaces is not closed,
the incident heat flux contains also the contribution from the space node.
Let dS and dS ∗ be infinitesimal areas at points x and x∗ . The fraction of the incident
flux on dS that leaves dS ∗ is calculated by
dqi (x) = K(x, x∗ ) · qo (x∗ ) dS ∗ ,
(4.90)
76
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
where K(x, x∗ ) is the surface view factor between x and x∗ . According to the Lambert’s cosine law for diffuse radiation, whenever dS and dS ∗ see each other, K(x, x∗ )
is given by the formula
K(x, x∗ ) = −
[(x∗ − x) · n][(x∗ − x) · n∗ ]
,
π[(x∗ − x) · (x∗ − x)]2
(4.91)
where n and n∗ are the unit normals to dS and dS ∗ (these are outer normals on the
surface of the radiating body). On the other hand, when dS and dS ∗ do not see each
other, K(x, x∗ ) vanishes:
K(x, x∗ ) = 0.
(4.92)
Hence the view factor K(x, x∗ ) is always symmetrical:
K(x, x∗ ) = K(x∗ , x).
(4.93)
Space node
Since Dupret et al.  consider the Czochralski process with full casing, a modification
has been made here by including additionally a formalism in terms of the so-called
space node in order to reduce the task and avoid calculating a fully closed radiating
surface system of the floating zone process. The space node characterizes the influence
of the surrounding space. It accumulates all the radiative heat flux not incident on the
explicit surfaces and does not reflect anything but radiates back as a black body with
an effective temperature, the ambient temperature Tamb . Hence, for the space node,
the outgoing radiation heat flux (4.87) reduces to
4
qo (space) = σSB Tamb
.
(4.94)
It is also assumed that a space view factor K space (x) may be defined so that it fulfills
two equations:
• The part of incident flux at point x that is supplied by the space node equals
K space (x) · qo (space).
This leads, if using (4.90), to the following total incident heat flux at x:
Z
qi (x) =
K(x, x∗ ) · qo (x∗ ) dS ∗ + K space (x) · qo (space),
(4.95)
x∗ ∈S
where S designates the whole radiating surface.
4.7. RADIATION MODELLING WITH VIEW FACTORS
77
• On the other hand, the integral incident flux onto the space node contributed by
a radiating surface element dS ∗ positioned at point x∗ equals
K space (x∗ ) · qo (x∗ ) dS ∗ ,
where qo (x∗ ) is the outgoing flux at x∗ . Adding the integrated contribution of
the same surface element dS ∗ over the whole surface S leads to the total outgoing
power from dS ∗ :
∗
∗
Z
[K(x, x∗ ) · qo (x∗ ) dS ∗ ] dS + K space (x∗ ) · qo (x∗ ) dS ∗ .
qo (x ) dS =
x∈S
Dividing both sides of the last equation by qo (x∗ ) dS ∗ leads to an integral relation the
view factors satisfy:
Z
K(x, x∗ ) dS + K space (x∗ ) = 1.
(4.96)
x∈S
The obtained equation (4.96) yields K space (x∗ ) for each x∗ ∈ S if the calculation
procedure of K(x, x∗ ) is known.
To write the integral equation for the net heat fluxes q rad (x), the expressions (4.89)
and (4.94) are substituted into (4.95):
−
(x)
Z
x∗ ∈S
1 − (x∗ )
K(x, x∗ ) q rad (x∗ ) dS ∗
(x∗ )
4
= σSB T (x) −
4
σSB Tamb
K space (x)
Z
−
σSB T 4 (x∗ ) K(x, x∗ ) dS ∗ .
x∗ ∈S
In the special case of a closed system, i.e., without free surrounding space, we have
K space (x) ≡ 0 and the above equation reduces to the 3D integral equation in .
Using (4.96) and (4.93), we obtain the final form of the 3D integral equation for an
−
(x)
1 − (x∗ )
K(x, x∗ ) q rad (x∗ ) dS ∗
∗)
(x
∗
x ∈S
Z
4
4
4
= σSB T (x) − Tamb −
σSB T 4 (x∗ ) − Tamb
K(x, x∗ ) dS ∗ . (4.97)
Z
x∗ ∈S
78
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
2D radiative integral equation and the axisymmetric view factor Kc
The next step is to take into account the axial symmetry of the radiating surface S.
Let r, θ and z denote the cylindrical coordinates of the point x and let p(S) stand
for the intersection of the axisymmetric surface S and the half-plane θ = 0. The
“axisymmetric view factor” Kc (x, x0 ) is defined then by the integral
Z π
0
Kc (x, x ) = 2
K(x, x∗ ) dθ∗
(4.98)
0
with the following x, x0 and x∗ given in Cartesian components:


x = (r, 0, z) ∈ p(S)



x0 = (r0 , 0, z 0 ) ∈ p(S)



x∗ = (r0 cos θ∗ , r0 sin θ∗ , z 0 ) ∈ S.
(4.99)
For each x ∈ p(S) we rewrite the integral equation (4.97) in the 2D form
Z
1 − (x0 ) 0
−
r Kc (x, x0 ) q rad (x0 ) ds0
0
(x)
(x )
x0 ∈p(S)
Z
4
0
4
4
= σSB T (x) − Tamb −
σSB T 4 (x0 ) − Tamb
r Kc (x, x0 ) ds0 , (4.100)
x0 ∈p(S)
where s is the curvilinear abscissa on p(S).
According to equations (4.93), (4.98), (4.99) and keeping in mind the invariance of
the system with respect to rotational transformations, it is easy to proof that the
axisymmetric view factors Kc (x, x0 ) obey the same symmetry rule as the 3D view
factors K(x, x∗ ):
Kc (x, x0 ) = Kc (x0 , x).
(4.101)
Considering the relation (4.96), there is an analogous rule for the axisymmetric view
factor, too. By using the equations
(4.93), i(4.96), (4.98), (4.99) and the identity
hR
R
R
2π
K(x, x∗ ) dS ∗ ≡ x0 ∈p(S) 0 K(x, x∗ )dθ∗ r0 ds0 , we obtain
x∗ ∈S
Z
r0 Kc (x, x0 ) ds0 + K space (x) = 1.
(4.102)
x0 ∈p(S)
Calculation of the axisymmetric view factor
In what follows, we keep the designations (4.99) considering x, x0 , x∗ and also introduce
the following expressions in Cartesian components for the respective unit normals n,
4.7. RADIATION MODELLING WITH VIEW FACTORS
79
n0 and n∗ (outer normals on the surface of the radiating bodies):


n = (cos φ, 0, sin φ)



n0 = (cos φ0 , 0, sin φ0 )



n∗ = (cos φ0 cos θ∗ , cos φ0 sin θ∗ , sin φ0 ),
(4.103)
where φ and φ0 stand for the polar angles of the vectors n and n0 , respectively, in the
plane θ = 0.
Introducing the vectors (4.99) and (4.103) into the equation (4.91), we can express the
dependence of K(x, x∗ ) on θ∗ :
K(x, x∗ ) = K̂(θ∗ ) =
(a0 + b0 cos θ∗ )(a00 + b00 cos θ∗ )
,
π (a + b cos θ∗ )2
(4.104)
where a, b, a0 , b0 , a00 , b00 only depend on r, z, r0 , z 0 , φ, φ0 (which are fixed) but not on θ∗ .
The explicit expressions are:



a






b





a0


b0






a00





b00
= r2 + r02 + (z 0 − z)2
= −2rr0
= r cos φ − (z 0 − z) sin φ
= −r0 cos φ
= r0 cos φ0 + (z 0 − z) sin φ0
= −r cos φ0
Integrating equation (4.104) with respect to θ∗ and taking into account that a2 > b2
leads to the primitive function I(θ) of K̂(θ∗ ):
Z
I(θ) =
θ
K̂(θ∗ ) dθ∗
0
r
= A θ + B arctan
!
sin θ
a−b
tan θ/2 + C
,
a+b
a + b cos θ
(4.105)
where coefficients A, B and C are functions of a, b, a0 , b0 , a00 , b00 . The expressions of the
coefficients (not given explicitly in  ) have been obtained as follows.
80
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
If r 6= 0, r0 6= 0 and x 6= x0 , then

b0 b00


A =


π b2





−a3 b0 b00 + 2 a b2 b0 b00 + a b2 a0 a00 − b3 a00 b0 − b3 a0 b00
p
B =2
2

π
b
(a + b) (a − b) (a + b) (a − b)






(a b0 − b a0 ) (a b00 − b a00 )

C = −
π b (a + b) (a − b)
If r0 6= 0 and x 6= x0 but r = 0 (which implies b = b00 = 0 ), then

a0 a00


A
=


π a2


B =0



00 0


C = a b
πa
If r 6= 0 and x 6= x0 but r0 = 0 (which implies b = b0 = 0 ), then

a0 a00


A
=


π a2


B =0



0 00


C = a b
πa
If x = x0 (which implies a + b = a0 + b0



A




B





C
= a00 + b00 = 0 ) or r = r0 = 0, then
a0 a00
=
π a2
=0
=0
To calculate the axisymmetric view factor Kc (x, x0 ) we need to know the range Θ of
values of θ∗ for which K(x, x∗ ) does not vanish:
K̂(θ∗ ) > 0
⇔
θ∗ ∈ Θ.
(4.106)
It is possible to characterize Θ as a set of intervals (θmı , θMı ) :
Θ=
[
ı
(θmı , θMı ),
0 6 θmı < θMı 6 π.
(4.107)
4.7. RADIATION MODELLING WITH VIEW FACTORS
81
According to (4.98), (4.104) and (4.105), knowledge of Θ allows to calculate the expected result:
Kc (x, x0 ) = 2
X
I(θMı ) − I(θmı ) .
(4.108)
ı
In order to obtain Θ, the values of θmı and θMı must be detected considering the viewed
and hidden parts of the radiating surfaces. It is done following closely the analytical
approach described in , which is based on the cylindrical symmetry of the system.
Since the procedure is complex and described well in the reference, the details are
omitted here.
4.7.2
Numerical implementation of the radiation model
Discretization of the integral equation
In order to obtain the distribution of the net radiation heat fluxes q rad (x) along the
radiating surface S with fixed distribution of temperature T (x), the equation (4.100)
is discretized and solved numerically as a system of linear equations by means of the
Gauss procedure.
The surface S is discretized to coaxial ring-type elements Sı , where ı represents the
element index. For the corresponding line segments p(Sı ), the length Lı and the midm
m
point xm
ı = (rı , 0, zı ) ∈ p(Sı ) is considered. Inside the ı-th element, the emissivity ,
the temperature T and the net radiation heat flux q rad are assumed constant and are
denoted by ı , Tı and qırad , respectively. The quantities qırad are the ones to be found
via the solution of the radiation equation (4.100), which is discretized by splitting
R
P R
the integrals x0 ∈p(S) into sums ı x0 ∈p(Sı ) . By writing the equation at each element
midpoint, a system of linear algebraic equations with respect to qırad is built up (index
ı runs over all elements):
X 1
X
4
[δı − (1 −  ) Vı ] · qrad = σSB
(δık − Vık )(Tk4 − Tamb
),


k
(4.109)
where δı is the Kronecker symbol and Vı is the designation for the integral over the
-th element:
Z
Vı =
x0 ∈p(S )
0
0
r0 Kc (xm
ı , x ) ds .
(4.110)
82
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Approximation of integrals and speed optimization
The building of matrix for the system of equations (4.109) includes calculation of the
axisymmetric view factors Kc (x, x0 ). Each calculation of a view factor contains a run
through all surface elements to detect the visible and hidden parts (see  ). Thus
there is a threefold run through all surface elements, which makes the matrix building
time-critical.
To reduce the necessary computational resources, the simplest approximation for the
integrals (4.110) is used, which is justified by a small size of the elements:
m
Vı ≈ L · rm · Kc (xm
ı , x ).
(4.111)
Due to the symmetry property (4.101) of the axisymmetric view factors, we actually
m
need to calculate only those view factors Kc (xm
ı , x ) with ı 6 . To reduce the amount
of necessary calculations to obtain the values of the view factors, different tricks related
to the algorithm detecting the visible and hidden parts have been used. So, during
m
calculation of a certain Kc (xm
ı , x ), we have to run through all the surface elements
and check if they are the “hiding elements”, i.e., if they partly or fully hide element
ı from element . It is possible, however, to use different strategies to decrease the
number of elements that have to undergo the control. For example, we exclude from
consideration as an eventual hiding element the elements whose z-coordinate is higher
or lower than both zı and z . We stop the control run after the first detection of a fully
hiding element. In this context much helps also a prior control of the elements ı and
, because they often are oriented in a way that one of them is a fully hiding element
itself.
The result of the used algorithm optimizations was a considerable reduction (about a
factor of 20) in the necessary computational resources for the view factors calculation
and building of the radiation matrix.
Test of precision
According to equations (4.102) and (4.110), the following equality holds:
X

Vı + Kıspace = 1,
(4.112)
4.8. COUPLING OF ALL MODELS IN FZONE
83
where
Kıspace ≡ K space (xm
ı ).
Using the identity (4.112), we can check the accuracy of the approximated integration
(4.111) by a similar method as done by Dupret et al. in . We verify the deflection
from 1 of the left-hand side of (4.112) in locations from which the surface element dS
may not see the space. In these locations the space view factor K space is zero. We
have detected the error level 3–4%, which can be regarded as very good in the context
of the reference work , where the authors notice errors even about 70–80%. They
have solved this problem by subdividing selected surface elements. Our good success
without the additional measures is obviously a consequence of the relatively small sizes
of the surface elements we use.
4.8
4.8.1
Coupling of all models in FZONE
The radiating surfaces include the surfaces of the inductor, which is kept cold by means
of cooling, and, eventually, one or several reflectors. In the present implementation,
however, the temperature field in these bodies is not calculated explicitly but the
inductor surface temperature Tind and the reflector surface temperature Trefl are taken
as fixed model parameters and applied for the radiation calculation, together with the
respective emissivity values εind and εrefl . Also the temperature of the open melting
front is fixed and equals the melting point temperature of silicon. The temperature
on the rest of the radiating surfaces has to be calculated by taking into account the
The previous description of the calculation of the net heat fluxes q rad (x) (see Section
4.7) included the distribution of the temperature T (x) at the radiating surfaces as
fixed parameters in the equations. To obtain the actual temperature distribution on
the surfaces where it is variable, the temperature calculation inside the silicon parts
and the radiation calculation have to be repeated several times. The view factors for
a constant geometry need meanwhile to be calculated only once.
Each of the separate temperature calculations in crystal, melt and feed rod is performed
iteratively. The calculation of temperature inside the melt in presence of convection
84
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
was described in details in Section 4.6. The calculation of the temperature in crystal
and feed rod is also performed with FEM but is simpler than the calculation in melt
since no fluid flow has to be calculated parallel to temperature and no stabilization
is needed (hence a simple Bubnov-Galerkin formulation can be used). Nevertheless,
the convection term due to the constant downwards movement of the crystal and feed
rod is taken into account. Also taken into account is the temperature dependence
of the thermal conductivity of solid silicon, which makes the temperature equation
non-linear. Another source of non-linearity (at the global level though) is the radiation heat exchange, which is taken into account as heat flux q rad (x) via boundary
conditions in each of the separate temperature calculation procedures. The coupling
of the temperature calculations in the separate parts of silicon and the global heat exchange via radiation is performed in an outer iteration cycle where the last calculated
temperature distribution is the input for the next radiation calculation and vice versa:
. . . → T(n) → q(n)
→ T(n+1) → q(n+1)
→ ...
If the intermediate results for temperature, T(n) , are calculated till a full convergence
of the temperature iterations in crystal and feed rod, then the outer iteration sweep
diverges due to the non-linearity of the global heat exchange. To avoid that, we
couple closer the temperature with the radiation fluxes by finishing the intermediate
calculation of T(n+1) in the crystal and feed rod as soon as the maximum allowed
change in temperature with the respective iteration process is reached, i.e., when
max |T(n+1) − T(n) | ≈ ∆max T(n) . The value of parameter ∆max T(n) is dependent on the
actual outer iteration. The starting value, ∆max T(0) , is a chosen constant, for example
5 K. In course of the outer temperature–radiation iterations the parameter ∆max T is
modified automatically in order to get a convergence. The following simple rule is used:
if the sign of max{T(n+1) − T(n) } is opposite to the sign of max{T(n) − T(n−1) }, then
let ∆max T(n+1) = 21 ∆max T(n) , otherwise let ∆max T(n+1) = ∆max T(n) . Such a treatment
avoids divergence and amplifying of the oscillations around the solution during the
temperature–radiation iterations, which is particularly important at the beginning
stages of calculation with the initial guess of temperature distribution strongly different
from the sought solution.
4.8. COUPLING OF ALL MODELS IN FZONE
4.8.2
85
Total calculation algorithm
the laboratory reference system) solution of phase boundaries is depicted in a simplified way in Fig. 4.15. The choice of a time step (called also the geometry time
step and having the typical order of magnitude 1 second) and moving of the fronts
(see Section 4.1) is followed by finding the new ITP location, which is coupled to the
EM field (Section 4.2) and the free surface shape (see Section 4.4). The new ITP is
found by minimization of DITP , the pressure imbalance at ITP. The following coupled
calculation of the temperature and radiation (see Section 4.8.1) yields the necessary
temperature gradients for the determination of the new front velocities. In the melt,
the temperature calculation includes also the calculation of the melt flow as described
in Section 4.6. The geometry time step is subdivided in smaller time steps (the hydrodynamics time step is typically only some milliseconds large) and a time dependent
flow is calculated. The relevant heat fluxes at the fronts are averaged over all hydrodynamics time steps in frame of the current geometry time step. Sometimes reasonable
studies of the phase boundaries can also be performed by neglecting the effect of the
melt flow in order to reduce the computational recourses needed (see one such study
in Section 5.2). For more accurate comparisons to measurements, however, the flow
effect can occur being important, as it is shown in Section 5.3.
If the new front velocities are very different from the old ones, the precision might
be low due to the geometry time step chosen and the calculation is repeated with a
smaller time step. Otherwise, the next step is made and the calculation proceeds.
Such repeating of the last geometry step is, however, only reasonable in case the
hydrodynamics is neglected.
As the solution approaches a steady state, the front velocities diminish. We assume
that the stationary solution is found when all velocity values fall below a predefined
convergence level. In case the melt flow has strong effect, it can though occur that
there is no real steady state at all, due to the time-dependent character of the flow,
and the shape of fronts will be oscillating about some average shape.
86
CHAPTER 4. AXISYMMETRIC MODEL OF PHASE BOUNDARIES
Figure 4.15: Simplified calculation scheme. The temperature calculation includes the
calculation of the melt motion in the floating zone.
4.8. COUPLING OF ALL MODELS IN FZONE
4.8.3
87
Zone height targeting by adjusting inductor current
It will be seen below in Sections 5.2– 5.3 that the most floating zone calculations have
as input parameter the zone height HZ , instead of the inductor current I. For targeting
the needed zone height, the following simple algorithm for the change of the inductor
current has been implemented in FZONE.
Before the calculation, the initial step of change of the electric current, ∆I(0) , has to be
chosen (a typical value could be 16 A). The adjustment of I during the calculation is
then performed along with the convergence check (cf. the control box “steady state?”
in Fig. 4.15) before going to the next time step.
Let us assume we have finished the n-th time step (n ≥ 1). Prior to modifying I, the
actual step of change ∆I(n) is calculated from the previous value, ∆I(n−1) . In doing
so, the values of the zone height at the actual moment, HZ(n) , and time step back,
HZ(n−1) , are taken into account and compared to the target value HZtarg . If
(HZtarg − HZ(n) ) · (HZtarg − HZ(n−1) ) < 0
then the zone height (as a function of time) is crossing the target. In this case the
step of change of I is reduced:
∆I(n) = max
∆I(n−1)
, ∆min I ,
2
where the value of ∆min I is a predefined constant (e.g., 1 A). In all other cases the old
step of change of I is kept: ∆I(n) = ∆I(n−1) . Hence: ∆I(n) ∈ [∆min I, ∆I(0) ] for all n.
The current I is only changed if the zone height is going away from the target:
|HZtarg − HZ(n) | > |HZtarg − HZ(n−1) |.
In this case the new value of the inductor current is calculated by
I(n+1) = I(n) + sign(HZtarg − HZ ) · ∆I(n) ,
where it has been taken into account that an increase in current is needed to augment
the zone height. If the above condition is not fulfilled, the old value of current is kept:
I(n+1) = I(n) .
Despite the simplicity, the targeting algorithm showed a very good performance.
88
5
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Calculation of phase boundaries
The models for the axisymmetric calculation of FZ phase boundaries and their implementation in the computation code FZONE were described in Chapter 4. In the present
chapter, actual calculations with FZONE are undertaken in order to study the phase
boundaries in an 8 inch FZ growth process and to make a comparison of the results
to experimental data.
5.1
Calculation example
To illustrate the way of functioning of the phase boundary calculation, let us consider as
example an 8 inch FZ crystal growth process and neglect, for simplicity, the melt flow.
The silicon properties are taken from Table 3.1. The emissivity of the open melting
front is assumed equal to εs (T0 ). The chosen inductor current I, crystal radius RCr ,
feed rod radius RF and other process parameters are summarized in Table 5.1. The
reflector is positioned like in Fig. 4.1, the main slit and three additional slits for the
HF inductor are considered as well like in Fig. 4.1. The effective width of each slit is
set 2 mm. The modelling parameter Imslit is assumed equal to 0.5.
The initial rectilinear geometry used is shown in Fig. 5.1 together with three successive stages of the convergence illustrating a typical calculation progress. The vectors
of the front velocities in the reference system of inductor, vn , are vanishing as the
solution approaches the steady state. The initial melt, crystal and feed domains are
triangulated as needed for the FEM calculation. In the course of calculation, the finite
element mesh is adapted in every step and the triangulation is repeated time by time
due to the strong changes in shapes of the domains. The final mesh and the obtained
steady-state phase boundaries and the temperature field are shown in Figs. 5.2–5.3.
The lines of magnetic field of the HF inductor are depicted in Fig. 5.2. Most of
them are crossing the inductor due to accounting of slits in frame of the axisymmetric
approximation. The vertical separator drawn inside the cross-section of the inductor
5.1. CALCULATION EXAMPLE
Parameter
89
Symbol
Value
Inductor current
I
1500 A
EM field frequency
f
2.8 MHz
RCr
102.0 mm
RF
77.5 mm
Single crystal pull rate
VCr
1.80 mm/min
VF
3.12 mm/min
Crystal rotation rate
ΩCr
5 rpm
Emissivity of inductor
εind
0.3
Emissivity of reflector
εrefl
0.3
Temperature of inductor
Tind
400 K
Temperature of reflector
Trefl
1000 K
Tamb
600 K
Feed rod push rate
Ambient temperature
Table 5.1: Calculation example: FZ process parameters and other input parameters.
marks the end of the additional slits. At larger distances from the center, the few field
lines still going through the inductor are due to the main slit. The influence of the
end of the additional slits on the shape of the open front can be observed.
The distribution of the net radiation heat flux density q rad at the silicon surfaces is
shown by the varying length of the vectors in Fig. 5.3. Steep change in q rad takes place
at the inner and exterior triple points due to the different emissivity of the liquid and
solid phases. A slight influence of the reflector may be observed in the net radiation
flux from the crystal and the temperature field inside the crystal.
The numerical solution of the ITP region and the respective finite element mesh in the
melt and feed are in view in Fig. 5.4. The inner edge of the inductor shows the scale
in Fig. 5.4(a). An even closer view of the finite element meshes in the ITP vicinity is
demonstrated in Fig. 5.4(b). These two pictures display the smooth transition “melting
interface—open front”, which, however, does not seem smooth in large scale, e.g. in
Fig. 5.2. Since we use approximate model of ITP, the large-scale image (like Fig. 5.2)
should be considered as the result of the ITP calculation while Figs. 5.4(a) and 5.4(b)
mostly reflect the numerical approach.
90
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Figure 5.1: Calculation progress: the triangulated starting geometry and 3 successive
stages of the convergence to a steady state. Shown are also the vectors of the front
velocities vn .
5.1. CALCULATION EXAMPLE
91
Figure 5.2: Steady state solution: the temperature isolines in the melt with step 2.9 K
(maximum 1745 K) and the magnetic field lines. Shown is also the finite element mesh
in the crystal and feed rod.
Figure 5.3: Steady state solution: the temperature isolines with step 10 K in the
crystal and feed and the vectors showing the magnitude of q rad at the silicon surfaces.
Shown is also the finite element mesh in the melt.
92
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
(a)
(b)
Figure 5.4: The inner triple point and its triangulated vicinity in the melt and feed
rod.
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
5.2
93
Numerical study without melt flow
In this section, we use FZONE to study numerically the qualitative and quantitative
relationships between the various growth process characteristics as well as explore
the limits of the process parameters allowing the existence of a steady-state floating
zone. The existence of the floating zone is considered with the focus on having a
permanent liquid bridge between the feed melting front and the crystallization front.
It is ensured by a sufficient melting of the feed rod, especially of the central part of it,
and by avoiding a breakdown of the neck of the liquid zone, i.e., by the existence of a
stationary free melt surface.
We neglect at this stage the convective heat transfer due to the melt motion in the
molten zone and concentrate our attention on the other factors forming the zone
shape. This approximation is justified by the existence of many flow structures of
practical relevance (which can be created, e.g., by different ways of crystal rotation)
that influence the phase boundaries negligibly. Consideration of the influence of flow
on the zone shape and comparison with concrete measurement data is the subject of
Section 5.3.
We consider 8 inch FZ silicon crystal growth. The reflector position as well as the main
slit and the three additional slits of the HF inductor are considered like in Fig. 4.1. The
most relevant process parameters for the reference configuration are listed in Table 5.2,
for the rest of parameters see Section 5.1. The material properties of silicon used in
the calculations were given in Section 3.1. The chosen growth system configuration is
taken as the starting-point for the study of the influence of different modifications.
The steady-state phase boundaries, the temperature field and the lines of magnetic field
of the high-frequency inductor for the reference configuration are shown in Fig. 5.5.
5.2.1
Zone height and inductor current
A significant FZ process parameter is the height of the zone, HZ , i.e., the distance along
the vertical between the edge of the feed rod and the exterior triple point (ETP), at
which the exterior surface of the single crystal is adjoined by the free surface of the
melt. In the example in Fig. 5.5, the zone height is HZ = 37 mm. It is possible to
adjust the zone height by changing the inductor power and keeping all other process
parameters constant. That is illustrated in Fig. 5.6 showing the phase boundaries
94
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Parameter
Symbol
Value
Inductor current
I
1510 A
EM frequency
f
2.8 MHz
RH
16.5 mm
Lslit
36 mm
Rslit
52.5 mm
= RH + Lslit
RCr
102.0 mm
RF
77.5 mm
Single crystal pull rate
VCr
1.80 mm/min
VF
3.12 mm/min
Feed rod push rate
Table 5.2: Parameters of the chosen reference configuration (some other model parameters see also in Section 5.1).
end here
1687 K
HZ
HM
1745 K
H Cr
1687 K
Figure 5.5: The temperature isolines in the melt (∆T = 58 K) and the magnetic field
lines for the reference configuration. The zone height HZ = 37 mm, the crystallization
interface deflection HCr = 48 mm and the melting interface deflection HM = 4 mm.
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
1610 A
95
1410 A
1610 A
1410 A
1610 A
Figure 5.6: Phase boundaries with different zone heights corresponding to inductor
current values from 1410 till 1610 A with step 50 A. The thick phase boundary lines
correspond to the reference case with 1510 A and HZ = 37 mm.
calculated for different inductor current values. The reference case with the current
1510 A and zone height 37 mm is shown with a thick line. The inductor current has
been changed up to 1610 A and down to 1410 A, i.e., only ±100 A or ±7% of the
reference current value. On both ends of the change area, the further change was
limited by physical reasons. So a further lifting of the current above 1610 A (say to
1660 A) leads to a cutting of the liquid zone neck. The disconnection of the upper and
lower part of the growth system prohibits a stable growth process. On the other hand,
if the inductor current falls below 1410 A, then the distance of the inductor to the
open melting front and meniscus becomes critical. This is seen also in Fig. 5.7. The
zone neck radius RN of the liquid floating zone approaches the inductor hole radius
RH as the current value diminishes. The other curve on Fig. 5.7 shows the zone height
as a function of the inductor current I. The curve HZ (I) is linear and it is explained
by the relatively small change of I.
The calculated region around the inner triple point in three cases with very high values
of I, implying large zone heights, is treated in more detail in Fig. 5.8. Despite the
numerical algorithm of the triple point calculation, which smoothes the angle between
the melting interface and open melting front, a sharp solid rim can be seen at ITP.
Although these modelling limitations hinder obtaining a more precise picture of ITP,
the calculation result agrees well with the tendency known in practice: uncontrolled
96
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
50
f(I), mm
HZ (I)
40
30
20
RH
R N(I)
10
0
1410
1460
1510
1560
I,
A
1610
Figure 5.7: The zone height HZ /mm = 62.3 · I/kA + 56.9 and the zone neck radius
RN as function of the inductor current I. The inductor hole radius RH is shown too.
Feed
ITP
1590 A
Melt
1610 A
1630 A
Figure 5.8: The calculated inner triple point in case of very high inductor current: I =
1590 A, 1610 A, 1630 A.
growth of sharp pikes (“noses”) occurs at ITP in case of the zone height being too
large .
As discussed above, the change area of the inductor current allowing the existence of
a steady-state floating zone constitutes only about ±7% of the absolute current value.
Although the power supply from the vacuum tube HF generator to the inductor and
the corresponding current value can be altered monotonically, e.g. with the power
supply from DC circuit, the spatial distribution of the HF current density on the
surfaces of current suppliers and other parts of the oscillation circuit makes it difficult
in praxis to measure the absolute value of the HF electric current precisely enough
concerning that high growth system sensibility. Hence it is reasonable to use the zone
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
97
height HZ as the control parameter of the process by relative changing of inductor
current to meet the target value of HZ . In the following numerical studies, we adjust
appropriately the inductor current I to keep the zone height constantly at 37 mm.
5.2.2
Reflector
A side reflector (see the example in Fig. 4.1) is used in praxis to reduce the temperature gradient and thermal stress in the crystal where high temperature differences
arise, particularly due to the large diameter of the crystal. In our calculation model,
we assume the silver reflector being slitted to avoid eddy currents, hence the magnetic
field lines are freely crossing the reflector as shown in Fig. 5.5. The comparison of the
phase boundaries with and without reflector is given in Fig. 5.9. The case with reflector positioned low is the reference configuration as shown in Figs. 4.1 and 5.5 with
inductor current 1510 A. In case with reflector positioned high, the reflector has been
shifted upwards so that the top edge of the reflector is approximately at the height
of the exterior triple point (ETP). In this case the inductor current is only 1460 A.
Without any reflector a much higher current (1600 A) is necessary in order to maintain
the same zone height. It is explained by the action of the reflector as a passive heater.
Another effect of the reflector is seen on the temperature field in the crystal center
where the heat flux from the crystallization interface has to find a long way down to
the lower edge of the reflector in order to radiate away through the free end of the
mono-crystalline ingot. Hence the presence of a reflector reduces not only the radialbut also the axial gradient of temperature in the crystal. Consequently, the deflection
of the crystallization front, HCr , becomes larger to ensure the balance of heat fluxes at
the phase interface. The calculation shows that without reflector the axial temperature gradient on the crystal axis near the phase boundary is about 8.7 K/mm whereas
with the low reflector, 7.3 K/mm only. Obviously the change in the temperature gradient has not been fully compensated by the deflection of the crystallization interface,
because the lowering of the inductor power to preserve the zone height diminishes the
necessary augmentation of the crystallization interface deflection by reducing the heat
flux from the melt. Indeed, the axial temperature gradient in the melt center near
the phase boundary is about 1.0 K/mm and 0.56 K/mm without reflector and with
the low reflector, respectively. The maximum temperature difference in the melt is
reduced from 71 K (without reflector) to 58 K (with the low reflector) or even to 45 K
(with the high reflector). Also the increase in the deflection of the melting interface,
98
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Without reflector
Low reflector
High
Without reflector
reflector
Low reflector
Long reflector
Figure 5.9: Phase boundaries with the reflector positioned low or high, without the
reflector or with a prolonged reflector.
Reflector
I, A
∆T , K
HCr , mm
HM , mm
no
1600
71
35
2.2
low
1510
58
48
3.8
long
1460
45
45
8.6
high
1460
45
43
8.9
Table 5.3: Different reflectors (HZ = 37 mm).
HM , is explained by the reduction of the inductor power when applying a reflector.
Beside the low and high reflectors, a third example considered in Fig. 5.9 is a prolonged
reflector whose top edge coincides to that of the high reflector while the lower edge,
to that of the low reflector. Since the local action of the long reflector in the vicinity
of ETP is similar to that of the high reflector, the inductor power and the melting
interface are not changed significantly by replacing the high reflector by the long one.
The crystallization front, however, gets deflected slightly more than with the shorter
reflector (see Fig. 5.9). Hereby we see the pure effect of the reflector’s lower edge
height, without change of the inductor power.
The calculation results with different reflectors are summarized in Table 5.3: ∆T
stands for the maximum temperature difference in the melt, HCr , for the crystallization
interface deflection and HM , for the melting interface deflection (as defined in Fig. 5.5).
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
5.2.3
99
Pull rate
The pull rate of crystal is one of the most important FZ process parameters. During
the study of the zone shape at different growth rates the feed push rate was adjusted
to satisfy the steady-state FZ process condition:
2
VF RF2 = VCr RCr
.
(5.1)
The phase boundaries corresponding to the reference case with VCr = 1.8 mm/min are
shown with the thick line in Fig. 5.10, the other lines correspond to different growth
rates. Table 5.4 shows the change of some parameters including the floating zone neck
radius, RN , and the height of the free bulk liquid surface, HL , which is defined as
the vertical distance between ETP and ITP. The inner triple point, which delimits
the melting interface from the open melting front, has no exactly defined location in
frame of the fluid film model and the values of HL have an accuracy threshold below
0.5 mm. Since HL depends strongly on the free surface angle at ITP, we also use
another characteristic quantity, the height of the zone neck, HN , which is defined as
the vertical distance between ETP and the zone neck’s thinnest place, where the free
surface is vertical. HN is dependent on the physical properties of the melt as well as
on the crystal size and neck radius determined by the inductor and feed.
The smaller the pull rate, the smaller the deflection of the crystallization front and
the higher the position of the melting interface. There exists a lower limit between 0.6
and 0.8 mm/min below which no steady-state floating zone for the considered 8 inch
process with the fixed zone height is possible. At that small pull rates, the melting
front stays above the inner edge of the inductor and enlarges the height of the free bulk
liquid surface, HL . If a critical value of HL (slightly above 18.5 mm) is exceeded, the
zone neck collapses due to the effect of surface tension. Nevertheless, the lower limit
of the pull rate depends substantially on the inductor and zone height. For example,
a stable free melt surface at a pull rate of only 0.1 mm/min can be made possible,
according to calculations, by means of enlarging the inductor hole diameter by 20 mm
and reducing the zone height to 33 mm, which helps to diminish the increase in HL .
Although HL reaches 19.5 mm (and HN reaches 16.5 mm) in that case, the free melt
surface stays stable due to a large neck radius (RN exceeding 22 mm), which heightens
considerably the critical value of HL .
With high pull rates, the deflection of both the crystallization and melting interfaces
increases. Especially the melting interface becomes steep. Despite the shape of the
100
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
0.8 mm/min
2.8 mm/min
0.8 mm/min
2.8 mm/min
Figure 5.10: Phase boundaries at different crystal pull rates from 0.8 till 2.8 mm/min
with step of 0.2 mm/min.
VCr (VF ),
mm
min
I, A
∆T , K
HCr , mm
HM , mm
RN , mm
HL (HN ), mm
0.8 (1.39)
1510
80
31
-1.1
7.3
18.5 (15.9)
1.2 (2.08)
1510
71
36
0.2
9.2
18.1 (16.0)
1.6 (2.77)
1510
62
44
2.1
10.3
17.1 (16.1)
1.8 (3.12)
1510
58
48
3.8
10.7
16.6 (16.1)
2.0 (3.46)
1510
54
54
6.3
11.0
16.1 (16.1)
2.4 (4.16)
1515
46
67
15
11.5
16.2 (16.2)
2.8 (4.85)
1525
40
84
33
11.9
15.9 (15.9)
Table 5.4: Different crystal pull rates (HZ = 37 mm).
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
101
melting interface, the distance between the deepest point of the melting interface and
that of the crystallization interface is increasing with pull rate, in the considered area of
pull rates. Apart from the practical issues leading to crystal dislocation and cracking if
grown at too high speed with too steep crystallization front (as happens already above
2 mm/min), the limiting factor would be here the approaching of the open melting
front to the inductor, which does not melt the feed rod fast enough if the zone height is
fixed (see Fig. 5.10 showing the distance between the feed rod and inductor decreasing
with growth rate). The problem could be overcome by heightening the inductor power
and zone height appropriately. Another and unavoidable upper limit of the pull rate is
set by the total ability of the crystal surface to radiate the heat away. The maximum
growth rate can be achieved and the maximum heat can be emitted by the solid crystal
surface at the melting point temperature, i.e., when the crystallization interface nearly
coincides with the exterior surface of the crystal (a thin “nutshell” of crystal is left
over).
It is interesting that the zone height stays practically constant when reducing the pull
rate (and the feed push rate) at a constant inductor power. Hence the calculations
with fixed zone height for the pull rates about and below 2 mm/min correspond to the
inductor current 1510 A (see Table 5.4). At higher pull rates, a slightly heightened
inductor power was necessary, e.g., the case of 2.8 mm/min corresponds to I = 1525 A.
5.2.4
Single crystal diameter
FZ process development toward a larger single crystal size usually requires serious
modifications of the whole growth system including the HF inductor. Nevertheless,
for the purpose of illustration, we can consider here the zone shape with different
crystal diameters from 4 to 8 inches by keeping the inductor, the zone height and
the pull rate of the 8 inch process configuration. The reflector is removed to avoid
interference of different effects. We change the feed push rate, to satisfy the condition
(5.1), as well as the inductor power, to fuse the feed at the respective rate and keep
the zone height constant.
As seen in Fig. 5.11, the deflection of the crystallization interface is changing most
dramatically. The untypical convex crystallization front about the center of the 4 inch
zone is explained by the effect of the relatively long additional slits of the actual inductor reducing the ratio of the heat supply in the central part to the heat supply in
102
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
RCr , mm
VF ,
mm
min
I, A
∆T , K
HCr , mm
RN , mm
HL (HN ), mm
51
0.78
1060
26
0
9.0
17.6 (16.7)
76
1.73
1305
44
13
9.8
17.2 (16.3)
102
3.12
1600
71
35
10.3
17.5 (16.1)
Table 5.5: Different single crystal sizes (VCr = 1.8 mm/min, HZ = 37 mm, no reflector).
26 K
44 K
DT = 71 K
Diameter 4 in
6 in
8 in
Figure 5.11: Phase boundaries and the maximum temperature difference ∆T in the
melt for FZ processes with different crystal diameters (in all cases the zone height is
37 mm, the inductor is the same and no reflector is applied).
the periphery of the molten zone. Beside the deflection of the crystallization front, as
a consequence also the maximum temperature difference in the melt, ∆T , increases
rapidly with crystal diameter: the heat flux from the free melt surface has to be conducted through a larger molten zone. Table 5.5 summarizes some calculation results
obtained with different crystal radii, RCr , including the total height of the free melt
surface, HL , and the height of the zone neck relative to ETP, HN , as defined previously. We see that HN , which was practically independent on the pull rate (see back
Table 5.4), decreases monotonically with crystal radius, whereas HL changes in a more
complicated way and is, for 8 inch zone, higher than in the case with reflector. The
value of HL stays however always (according to Tables 5.4 and 5.5) below the Heywang
limit for crystal and feed of strongly different diameters (see Section 2.2).
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
RF , mm
VF ,
mm
min
103
I, A
∆T , K
HM , mm
93.0
2.17
1580
58
1.4
77.5
3.12
1510
58
3.8
62.0
4.87
1440
58
12
46.5
8.66
1395
56
39
Table 5.6: Different feed rod sizes (HZ = 37 mm, VCr = 1.8 mm/min).
31 mm
93 mm
93 mm
31 mm
(transient state)
Figure 5.12: Phase boundaries with feed rod radii form 93 mm till 31 mm. No stationary melting interface is possible with a feed rod radius of only 31 mm.
5.2.5
Feed rod diameter
The size of the feed rod enters the relation (5.1) and determines the feed supply speed
needed to grow the fixed-diameter single crystal with a given pull rate. In Fig. 5.12, a
series of calculation results with different poly silicon rods is shown. The feed diameter
has been changed from 186 mm down to 62 mm with a step of 31 mm. The pull rate
VCr = 1.8 mm/min is kept unchanged. The smaller the feed rod diameter, the larger the
feed push rate VF and the deeper the melting interface deflection (see also Table 5.6).
It is seen that a too small feed rod size makes the steady state growth impossible and
a solid bridge is built between the feed and the grown crystal. The reason is the high
(about 19.5 mm/min for RF = 31 mm) supply rate of the feed, which can not be fused
fast enough in the central part.
104
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
33 mm, small zone height
63 mm
63 mm
43 mm
Figure 5.13: Phase boundaries obtained with varied length of the additional slits:
Rslit = 62.5; 52.5; 42.5 mm (HZ = 37 mm) and Rslit = 32.5 mm (HZ = 35 mm).
RH , mm
Lslit , mm
Rslit , mm
I, A
∆T , K
HCr , mm
HM , mm
RN , mm
= RH + Lslit
16.5
26
42.5
1600
73
53.7
-0.4
7.1
16.5
36
52.5
1510
58
48.4
3.8
10.7
16.5
46
62.5
1435
46
40.3
25
12.3
Table 5.7: Different inductor slit lengths (HZ = 37 mm).
The upper limit of the feed rod diameter is determined by the ability of the inductor
to ensure a sufficient slope everywhere at the open melting front so that the melt flows
constantly to the center and no accumulation and dropping of the melt occurs.
5.2.6
Inductor modifications
The dimensions and shape of the inductor have a crucial role in the performance of the
FZ growth process. Here we consider the effect of the inductor hole size and the length
of the additional slits. Both the increase of the inductor hole and the lengthening of the
slits reduce the induced power around the central part and shift the power maximum
on the free melt surface further outwards.
The phase boundaries shown in Fig. 5.13 demonstrate the effect of varied length of
5.2. NUMERICAL STUDY WITHOUT MELT FLOW
105
Small hole
Large hole
Small hole
Figure 5.14: Phase boundaries obtained with varied radius of the hole of inductor:
RH = 14.0; 16.5; 19.0 mm. To simplify the figure, the case RH = 21.5 mm of Table 5.8
is not shown here.
RH , mm
Lslit , mm
Rslit , mm
I, A
∆T , K
HCr , mm
HM , mm
RN , mm
= RH + Lslit
14.0
36
50.0
1560
63
50.4
0.8
7.6
16.5
36
52.5
1510
58
48.4
3.8
10.7
19.0
36
55.0
1465
54
46.0
9.2
13.3
21.5
36
57.5
1420
50
42.9
22
15.9
Table 5.8: Different inductor hole sizes (HZ = 37 mm).
the additional slits (see also Table 5.7). The slit length is reduced from Lslit = 36 mm,
which is the reference configuration (Rslit ≈ 53 mm), to Lslit = 26 mm (Rslit ≈ 43 mm)
and a steady-state solution is obtained. Another reduction of the slit length by 10 mm
leads to cutting of the zone neck at the defined zone height of 37 mm. It is, however,
possible to obtain a steady-state zone with that short slits at a smaller zone height of
35 mm (see the thin phase boundary lines in Fig. 5.13). It is theoretically possible to
remove the additional slits at all and to compensate the decrease of the zone neck radius
by a further reduction of the zone height (cf. Fig. 5.6) but it leads to a substantial
change of the open front’s slope, which may cause dropping of the liquid onto the
inductor from the insufficiently sloped surface.
106
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Increasing the length of the additional slits till Lslit = 46 mm (Rslit ≈ 63 mm) leads
to a strongly deflected melting interface as well as reduced crystallization interface
deflection, due to the reduced inductor power. A further increase of the slit length
by 10 mm does not yield any stationary solution, as the melting front meets the
crystallization front.
Another possibility to change the power distribution and the neck radius considerably
is the variation of the inductor hole size (see Fig. 5.14 and Table 5.8), which, however,
does not impact remarkably the open melting front, excepting the neck region. The
length of the additional slits has been left unchanged. Like in case of the slit length
variation, the lower and upper limits of the inductor hole size are determined by cutting
of the zone neck and the melting interface deflection, respectively. That demonstrates
the necessity for a needle-eye inductor.
5.2.7
Frequency
According to the equations (3.1) and (3.14), the EM field frequency f influences directly the integral surface density of the induced power:
r
q EM ∝
f 2
i ,
σ ef
(5.2)
where σ is the electrical conductivity of the solid or liquid silicon and ief , the local
effective surface current, which depends on the inductor current I. Hence increasing f
results in higher q EM if not compensated by a reduction of I. A more complicated effect
of the frequency takes place at the open melting front, which is covered, according to
the assumed model, by a thin fluid film. The higher the frequency, the larger the part
of the electric current induced inside the liquid film. Due to the different electrical
conductivities of the liquid and solid silicon, the total heat amount depends on the
ratio of the fluid film thickness and the EM skin layer depth. These effects are taken
into account in the mathematical model and produce the results illustrated in Fig. 5.15
where the phase boundaries corresponding to the reference frequency and a 4 times
higher frequency are shown. In order to keep the zone height unchanged, the inductor
current is reduced from 1510 A in the reference case to 1160 A in the high-frequency
case. We see that due to the change of the placement of the open melting front and
the subsequent redistribution of the surface currents i2ef , the necessary decrease of the
inductor current I could not be estimated precisely enough by the expression (5.2).
5.3. INFLUENCE OF MELT FLOW AND ITS VERIFICATION
107
2.8 MHz
11.2 MHz (1160 A)
2.8 MHz (1510 A)
Figure 5.15: Influence of a 4 times higher EM frequency on the phase boundaries.
If not counting the strong changes in the inductor current, the influence of the EM
frequency on the phase boundaries is weak and the frequency change considered in
Fig. 5.15 has been chosen very large in order to see that influence good enough. For
real FZ growth, however, the frequency might not be changed in a so wide range
without disturbing the process performance. A high frequency necessitates a high
voltage at the inductor and increases the risk of arcing with subsequent EM field
breakdown. On the other hand, the frequency must stay high enough to ensure a
small field penetration depth into silicon (i.e., the skin effect) and consequently a
stable melting of the feed rod. A too low frequency leads to heat generation deep in
the solid, leaving the surface cold and deteriorating the melting process.
5.3
Influence of melt flow and its verification
The above study in Section 5.2 was performed without taking into account the melt
flow. This was justified by the wish to focus attention on the pure effect of other
parameters, whereas the effect of melt flow can vary depending on the rotation of the
crystal, which would make due to the additional degrees of freedom (the art of crystal
rotation) the above parameter study too immense and resources consuming. In some
cases, it can even be justified to neglect the effect of melt flow at all (e.g., it was stated
in  that the melt flow has only little influence on the phase boundaries). The
present axisymmetric flow calculations with FZONE show, however, that the flow can
108
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Figure 5.16: The photo-scanning resistivity measurement in the vertical cross-section
of an 8 inch FZ crystal (Siltronic AG) has been performed at the Institute of Crystal
Growth .
also have a significant influence on the phase boundaries, particularly on the shape of
the crystallization front, which is characterized, for simplicity, by its deflection HC .
The melt flow effect is illustrated here for two cases, in which the calculations without
hydrodynamics yield a crystallization interface deflection significantly different from
the measured one, and for one case where the hydrodynamic influence is small. The
respective interface forms have been determined from the photo-scanning resistivity
measurements in the vertical cross-section of the grown crystal .
5.3.1
FZ 8 inch process
The first example is an 8 inch floating zone. The measured (see Fig. 5.16) deflection of
the crystallization interface is about 44 mm, whereas the calculation without account
of hydrodynamics yields a deflection of about 50 mm. Hence the flow calculation
was used to explain the difference. The flow showed a time-dependent character, see
Fig. 5.17 for the fluctuations of the maximum and minimum values of the stream function, characterizing the intensity of the flow vortices in one or the opposite direction,
respectively, and the maximum of the melt temperature. Due to the mixing of the
fluid, the latter is significantly lower than the characteristic temperature maximum in
calculation without hydrodynamics (see, e.g., the value of ∆T = 58 K in Fig. 5.5).
As can be observed from the frames shown in Fig. 5.18, the time dependence of the
distributions of the stream function and temperature is particularly strong in the
peripheral part of the molten zone, i.e., in the region near the exterior triple point,
5.3. INFLUENCE OF MELT FLOW AND ITS VERIFICATION
109
stream func. extremes (10-6 m3/s)
20
15
10
5
0
-5
-10
-15
-20
0
200
400
600
800
1000
1200
1400
1000
1200
1400
time (s)
max relative temperature (K)
52
50
48
46
44
42
40
38
36
34
0
200
400
600
800
time (s)
Figure 5.17: The calculated fluctuations of the maximum and minimum values of the
stream function (the upper figure) and the maximum of melt temperature relative to
the melting point, ∆T (the lower figure).
110
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Figure 5.18: Isolines of the stream function (left) and temperature (right) in the melt
in four successive time instants with interval of 0.5 s. (The transient flow calculation
was performed with a much smaller time step of 2 ms.)
5.3. INFLUENCE OF MELT FLOW AND ITS VERIFICATION
111
Calculation with HD
The measured
crystallization front
Calculation without HD
Figure 5.19: Comparison of the FZ 8 inch phase boundaries calculated with hydrodynamics (thick lines) to the measured crystallization interface (thin line) and to the
calculated interface without taking into account the melt flow (the thin line with larger
deflection).
where the Marangoni force tries to build a vortex with a movement towards ETP
along the free melt surface, whereas the electromagnetic force acts in the opposite
direction. This unstable vortex structure in the peripheral part of the zone has an
influence on the deflection of the crystallization interface, which consequently shows
a fluctuating character too. Since the melting/crystallization processes are relatively
slow in comparison to the melt flow fluctuations, the changes of the front deflection
take also relatively much time and long calculations of the time dependence of the flow
are needed to bring the crystallization interface to a steady-state position1 , if started
from a bad initial guess. In Fig. 5.20, calculations with 3 different initial guesses
are considered: 40, 46 and 43 mm front deflection. It can be seen that in the first
two cases the interface showed clear tendency to move to a larger or smaller deflection,
respectively. Only for the third initial guess it stayed at the level slightly above 43 mm,
which is hence the found value of the interface deflection under the influence of melt
motion.
The picture showing the calculated zone shape and a comparison to the calculated
interface without accounting melt hydrodynamics, as well as the curve of the interface
drawn from the photo-scanning measurement is shown in Fig. 5.19.
1
Steady-state position for the crystallization interface means that the fluctuations take place
around a stable average shape. Ideal steady state, i.e., without fluctuations, is not possible if taking
into account the time-dependent melt motion.
112
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
front deflection (mm)
42.5
42.0
41.5
41.0
40.5
40.0
0
200
400
600
800
1000
1200
1400
1000
1200
1400
1000
1200
1400
time (s)
front deflection (mm)
47.0
46.5
46.0
45.5
45.0
44.5
0
200
400
600
800
time (s)
front deflection (mm)
44.5
44.0
43.5
43.0
42.5
42.0
0
200
400
600
800
time (s)
Figure 5.20: Calculation of the FZ 8 inch phase boundaries taking into account melt
flow: convergence of the deflection of the crystallization interface to a steady-state
value slightly above 43 mm.
5.3. INFLUENCE OF MELT FLOW AND ITS VERIFICATION
Parameter
Symbol
Value
HC
22.7 mm
f
3 MHz
RH
15 mm
RCr
25 mm
RF
25 mm
Single crystal pull rate
VCr
2.8 mm/min
VF
2.8 mm/min
ΩCr
6 rpm
Zone height
EM frequency
Feed rod push rate
Crystal rotation rate
113
Table 5.9: Parameters of the 2 inch process.
5.3.2
FZ 2 inch process
The second example is a 2 inch floating zone with inductor placed relatively close to
the free melt surface (Fig. 5.21). The main process parameters are listed in Table 5.9.
The measured deflection of the interface is about 7 mm , the calculation without
hydrodynamics yields, however, a much smaller deflection of 1.8 mm. Like in case of
the 8 inch example, this difference can be explained by the effect of the melt motion:
the interface deflection fluctuates due to the unstable flow around 6–7 mm, depending
on the calculation approach used (see Fig. 5.24). In the following we discuss it in more
detail.
Due to the proximity of the inductor to the free melt surface, the EM forces in the
melt create a very strong flow with a permanently changing pattern (see Fig. 5.25).
With the Reynolds number of the flow sometimes exceeding 10000, the calculation
by an axisymmetric model is not reliable, because the non-axisymmetric modes of
the flow instability are not taken into account. Since the goal of the calculation was,
however, just to demonstrate that the large difference between the thermal calculation
without HD and the measured interface deflection can be explained by the effect of
melt motion, the demands to DNS2 were relaxed and the melt flow was calculated
2
DNS stands for Direct Numerical Simulation, i.e., the direct calculation of turbulent flows by the
Navier-Stokes equations. Differently from the turbulence modelling, where the mean-flow equations
instead of the Navier-Stokes equations are solved, the DNS calculation has to be able to resolve all
the scales of motion, hence the computational cost of such a calculation is immense (some estimations
are given in ).
114
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
Calculation with HD
Feed rod
Inductor
Calculation
without HD
Melt
Crystal
Calculation with HD
Figure 5.21: Comparison of the FZ 2 inch phase boundaries calculated with hydrodynamics (thick lines) to the calculated interface without taking into account the melt
flow (thin lines).
Figure 5.22: Finite element grid in the melt as used for the calculation of the 2 inch
floating zone. Because the phase boundaries move, the grid is regenerated from time
to time during the calculation.
5.3. INFLUENCE OF MELT FLOW AND ITS VERIFICATION
115
2.8 mm
3.7 mm
HD effect = 0.8 mm
Figure 5.23: Example of the direct effect of HD on the free surface shape: due to
instantaneous strong melt flow along the free surface, its distance to the inductor
increases by up to 0.8 mm in comparison to a calculation without accounting for this
effect.
with the axisymmetric solver of FZONE on the grid shown in Fig. 5.22 by using a time
step of 2 ms.
First a calculation for 3900 seconds was done by starting from an initial guess of
crystallization interface with deflection of 7 mm (i.e., the experimental value). This
part of calculation is shown on the top graph in Fig. 5.24. It should be taken into
account when interpreting these results that, as usually in FZ calculations, the zone
height was kept constant by changing the inductor current. The targeting of the zone
height was done by using the algorithm described in Sec. 4.8.3 (with the parameter
∆min I = 1 A). The continuation of the calculations from t = 3900 s to 5600 s was
done with different approaches as shown in the middle and bottom graphs of Fig. 5.24.
So some calculations were made with keeping the inductor current constant at I =
488.9 A, which was the average value of the previous 3900 s (see the thin curves in the
graphs).
Because of the strong flow in contrast to typical 4–8 inch floating zone processes, the 2
inch example was calculated by accounting for the direct effect of the melt flow on the
shape of the free surface, which was considered in Sections 3.5 and 3.6. It was observed
that although important at the time instants with strong flow along the free surface
(see Fig. 5.23), this effect did change the average value of the interface deflection just
slightly, as seen if comparing the curves in the middle graph to those in the bottom
graph of Fig. 5.24, the latter having this effect turned off. These differences seem to
be below the numerical level of accuracy of the calculations.
116
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
9
front deflection (mm)
8
7
6
5
4
3
2
1
0
500
1000
1500
2000
2500
3000
3500
time (s)
9
I=const
front deflection (mm)
8
7
6
5
4
3
without HD
2
1
3900
4400
4900
5400
time (s)
9
front deflection (mm)
8
7
6
I=const
5
4
3
2
1
3900
without the HD effect
on the free surface
4400
4900
5400
time (s)
Figure 5.24: Calculation of the FZ 2 inch phase boundaries: fluctuation of the deflection of the crystallization interface about 7 or 6 mm with hydrodynamics (HD), and
the convergence to 1.8 mm if HD is turned off.
5.3. INFLUENCE OF MELT FLOW AND ITS VERIFICATION
(a) t = 4204 s
(b) t = 4242 s
(c) t = 4265 s
(d) t = 4304 s
(e) t = 4350 s
(f) t = 4375 s
117
Figure 5.25: Some typical stream function pictures of the very dynamical melt flow
in the calculated 2 inch floating zone. The arrows show the instantaneous moving
velocities of the solid–liquid phase boundaries. For the time instants t, cf. Fig. 5.24.
The proper result of the 2 inch floating zone study is shown in the middle graph of
Fig. 5.24: turning the hydrodynamics off lets the crystallization interface assume a flat
form very far from the measured one, while the calculation with hydrodynamics shows
fluctuations about a large value of deflection. Hence the measurement result with the
surprisingly large deflection can be explained by the convective heat transport in the
melt.
The convection effect reduced the maximum relative melt temperature from ∆T =
53 K (without HD) to ∆T = 31 K, i.e., by 22 K, which is more than in case of the
8 inch floating zone with only 13 K reduction.
118
CHAPTER 5. CALCULATION OF PHASE BOUNDARIES
11.0
front deflection (mm)
10.5
without HD
10.0
9.5
9.0
with HD
8.5
8.0
0
500
1000
1500
2000
2500
time (s)
Figure 5.26: Calculation of the FZ 4 inch phase boundaries: fluctuation of the deflection of the crystallization interface about 9.3 mm with HD, and the convergence to
10.0 mm if HD is turned off. Both values agree well with the experimental value of ca.
10 mm. Both calculations have been started from an initial guess calculated without
HD on a coarser grid.
5.3.3
FZ 4 inch process
Let us shortly mention another calculation example, a 4 inch floating zone process
with pull rate 2.8 mm/min, where the influence of the melt flow did not bring much
change in the thermal field: the convection effect reduced the maximum relative melt
temperature from ∆T = 31 K (without HD) to ∆T = 27 K, i.e., by only 4 K. The
corresponding changes of crystallization interface were negligible. As seen in Fig. 5.26,
the difference between the interface deflections calculated with and without hydrodynamics is about 0.7 mm, which can be considered being below the level of achievable
accuracy if accounting the approximations used in the calculation model, e.g., the axisymmetric approximation of the EM field of the slitted inductor, and if the calculation
is not tuned by empirical parameters. Hence in this case, both calculations show a
good agreement to the measured interface deflection, which was ca. 10 mm .
119
6
3D Melt flow and rotational striations
6.1
Introduction
The kind of axisymmetric modelling of floating zone growth like described in the
previous chapter yields, typically, a good approximation for the shape of the phase
boundaries that can be further used for the modelling of dopant incorporation or
defect distribution in the grown crystal. There are numerous works by other authors
(see Section 2.2) using the axisymmetric approximation for the dopant transport study
in the floating zone, while the question about the influence of the three-dimensional
effects even in an axisymmetric floating zone can be posed as well.
The needle-eye inductors for FZ processes are designed to stand strong electric currents
at high frequencies, which implies a high voltage between the current suppliers and a
danger of electrical breakdowns. Consequently, the needle-eye inductors are pancakeshaped and have just one turn. The EM field created by such an inductor and the
corresponding distribution of the heat sources and forces at the silicon surface are
only roughly axisymmetric. The non-symmetry influences the melt flow and generates
micro-inhomogeneities of resistivity in the grown crystal rod, which are known as
the so-called rotational striations. The unwanted rotational striations arise due to
the rotation of the crystal relative to the inductor under the conditions of disturbed
symmetry and repeat periodically in the longitudinal direction of the crystal with the
wave length being determined by the growth rate and single crystal rotation speed.
Since the rotational striations are originated by 3D effects, they cannot be calculated
within limits of a 2D model.
There are two main objectives of the present chapter: 1) to see the effects of the
non-symmetry of the inductor on the structure of the three-dimensional melt flow and
2) to examine the rotational striations. The three-dimensionality of the flow is created
in our model by the non-symmetric shape of the inductor only: we make here an
approximation by assuming that the shape of the free melt surface stays axisymmetric.
120
CHAPTER 6. 3D MELT FLOW AND ROTATIONAL STRIATIONS
In what follows, a series of publications1 where the 3D flow and the rotational striations
have been calculated numerically is included. The software used for these calculations
was the commercial computational fluid dynamics package FLUENT ([90, 91]). Unlike
the self-developed code FZONE, which calculates the flow in terms of the ψ − ω variables by the Finite Element Method (see Section 4.6), FLUENT is working with the
velocity−pressure variables on basis of the Control Volume Method (known also as
the Finite Volume Method), which is described e.g. in . A comparison between the
two approaches for a 2D flow was mentioned in Section 4.6.9. The approach used in
the own-made code FZONE was more effective in 2D computations, the present study,
however, deals primarily with 3D phenomena. Due to practical reasons, the numerical
approach in the 3D calculations is coarser and fine effects like influence of the fluid
flow on the zone shape are neglected.
6.2
Included paper 1: Effect of EM and Marangoni forces
The first of the papers is mostly devoted to the analysis of the influence of the different
forces on the melt surface. Due to the high frequency of the EM field, the EM forces
act in a thin boundary layer of the melt and, as quasi-surface forces, counteract the
surface forces created by the gradient of the temperature-dependent surface tension,
i.e., the Marangoni forces. A schematic illustration of the action of forces in a crosssection of the molten zone is shown in Fig. 3.1. The EM- and Marangoni forces have
also minor azimuthal components due to a non-axisymmetric distribution of the EM
power density and temperature along the free melt surface.
In order to distinctly see the individual impact by EM- and Marangoni forces on the
melt flow and rotational striations, studies have been carried out with neglecting either
EM forces or Marangoni forces (or both of them) while buoyancy forces stay always
accounted. Physically, the results with neglecting Marangoni force may be interpreted
as a model of a case with lower frequency of EM field of inductor (domination of EM
force) while the results with neglecting EM force, as a model with higher frequency of
the field (domination of Marangoni force).
The results of the studies have been published as included below in the article  in
the journal Magnetohydrodynamics.
1
The author of thesis acknowledges gratefully the contribution of about 10% by the coauthors of
the included publications. The text of the publications has been written by the author of thesis.
6.2. INCLUDED PAPER 1: EFFECT OF EM AND MARANGONI FORCES
+
!
"
#
\$
%
&
'
(
)
−
7
8
−
9
−
−
D
N
Y
*
R
,
-
.
/
0
1
2
3
1
4
5
6
:
;
<
=
>
?
@
A
@
B
C
E
F
G
H
I
J
K
L
M
E
O
G
P
S
T
U
V
W
X
Q
Z
[
\
]
^
_
`
a
\
b
`
c
d
e
f
g
h
i
j
h
k
l
b
i
m
\
_
h
i
`
g
c
d
n
^
`
m
i
^
k
o
p
q
q
r
s
t
u
v
w
x
y
z
{
|
}
}
~
x




x
y

t





¡
¿
À
×
ç
è
Á
Ø
é
Â
Ù
ê
Ã
Ú
ç
ë
ë
ú
Ä
×
ì
û
ü

¥
Ç

§


¨
î
«
§


¯

°
Ê
ñ
§

µ
Ì

¶


±
Í
Î


º
»
±
"

º
¾
Ð
Ò
Û
Õ
Ý
ö
!

¹
Ô
è

¦
Ù
ï

®
Ó
æ
ö

¥
Í
å

½
Ò
ñ

®
ä
õ
¥
Ñ
ã
ñ

¼
Ð
á

¹
ë

Ï
ô

¸
Ú
ó

·
Ø
ò

´
Ý
è

³
â
í

Ë
á
ð

²
Æ
à

±
Ë
Û

®
É
Ý

­
é

¬
È
ì

¤
ß
í

Á
Þ
ï

ª
È
Ø

É
Ý

¦
È
ë

£
Ü
è
ÿ

¤
Ø
ç
þ

£
Æ
×
í
ý
¢
Å
Û

í
#
\$
Ð
Ù
÷
%
(
Þ
õ
*
+
Ö
Ú
ç
)
Ð
×
ì
'
Í
Ø
ë
&
Ì
æ
à
ò
,
-
â
í
ï
ø
ì
ù
.
/
I
J
Y
I
Z
[
l
n


¬


­
Ä
®
Å
æ
ò
î
ô
ý
þ
þ
ý
!
"
ç
#
Ó
\$
£
£
´
ð
·
´
¦
½
¢
²
¤
¾
»
§
}

¤
¸
¥
¨
»
¿
¤
²
t

´

®
¤
´


®

¯
À
£
¸
²


¾
»
n
¸
~
Á
}
¡
Á
¿

¦
Â
®
¤
¼
±

²
|

¾
¯

µ
´
ª
»


¤
z



¸


«
¼
[
w

£
®
a
z

X
\
|


J
^
~

µ
J
d


¤
M
Y
z

§
H
L
k


G
J
e
w

¢
Q
`


¥
O
`
w

E
W
e
u

F
D
6
N
j
u


?
W
g

2
U
e
t


6
I
i
m

C
M
e


9
V
c
z

B
M
f
w

A
K
g
~

@
U
h
n

?
J
[
z

>
M
`
|

5
N
g
u

4
T
f
n

=
S
Z
o

<
I
a
n

2
L
\
x

¥
»
Õ
è
ì
Ö
×
é
í
ý
Ø
ö
&
Ô
ê
n

6
M
e
w

<
O
d
w


ÿ
%
u
¤
±
ý
|
2
I
d

Ô
^

4
R
¤
¹

ª
Á
¤
±
Ã
Ó
ò
ý

¼
õ
¢
Ò
{
;
Q
c
z

³
!
¡
ô
ÿ

>
Ñ
ó
ÿ
y
:
N
b

»
Ì

2
R
[
n

4
I
Z
x

º
ð
Ð
ò
´
Ï
ð
n

9
P
a
w

¹
Î
ñ
t
6
M
[


¸
Í
ÿ
¬
ð
þ
Ì
ÿ
·
ì
u


9
O
[
o


8
I
`
v

¶
ï
ÿ

Ë
î
u
7
O
^

µ
Ê
í
´
Å
è
ÿ
³
ì
ü
É
ë
ô
ê
t

6
Q
\


²
Å
é

±
È
è
ô

°
Ç
ç
s

6
P
[
r

5
O
_


¯
Æ
æ
q

4
M
^
p

3
N
Z
n

2
M
]
o

1
L
\
m

0
K
ÿ
Ú
&
(
#
÷
ÿ
ÿ
ý
ß
ý
+
-
.
ä
é
ÿ
ý
Ø
ê
þ
ã
ç
ÿ
Ú
ó
"
Ý
ø
"
â
é
þ
,
á
è
&
î
ß
ç
*
à
ë
ÿ
(
Ú
ô
Ù
ò
þ
Ø
é
Û
ï
)
Þ
é
Ý
é
(
Ú
ó
%
Ü
è
ý
'
Û
ç
þ
Ø
ó
&
Ù
÷
ß
æ
þ
&
#
ý
%
ÿ
/
è
\$
þ
ÿ
-
Ú
Ø
"
"
þ
%
ò
ý
þ
"
á
ç
ý
0
ß
î
ÿ
â
û
ý
\$
Ø
ú
"
Ü
ý
þ
ÿ
#
Û
ç
Ø
ù
ý
ã
é
ã
ò
ÿ
å
ï
å
ð
ÿ
Ô
è
ÿ
&
1
2
3
4
5
6
7
8
7
9
:
;
3
<
=
;
>
8
2
:
?
7
@
2
A
<
=
A
2
3
;
B
9
7
8
A
C
3
7
2
2
:
D
?
7
E
7
>
9
7
>
8
A
F
G
;
>
3
B
B
;
8
9
3
H
I
2
7
;
=
:
>
7
6
7
H
A
>
8
7
8
2
7
;
J
K
?
7
E
;
?
E
7
>
6
7
L
7
3
2
@
M
6
8
7
9
A
=
:
H
3
>
E
4
;
8
>
4
B
;
8
7
@
7
B
L
9
A
2
3
H
I
2
:
2
D
N
A
@
>
E
E
=
4
;
7
B
P
=
;
7
:
2
@
H
8
2
3
7
7
>
=
F
Q
E
O
?
;
2
7
7
3
=
E
;
4
M
9
8
H
D
9
;
2
;
2
7
D
2
>
B
7
8
;
;
2
3
9
9
2
;
A
:
>
>
3
?
B
D
E
L
B
A
3
;
=
@
8
9
A
9
3
H
3
7
@
2
>
3
2
7
A
7
7
;
8
B
9
=
3
;
A
H
8
;
>
>
>
?
8
6
9
=
;
M
3
@
R
;
D
E
S
;
3
3
8
2
3
;
;
;
J
B
?
3
>
K
;
8
>
9
A
8
7
3
H
E
M
2
3
:
9
6
3
2
:
7
>
D
=
?
8
7
?
7
;
E
?
T
E
;
E
<
7
M
8
R
Q
:
8
=
>
9
4
A
>
I
?
E
U
A
V
=
W
;
X
2
Y
A
Z
6
[
9
Y
3
\
=
X
]
7
Y
E
3
^
_
2
\
;
Q
`
2
a
7
Y
Q
b
8
c
9
W
;
V
D
Y
B
d
;
e
9
f
2
g
7
h
Q
i
>
i
j
;
k
8
X
6
;
`
6
d
h
7
W
B
X
B
i
;
l
9
X
H
h
;
[
>
6
m
3
B
W
X
?
]
9
W
7
a
L
V
9
W
A
]
B
\
B
Y
2
W
:
n
B
Y
?
^
A
W
6
[
;
Y
8
\
7
o
B
W
\
p
X
]
h
n
o
]
k
Y
Z
k
Y
n
^
_
]
\
k
Y
V
W
V
i
i
W
W
q
j
r
W
s
\
h
k
X
W
k
V
k
d
`
i
]
n
h
Y
^
v
_
k
s
d
t
h
W
W
V
V
Y
Y
W
w
Z
Y
^
[
l
]
]
k
h
i
X
i
h
j
W
^
X
^
h
h
u
f
^
g
t
h
i
[
i
X
V
t
h
h
X
o
]
k
k
q
d
i
h
W
Y
n
X
i
]
Y
l
X
d
k
^
d
k
^
l
W
\
\
k
k
l
W
d
\
W
p
i
k
V
k
V
\
W
h
X
u


¬
­

¯
Õ
ß
è
é
ã
ê
á
ë
ì
J
8
V
H
r
s
y



v


¨



§
u


ª


¬

§

­




¯
}
w


®
u



°
}
°



²
~
~
v
­


³
¬
}


£
§

ª

«
´

w
X
a
x
~
z

~



µ
«


t
}


¬
}
}


¶
t
y


µ
w

¯


§

r
w


ª

y


§
s

´
r

µ
u

¯
s
r


±
}
}
w
s
v

·
y
v
¤
x

v


v
u

w
}




R
~
x
}
z



v
H
v
s
~
¥


x
|
¦
¡
¤
¢
}
u

~
w
s


K
b

~
y
}


J
u

}
]
`
v
v
O
X
N
q
~


N

v
I
S
o
s
}
.
I
F
p
%
F
M
o
~
G
N
S
f

}
X
R
R

y
5
R
`
v
}


M

u


X
Ý
ÿ
E
H
Þ
å
(
K
M
Ó
Ù
I
E

Ë
þ
'

«
á
ô
T
J

Ø
Ù
4
M
h

}
h
ª
2
I


Ì
ì
S
W
v
}
z
-
m
|
ö
N
W
~

d
Ý
Ü
E


H

ç
å
O
i

s
h
Ò
Ü
ï
G
M

Ë
ã
*
F

Ñ
ð
%
m
Ð
Ù
F
E


3
m
Î
ò
J
y
v
}
y

F
^
¡
á
N
K
n
~
}

s
J
i
z
-
F
n

Õ
E
J
J
a

(
M
i

£
Ü
ê
D
I
P
n


N
w
}

C
H

Ý
ý
S


Ê
Ô
.
I
t
í
R
«
æ
Õ
(
F
f
v


ª
u

~
T
R
h
é
U
G
U
b
~
}
v


µ
I
n
v

y

§
}
~
r

P
z
u
S
ö


ã
Ü
h
f
Ï
Ø
Û
]

Ê
Õ
.

Î
l
l
¡
á
ô
G
W
Í
F
P
T
d
t
~


­
~
v

G
ï
)
E

Ù
k
k
¦
â
+
N
S
`
\
\

Ì
è
ó
I
R
F
/
T
\
m
ï
V

Ý
Ø
W

«
Ë
ß
õ
2
J
F
^
s



Z
+
S
I
G
ô

ã
j
W
¥
Ê
Ü
N
l
~
v
y
S
u


z

}

H
O
d
ð

Ù
W
]
Ö
Õ
1
M
G
X
g
v




~
~

­

x


«
v
0
G
V
ï
[
É
ã
Õ
W
X

È
Ý
]

Ü
ü
I
I
`
û
-
F
F
T
U
a
ï
^

Ç
á
W

ª
â
X
^


Æ
Ø
(
S
J
S
j
é
/
H
S
I
a

z
v

®

u
R
î
.
R
Å
[
h


è
h
X

Õ
Ö
&
E
O
T
`
~

¯
}
%
N
S
k
u
~

°
v

x
E
k
y


³
u
v


}



u
u
M
ú

Ä
Ý
]
i
§
Ã
á
ß
ù

Â
Ü
h
k
£
Á
ò
I
I
G
F
k
Q
T
V
I
d
M
I
P
U
g
s
T
P
ì

Ù
a
]

Ý
Ü
-
J
À
h
[

£
å
,
M
»
ù
\
V


Õ
ï
)
H


¿
Ý
k
Y


Ý
Û
(
I
[
I
V
`
w
r
°
F
Z
M
Û
ù
+
I
X
Ü
X
V

å
i
W
¾
à
P
h
¢
á
W

£
ä
*
d
½
â
ø
j

¨
½
÷
O
N
j
~
w

¯
Q
r
)
W



F
ó
N

ß
â
ê
(
M
W
a
}


Y
I
s
'
¼
â
ö
I
R
i
s
s
&
è
ñ
L
N
T
y

~
%
K
v

õ
K
I
e
r
}
v


S
N
h
~
s

\$
J
S

~
}

x
|


±
u
X
é
Ø

Ö
t
k
¼
Õ
ß
»
d
v

Ù
h
h


>
Ö
Ü
ô
#
F
`
ï
I
N
a
u
"
M
M
`
v
z
y
S
ó
ã
^
]


º
Ø
n
`

¨
¯
Û
^
d

£
Õ
H
F
R
\
c
w
u
v

}
x
x
}
v
w
U
S
F
ò
G
­
Ø
Õ
!
I
f
ð
F
·
Ý
F
X
g
u
v
w
x
E
a
ì

§
k
d

â
i
l
¡
°
Ù
k
k

Õ
Ù
k
\
¦
·
E
G
P
|
u
v
x
M

¥
Ý
\
W

¹
á
ñ

±
Y
^
¢
Ø
D
T

Ý
ë
X
`
{
t
u
w
V
ð
S
R
´
w
d
¥
Ý
C
E
S
e
z
s
t
v

«
w
s
t
X
d
B
F
J
E
f
r
A

à
å
ê
I
]
I
y
r
s
W
á
@
G
`



T
e
v
R
å
Ü
\
k
¤
¸
Ø
h
X

£
·
ß
ë
?
H
S
x
r

T
d
}


§
I
w
~

J
t
á
í
;
I
c
é
>
T
O
v
}
I
b
u


v
N
`
t
}
H
ë
¶
Þ
]
Y


­
Ø
]
{
Ý
h
n
¢
±
Ô
×
=
Õ
y
Y
~

²
Ü
Û
ï
S
a
s
v
R
ï
<
Ø

¡
µ
Û
i
|
°
Ö
î
;
T
R
`
:
E
S
T
_
9
G
M
î
7
ã
í
6
\
Ù
ì
Ö
´
r
k

¡
Ú
y
k


Ö
x
o

³
Ô
a
h

¯
Ù
Ø
t
~
²
Ø
`
X
}

±
×
\
[
|

°
Ö
j
t
{

®
Ô
k
^
z

]


u





121
122
CHAPTER 6. 3D MELT FLOW AND ROTATIONAL STRIATIONS
°
³
µ
³
±
·
±
±
²
³
´
²
¸
¶
¹
º
»
»
¼
½
¾
¿
È
½
À
¹
h
i
j
k
l


½
º
À
Â
Å
¼
Ã
Ä
¾
¿
Â
¹
¿
Æ
¼
¹
½
Ã

Ç

n

o



p

q

r
s


t

u

v
¡
Ã
¼
}

¼
Ã
k
m

Á
¾
q

w

x

¢
y


s
£
¤
z
q
¤
{
t
¥
¤
s
|


u

v

~






































q

¢
¦

¦



¤
¢


¤


§
¨
¤
¤
¦



¦
¦



¤





¤

¥
§


¦
ª
«
¬
­
®
¯
»
Ò
Î
Æ
¾
Å
Æ
Ç
Ä
Î
Å
¾
Ä
Ð
Æ
À
Å
Ã
¾
Ò
Ï
Î
Á
Ä
Í
Ã
ç
Û
Ç
È
Î
Ü
Ï
ì
Þ
¾
Å
ê
Ë
Ä
Ô
Ú
Ï
É
Ð
è
ã
í
Ã
Æ
À
Ç
Ç
Í
Ó
ï
Ñ
Í
À
Â
Î
À
Í
À
À
à
Î
æ
Ä
î
Ò
Á
Å
Ì
æ
Ç
À
Ð
Ä
À
Â
Õ
Å
Ï
ò
Î
Ñ
á
À
Å
Æ
Ð
Î
Ð
Á
Å
Æ
¾
é
À
Â
á
¾
Â
è
¾
Ð
Á
Ï
ç
Í
Ç
Ï
Ð
Î
ô
Ç
×
Ä
À
Æ
ó
Í
Ö
¾
Ñ
è
¾
Õ
Æ
Ù
Ì
í
Ä
Æ
à
Æ
Ä
é
Ì
Ñ
¾
À
Å
ñ
Ï
Ä
Ï
Î
å
Å
Á
Ì
Â
Ï
Ç
Å
Å
Ð
À
Ò
À
ê
¾
Ã
Ð
å
Í
¾
Î
Å
Å
ë
Ï
Ð
Ð
Á
¾
ð
Î
Ï
Å
Á
Ñ
í
Ã
Î
¾
Ä
Ç
ð
Í
Æ
Í
Æ
¾
é
¾
Ï
Ç
Ç
æ
Ç
Â
Ç
À
Í
í
À
Ì
¾
Î
¾
î
Å
Ï
Ç
Á
è
¾
Ð
Ä
Î
ê
Ä
¾
Ì
Æ
Ä
ç
Ì
Ä
Å
Ç
Ã
å
Å
Ð
ß
¾
Ñ
ã
¾
Î
Ü
Ã
Ç
æ
Ã
Ð
Ð
À
ì
Ê
Å
Ð
Æ
è
É
Í
Ý
Á
Ä
ã
À
Ã
Ã
è
Æ
Ä
Ú
À
Â
ë
Å
Ì
Ð
Ò
À
ê
Ä
Å
À
Ð
¿
é
Ã
Î
Ä
Å
é
Â
Ä
Ù
¾
Ð
è
Á
Ó
À
Æ
Ä
ç
À
¾
Ç
Å
À
æ
¿
Ì
Á
Ð
Á
å
¾
Á
Ä
Ç
ä
½
Ä
Ï
Ð
Æ
ã
¼
Ì
À
¾
À
í
À
Ç
ì
Õ
ß
å
Å
ê
¾
Ý
Ó
ê
ë
Å
Ì
Ä
í
Ì
Ð
â
Ã
ì
Ï
Å
Ó
Ð
Ä
ð
Î
Ø
Î
Ä
Ì
Î
Ï
à
Å
Æ
Ä
Õ
Ã
Ä
Í
Ã
Ä
ñ
Ã
Å
Ä
Æ
¾
ì
í
á
è
õ
ö
ê
ú
ñ
ù
ê
÷
,
ü
*
ø
û
ù
þ
ø
ú
ý
ú
û
ÿ
'
ú
ø
ü
ý
þ
ø
ý
ù
ý
ÿ
+
ü
ø
*
-
ø
û
þ
ø
ø
ú
ø
,
ù
ü
!
*
-
)
ú
"
ù
ý
#
ÿ
\$
%
&
ý
ü
ø
'
(
û
ü
)
ù
*
+
ù
.
-
)
+
7
/
"
,
+
*
'
+
*
'
'
(
*
*
*
,
2
'
*
*
*
7
*
'
*
+
,
*
*
+
*
7
(
*
*
'
2
'
*
*
*
'
'
+
*
,
)
*
-
+
5
+
"
4
*
'
*
(
0
\$
*
*
'
#
+
7
7
*
7
*
(
(
*
(
*
)
'
"
"
+
)
8
*
0
5
4
2
+
'
,
+
+
8
*
*
*
(
\$
1
7
*
3
(
(
2
(
,
*
'
'
6
#
2
0
2
'
(
+
)
'
+
'
+
*
)
*
,
,
*
(
*
'
/
'
*
,
(
2
-
7
,
+
1
*
"
*
/
-
.
2
'
2
7
*
7
"
'
*
*
+
*
2
S
Z
R
Z
a
P
b
'
>
)
?
U
b
c
Y
Z
A
_
S
'
C
D
Z
R
E
f
]
U
P
?
+
Y
Z
)
2
'
)
,
*
+
'
)
#
*
+
'
7
)
+
2
*
#
*
(
5
*
\$
'
'
*
*
,
"
#
+
,
2
&
2
%
'
5
*
+
\$
*
(
*
/
-
(
*
'
"
4
,
*
;
*
1
+
&
(
:
%
+
2
7
*
)
\$
*
*
+
'
,
(
*
*
'
)
*
*
*
9
'
*
+
*
,
'
*
+
*
*
'
(
7
(
7
'
'
*
,
'
*
2
*
*
*
7
/
+
,
'
*
7
H
Z
R
*
?
O
G
c
*
+
*
,
P
\
*
*
*
\$
*
"
*
,
*
F
\
2
2
'
+
,
)
7
B
T
'
*
"
+
*
2
V
*
*
*
+
R
R
!
(
?
Z
'
@
b
'
*
2
7
"
(
T
b
)
=
V
,
)
'
'
+
"
\
*
<
_
(
*
'
*
+
7
(
*
'
(
)
-
,
"
+
-
#
2
V
]
I
b
V
D
V
X
c
V
V
H
Z
P
C
J
K
[
]
V
[
P
Z
L
H
@
d
S
P
V
S
M
T
Z
U
U
N
O
d
V
b
c
P
R
Q
P
Q
_
P
V
Z
R
]
[
P
P
c
S
V
O
T
U
Y
P
S
b
c
f
V
O
P
S
]
P
W
P
X
f
P
P
`
P
]
R
U
b
Z
Y
P
\
g
P
Z
R
[
V
b
\
Z
R
Z
T
]
U
P
[
U
U
V
Z
^
T
T
c
_
b
`
R
Q
M
e
¸
¹
º
6.2. INCLUDED PAPER 1: EFFECT OF EM AND MARANGONI FORCES
Ì
ä
å
å
æ
ð
ä
E
f
F
g
h
}
i
~






­
¢
£
Æ
Ï
Ñ
Ò
¾
Ó
Ñ
Î
ä
ê
ë
Ð
Ô
Õ
&
ë
Ò
Î
£
¶
À
×
Ø
Ù
®
Ç
Õ
Ú

û
Þ
ß
í
ü
ì
Û
å
ý


ê
Þ
ñ
ÿ
Û
ô
þ
Ô
ò
ý

«
¬
¦
Á
Ü
Ý


Ñ
õ
Ü
ç
ú


¢
­
ï
Ð
ì
Ý
×
Û
Þ
í
Ð
ë
¬
Â
¤
þ
Ð
ö
Û
ì
ø
Ñ
ë
ý
ÿ
¤
¥
¯

É
¨
¬
¾
¯
¿

à
ñ
Õ
ê
þ
Ù
ò
Ð
ä
ý
ï
ø
­
½

À
Þ
ï
Ô
á
÷
ÿ
Ã

à
õ
ú
Ò
÷
ø
Ñ
ä
î
ý
º
Á

»


Û
î
¢
¼
½
½
Ý
ö
þ
â
Ð
Þ
ë
±
À
»
Ä
í
ø
ã
ê
ó
Á
Ë
~

¡
¾
¾
½
Â
¼
Á

}



¨

³
Ä
È


}
»
½

~
®
Ã
Ë


~
¦
v
~


e
g



»


1
d
k
}

0
V
u


7
Y
|



¡
Ì
f


<
_


¿
Ç
5
Z
~

²
4
c
j

~
¾
Â




¤
¿
¾

]
{


1
b
f


A
^


¬
:
[
i


¤
¾
È
~
~
~
£
»
Æ


4
Y
j


<
{


5
a
j




6
^
r


7
Y
j

¦
¹
Å
x
~

<
`


­
¸
Â
z


1
_



8
W
g



8
V
k


}
:
^
i


°
A
]
~

~
¦
Æ
~

¬
¾

A
Z



5
t

~

8
Y
u
~



7
\



A
w


1
[
n



C
Z
m

~
¢
¾
Y
y


®
1
X
i

}
B
W
}


¼
h


A
V
~


®
Ç



<
v



Å

~
~
1
U
t


:
L
x

¦
Æ
@
Q


¡
Ä
1
P


¬
8
w

~

=
v


?
T
i
~
·
0
G
u

ª
Ê
Û
h

¤
Â
Ô
ó
>
J

¥
É

~

ú
5
f


®
Ä


¨
0
G
g




­
Æ
Ð
Ò
Õ
Î
ô
Õ
´
»
¾
¾
»
Å
Ã
É
Ã
º
Û
Ñ
Î
â
Ö
Õ
#
ý
ï
í
ò
Ô
Õ
õ
(
%
õ
!
é
å
ï
Ñ
Ñ
Ï
Ñ
Ð
Õ
ë
ç
Ö
%
Ô
á
ò
×
ã
Ö
á
ÿ
Ò
Ð
Ð
Ï
×
Î
ì
ä
Ò
æ
Ð
õ
%
Ô
Ò
ì
'
Ò
Ö
þ
ç
ä
Í
æ
Õ
Î
æ
Í
%
Ð
ò
!
"
ñ
Ï
Ô
ÿ
å
Ó
ê
Ñ
Ò
ò
Î
Ó
î
×
Ò
ó
!
Ñ
Õ
ê
å
è
%
Ó
Ò
Ñ
Ö
þ
Ô
Î
á
Ñ
\$
ä
Ô
ü
Î
×
û
!
×
ú
"
Í
Ð
ù
Ô
Í
Ó
Ô
ø
Ò
×
÷
ã
Ð
ö
"
á
â
õ
Ï
Ô
Î
ó
\$
Õ
ë
#
Ò
ã
î
Ð
Ï
ë
á
Ö
Í
ð
á
ì
ª
Ç


Õ
ä
ù
N
r


Ý
ë
ø
S
t

Û
ç
÷
=
F
s



§
;





¥
Ð
×


Ã
Í
Ò
ñ
!

Ö
Ï
ó


Â
~
~
I
r
ï
Ó
ñ
à
Ô
ò
!
Í
ñ
¦


å
å
,
<
F
Ô
ò
ò
+
Ø
ì
*
D
g
Õ
ï
ê
;
s

¤
½
Ñ

5
Ü
ì
ñ
)
G
k
~

Í
Ï
ð

r
7
L


¾
Ï

è
å
(
:
P
j


¦
¥
h
î
&
9
Û
ï
î
I


~
Ô
Î
ï
!
Í
î
Ó
Ò
í
Ï
ì
ß


È
Þ
Ý

®
½
Þ


¢
¤
½


¥
¬
Ç
q



¤
¨
Â
~
~
¢
¾
Ð
£


}


5
N
Ô
ä
ê
!
8
p

~

®
¾
Ï

¢


7
Ú
ë
ï
R
Ù
ñ
'
6
L
o




À
Î

¡
µ
Á
Í

~
5
Q
n



m
}



~
g
4
P
ê
&
Ø
ì
ç
\$
Ñ
ð
ò
%
×
å
è
"
3
O
Ð
ï
ñ
2
N
Ö
ä
ç
!
1
Õ
í
å
M
Ô
ç
ò
\$
0
h
Ó
ê
ö
L


~

½


Ó
î
é
#
K
Ò
í
í
l
}

}
J
k

~
"
/
I
j


.
H
Ñ
ì
ê
!
G
Ð
ë
ì
-
D
ê
ð
Ï
é
å
Î
è
å
Í
ç
!
)
+
,
-
-
.
:
G
I
,
i
k
}
a
L



}











}


Á
Ö
Â
×
À
Ø
}
ó
ô
Ú
õ
×
ö
ø
ù
Ü
ó
£
¤
a


~


}






}

~



~
/
S
-
K
4
*
*
=
L
1
M
*
N
,
ý
O
-
1
,
I
h

l
3
?
R
2
G

l
1
9
H

e
(
4
=
+
N
/
5
J

-
-
V

n

o

³
p

´
Ý
j
µ
Þ

¶
¢
È
à
þ
§
Ä
§
¨
Í
Û
ü
£
Ì
â
ö
¦
Ë
Ý
ý
¤
Ê
á
÷
¦
Á
Ú
û
5
.
P

,
Q
ß
á
ÿ
q
,
N
R
r

¸
à
ÿ
j

·
à
þ
k

·
ß
ý
c
2
÷
ú
÷
Ý
ä
È

º
â
5
T
t
*
U
6
-
V
¼
O
¡
¾
å
v
½
ä
u

»
ã
>
G
2
4
P
`



a
N
?
6
O
!
-
+
/
L
:
4
U

}

~

.
/
T
}
/
;
G
@
F
P





~
O
l
:
/
G

p
9
-
?
4
X
/
:
N
g

i
A
?
U
B
C
-
L




e

D
/
S



I
6
0
2
L
/
3
U


}
~


E
4
J


~
-
:
3
O
<
8
?
M
H
}
q
j
n
i
l
8
Y
Z

l

~
h




}



~



z



}
r
}


r
h
r


h
l
}


l
d
h
~
~

p
q



~
n


}

d
h
}



}
a
l
a




i
|
o



~
g
d



n
p
h



q
a
g

j
h
~


n
l
h

}
}
}
i


g
q



j
e
l
}



p
k

}

l
{



i
q



n




n
}
}

}
g


n
p
i

}

a
d
p





a
y



o
h
k
}

~
a
l
j

`
m
a


i
d



h
z
i



k

~


å
¨
Ä
Û
û
Î
â
ù
£
É
ü
¥
Ì
ã
ø
Å
Û
¤
Ë
Û
ö
È
×
ÿ
5
S
s

¹
9
F
à
Û
ý
¥
Û
÷
Ð
Ù
.
W
6
.
N
P
6
X
7
T
2
S
,
Y
-
W
Z
[
8
\
W
¬
Ñ
è
W
U
N
R
]
Y
¢
£
·
è
y
y
¥
À
ç
x
¤
¿
æ
w
¦
Á
§
·
é
¨
º
ê
z
{
½
ì
}
«
Â
ë
|
ª
·
ê
y
ª
¿
í

º
ï

¨
Á
î

¬
Ã
î
~
¡
ï

¦
Å
ò

¹
ñ

­
Ä
ð

»
ó
­
Á
ö
£

¬
R
=
ê
¹
ó
»
ï
¡
½
ö
ò
¢
£
¤
¥
¯
ï
¦
õ
§
ô
ó
−
ª
*








«
ò

¨
ú
¦
Õ
Ö
ù
Ú
û

²
Ù
ú
l

±
Ø
ó
C
k

°
×
*
G
j

2
H
i

ø
1
h

ò
ü
E
c
Û
Ü
ü
¿
Å
Ý
0
@
g
¹
Ï
û
/
I
»
å
ó
f
Ô
æ
*
?
¾
Ä
Ý
/

½
ô
e
Ó
ò
.
G
¤
Ò
÷
-

¹
Ë
ã
þ
H
d
¢
Ñ
ñ
,
G
¶
È

¬
ê
ð
I

£
ó
+
¸
Æ
ü
c
Ð
ù
ï
b

¼
Å
û
+
a
Ð
÷
î
E

Ï
ø
*
B
`
¶
Ò

¨
Î
í
H

Í
â
)
G
»
Á
÷
=

Ì
õ
>
º
Õ
à
(
F
_

Ë
ì
'
E
^

Ö
ù
&
¶
Å
Ú
D
¹
É
Ý
ý
%
W

Ê
ø
Y
¶
Á
ì
C
¸
Ô
ë
\$
·
Ò
ô
B

É
Â
ã
#
]
¶
Á
A
N

È
@
T

ª
º
÷

¬
Ã
ó

Ç
ð
{
®
¼
õ

ª
Æ
ô

?
µ
Ä
Û
=
>
X
Ò
ê
"
=
´
Ó
Ù
!
<
³
É
Ú
Y
²
À
é
ù
R
±
Ë
Ö
;
N
°
È
×
;
U
®
À
Û
;
¯
Ê
å
:
®
Â
Ü
=
9
Ê
Ú
­
Ò
÷
5
Ñ
ç
ý
«
Ç
Ý
ª
È
æ
§
Ï
m
c
:
,
W
l
a
~



d
h



}
n
p
e




h

~

a
q


l
d


m
a



h
n

~

e
i

}
~
l
l
d




i
3
+
:
1
K
f
3
J
5
:
R
g
o



}
k
e

}


i
~

<
4
P
e
j



6
9
U
h
h


4
?
N
a
}
;
F
j
e
V
y

/
3
J
j
n
l

H
U
h
i

Q
0
2
N
n
-
N
S
e
0
U
N
g

/
/
g
r

}
T
U
h

}

e



}
¥
Â
Ý
ó




Ç
ß
ü
~


É
Þ
û
}
S
H
5
4
j
l
k

:
:
i
i
r



¡
È
Ý


a

N
P

¢
Ç
ú
¡
Ú

~




Æ
Ù
}





p




Å
Û
÷

Ä

}
a

~


Á


}
~

Â
Ù


`

l
9
9
P
h
d
8
?
J
g
d
!
1
.
I
f
g
i
~
}
}
~

Ã





e
`
m
~


~
e

Y
3
9
R
P
d
i
7
:
O
H
c
l
2
.
Q
M
b
/
/
I
N
6
-
P
[
4
:
J
K
i

}

À



O
I
1
2
x

3
/
a
h




}
~
}


a

"
5
N
`
.
_
o

4
S
_
w
-
\
^
i

3
,
M
[
v
g
~
2
+
O
]
1
3
M
u
!
/
K
S
t
1
J
N
s
0
=
X
/
1
H
G
*
ý
!
>
?
@
>
A
@
?
Q
y
z

{

}

B

"
D

U

V
@
W


C
X


F


\$
D
T

#
E
S
~

C
R
|

G
C



X
J
*
K


M
(
,
K

y


.
A
E
_


-
D
^


*
N
]


+
L
\


)
?
[


(
I
Z
z

'
H
Y


&
A
U


%

0
?
O
a



/
H
`

)
C
b

~

1
L
K
c

d

¢
0
/
3
*
4
5
6
7
(
8
)
*
8
9
4
+
8
/
.
(
:
;
8
<
0
0
*
+
)
;
=
P
b

¡
2
e
}


f



~
d
}
£
¤
g


h


£


f
c
i


j

k
¥
l
~
¦
m


§
n
z
¢
¦
o
}


~
p
q

r


¢
¨
p
s
z
r

¤
q
~
t


¨

u
z
¡
v
w

v




x
¤
~
t
¢
y
¨
n
z
o
ª




«
¬
¦
¾

±
´
¸
·
É
Ê
ª
Ë
²
³
µ
µ
·

¼
¼

³
¿

·
®
Å
¹
¼


½
³
¨
¶
°
¨
³
²
£

À
°
±
º


³
Æ
·
¢

¸
Ç
¸

µ
È
º

·
Ç
³
É
µ
Ê
¡
¹

¼
Ë

µ
É
Ì
ª
Ç
¼
«
³
É
­
±
®
²
Í
Á
Î
¯
·
Æ
¶
°
±
±
º
²
±
Ï
·
³
Ë
²
È
Ð
±
Ñ
°
±
º
Ò
Ç
°
´
¹
Ó
±
¯
Ó
²
¼
Ô
³
µ
Â
Ñ
¶
·
Ã
Õ
¸
Ñ
¹
¶
Ö
²
²
Ó
³
Ï
¹
È
°
º
º
Ñ
±
»
Ñ
º
±
Ò
¾
¶
×
·
³
È
µ
Ï
µ
¹
Ç
¼
¼
¶
Ð
Ñ
·
·
¸
Ç
Ò
¶
¼
Ä
½
Ø
¸
³
·
Ñ
³
Ö
Ö
µ
°
¹
±
¼
Ç
Ò
123
124
CHAPTER 6. 3D MELT FLOW AND ROTATIONAL STRIATIONS
Ú
Û
Ü
Ý
Þ
Þ
ß
à
Û
¶
·
¸
¹
º
Ý
Þ
ç
á
ú
ã
û
ú
â
þ
ã
à
ú
¿
Þ
Þ
ç
å
ú
é
À
ú
À
é
Þ
å
Ç
á
Ê
ã
Æ
Ü
ì
Þ
Ü
é
Ê
á
ë
É
à
å
À
Þ
ã
æ
ã
Ë
å
ç
Þ
É
Ü
Ü
å
Í
é
é
ÿ
Ë
ä
Ý
Ü
Ý
Þ
Þ
ß
ú
ú
ä
ï
Ô
Õ
Ò
å
ø
ç
Ô
Ñ
Þ
þ
è
Ö
×
ã
ç
Ø
×
ã
ß
Ï
ä
à
â
Ñ
Ù
í
Ü
ã
ë
é
ß
ü
Ü
Ü
í
è
é
è
þ
â
í
à
Þ
ã
ü
Ó
÷
å
ÿ
Ò
ë
ö
Þ
ÿ
Ñ
î
î
ç
Ð
Á
é
é
ã
û
Ë
è
ð
Ü
Î
æ
õ
É
á
ã
þ
È
è
ú
Å
ä
Ü
¿
á
á
è
¾
ã
ã
û
Í
Ü
ë
ü
È
á
à
á
Ã
ç
ë
æ
þ
È
í
ã
Þ
Å
ä
å
û
Ë
å
ç
È
ô
à
ú
É
ê
è
þ
Î
ó
ü
¾
ò
û
Ã
ñ
ú
Í
Þ
ä
ü
Ì
ë
Ý
î
Ë
Þ
Ü
ê
¿
ê
þ
É
ê
ç
È
Þ
á
Ü
À
Ý
ç
ÿ
Å
Ü
ð
ë
ú
¾
ä
ï
ÿ
Ç
è
í
Þ
Æ
Þ
Þ
í
þ
û
¾
å
ç
ä
ý
Å
ç
Þ
ã
ú
Ä
á
í
è
þ
Ã
æ
è
Þ
Â
â
ä
Û
ß
Á
å
á
ÿ
û
À
ä
å
á
ý
¾
Þ
è
½
á
ç
Ü
ü
ÿ
¼
à
ã
Þ
Ý
Ï
ß
í
Ý
Ü
¹
»
Ü
Û
é
é
þ
Þ
ä
ä
û
æ
á
Þ
í
è
ä
á
í
æ
à
ü
å
þ
ù
ÿ
ÿ
ü
û
þ
ú
ÿ
ü
ú
þ
û
ú
û
ú
ÿ
û
û
þ
ú
ú
þ
ú
+
þ
!
&
%
"
9
=
K
@
=
D
H
=
H
K
<
<
<
!
@
B
"
@
8
<
D
=
8
@
D
>
B
=
E
=
D
?
D
8
D
8
I
:
=
+
:
=
F
O
H
P
4
B
,
G
D
<
<
D
=
9
C
8
I
@
:
<
H
:
>
,
<
<
9
!
(
F
D
=
<
F
N
Q
D
A
H
A
8
%
*
%
1
F
<
F
P
>
>
=
(
.
8
P
D
A
9
=
*
8
K
<
R
"
;
<
F
3
:
@
=
@
)
&
9
=
=
<
-
(
!
G
8
)
(
,
=
=
ü
(
7
9
E
)
&
6
ú
(
*
/
%
&
1
%
)
ü
#
(
%
'
\$
D
K
!
5
=
<
%
&
/
&
+
!
:
M
A
&
+
\$
(
+
J
H
%
*
)
)
&
ú
\$
"
(
%
)
=
!
&
"
8
#
!
@
!
"
>
:
!
ú
!
!
%
"
K
(
\$
B
,
=
F
!
+
#
4
I
A
(
)
.
I
:
"
%
:
=
=
!
!
%
=
F
C
\$
>
A
+
)
H
%
H
?
ÿ
(
,
G
9
.
&
&
=
<
@
K
9
&
%
û
þ
"
#
(
<
:
<
A
,
,
#
<
)
%
F
8
F
@
%
)
ú
2
'
C
:
!
F
B
&
"
#
F
<
<
%
(
*
:
:
B
H
+
<
8
)
,
û
\$
+
#
%
þ
"
(
\$
E
@
<
=
D
@
)
ÿ
)
@
:
(
ú
þ
%
%
%
-
1
D
K
C
I
ú
+
C
=
=
<
þ
(
ü
!
+
A
,
=
@
9
+
9
ú
&
B
þ
(
<
A
@
#
#
F
@
A
"
A
0
\$
,
:
=
=
%
@
D
?
F
&
/
<
ü
þ
&
=
=
>
P
'
?
8
(
)
L
<
A
%
ú
þ
!
*
+
>
8
ü
û
&
(
=
8
þ
3
%
<
:
9
K
*
(
ú
3
(
<
!
(
<
ü
H
A
8
<
?
=
L
M
S
9
N
F
8
V
9
D
:
=
O
;
K
M
W
8
<
A
H
R
K
<
9
B
9
=
H
A
=
G
<
G
=
H
=
C
=
:
H
K
D
T
:
<
K
D
U
D
=
<
G
P
8
D
=
G
H
=
F
:
K
<
K
<
9
D
:
<
P
@
=
C
8
G
D
:
=
@
8
<
F
<
@
D
<
K
A
D
E
9
B
<
=
H
K
I
@
D
:
@
:
F
=
8
D
=
8
8
D
L
>
8
=
=
K
<
H
H
D
H
B
8
<
:
8
<
@
B
F
D
A
@
I
F
<
A
<
=
C
K
D
=
9
K
=
F
V
?
A
H
D
F
O
A
E
F
8
W
=
=
A
8
:
=
I
D
F
=
C
F
F
X
M
C
Y
B
V
K
D
<
R
O
:
F
>
H
A
F
P
<
Q
D
O
^
@
C
:
@
a
h
A
>
=
`
c
q
I
b
f
A
`
_
_
{









d

=
_
H
F
:
C
K
<
<
f
g
D
H
h
h
K
A
8
g
g
A
>
A
g
d
Q
P
:
^
b
A
D
=
e
_




¬

¬




¡



O
<
c
f
=
j
_
>
D
B
=
^
i
F
c
D
?
b
_
=
=
>
g
n
:
C
<
e
f
?
<
?
b
f
:
F
=
i
d















¬




<
8
r
A
<
f
_
=
G
C
O
h
f
9
=
=
g
h
<
9
@
b
s
I
K
B
`
f
:
=
A
l
e
8
@
@
k
^
F
=
`
d
´


¤







´


A
@
H
D
n
:
<
C
m
t
=
<
A
_
f
D
=
j
R
f
<
o
8
I
B
9
=
=
n
f
8
F
\
o
g
=
=
=
c
^
@
K
8
p
`
A
A
F
^
c
@
@
:
o
b
:
B
K
_
u
K
8
C
j
f
=
=
F
^
e
G
@
A
o
_
P
I
<
b
<
=
F
i
d
K
9
=
g
]
­

¬




¦


µ


¡














|










{


v
f
;
@
<
F
<
H
f
b
:
A
F
o
i



¬
P
[
9
R
p
8
H
i
D
<
@
^
_
H
:
L
O
g
`
<
F
g
^
=
=
<
i
^
9
>
8
g
]
M
=
A
c
_




¬
¬


«




­

¬





h
a

f
b
`
°




c







£



«

¬
¡




«

±










x



m
z

«


{




b


£

f

«






_




^






u


£
±
j
|


f

ª


c








£
°
²

d
¡

y


¨


g

¢
§

c

¦
¬

e

£

b



j
¡



f

«


|



{
¥


v


¬
°
f





£
³
h

¯




±









g
~



d
{



¬
b



y




_
{



g






f













o
|

£






o













y
z



i
{



x
{



`
|




b





`
{



d



¡



¤
¡

b


i



¬

f


­


_

£





n




g





^





¢

f








«





®

d




a




`





c





s




b



¬
j








j
{



¡
b
}




d








£


A
B
b
^
f



£







G
C
j
h






~




w
{


­
k
}

H
q
f
|


e
A
=
c
^
D
I
K
q
b
z
­
<
^
_
=
B
F
_
f
9
>
D
]
­
A
S
:
d
M
X
@
Z
D
7
M




Ù


Ú

Û
6.2. INCLUDED PAPER 1: EFFECT OF EM AND MARANGONI FORCES
p
1 68 5 K
1 72 2 K
q
1 70 9 K
1 72 1 K
1 68 5 K
4
5
6
7
8
7
9
:
;
<
:
=
>
?
@
=
:
A
B
:
C
D
−
E
F
]
_
`
a
ã
b
a
ä
å
+
B
>
6
3
<
è
3
8
<
j
x
k
l
n
j
J
m
o
j
m
m
6
C
M
q
<
J
j
q
;
P
;
Q
x
p
i
t
q
s
m
H
U
p
l
R
;
8
X
s
m
H
t
D
l
3
k
H
n
q
[
T
÷
H
ø
@
ù
3
^
k
ô
S
n
ú
#
3
9
G
M
K
û
"
<
:
g
ý
%
3
c
T
4
:
X
Q
÷
\$
(
'
;
6
H
ÿ
#
B
?
W
K
N
I
G
N
J
Y
Z
L
O
[
]
^
o
ú
'
8
V
]
ø
&
1
U
_
ÿ
"
B
;
H
h
þ
\$
4
L
f
ü
"
7
Q
d
_
÷
7
6
R
m
"
A
<
H
]
õ
:
I
g
!
9
)
?
5
;
4
ü
*
?
6
\$
C
D
'
B
1
+
,
=
4
?
B
+
D
/
:
;
.
4
>
-
6
6
D
3
0
3
,
'
<
<
?
6
\$
*
;
7
D
:
&
"
D
9
:
C
:
D
C
H
\
]
]
w
t
H
^
6
?
s
w
ö
:
v
e
K
a
?
?
Z
m
õ
;
Q
j
:
;
V
u
ó
<
2
r
P
a
?
<
Z
q
G
`
ô
;
?
Y
O
_
>
6
r
i
g
ó
:
N
f
4
6
U
t
j
K
ò
:
;
i
M
l
ñ
4
W
G
^
<
4
r
]
ð
4
V
k
L
_
=
=
K
g
6
:
j
j
3
B
7
k
<
C
T
n
h
è
;
6
S
m
a
?
G
R
o
J
ï
8
;
c
î
:
?
?
c
í
9
:
q
m
ì
8
7
3
j
u
1
O
p
ä
I
^
g
−
\
H
d
g
ë
7
6
N
n
å
6
^
_
6
:
]
a
;
B
m
h
5
=
L
o
i
ç
4
B
K
n
s
p
B
h
ê
3
8
;
h
ê
2
F
D
g
?
I
i
d
ä
1
E
1
d
é
"
?
f
c
%
;
e
ç
\$
d
_
æ
-
c
G
n
k
x
j
Y
q
y
w
w
X
z
q
^
x
x
\
w
j
V
t
```